

 Matthew Nelson
 1 years ago
 Views:
Transcription
1 FORSCHUNGSZENTRUM ROSSENDORF Institut fur Ionenstrahlphysik und Materialforschung Modeling and Computer Simulation of Ion Beam Synthesis of Nanostructures von der Fakultat Mathematik und Naturwissenschaften der Technischen Universitat Dresden genehmigte Dissertation zur Erlangung des akademischen Grades Doctor Rerum Naturalium (Dr. rer. nat.) vorgelegt von Dipl.Phys. Matthias Strobel geboren am 22. Februar 969 in Wurzburg
2 Tag der Einreichung: 3. Juni 999 Tag der Verteidigung: 3. Oktober 999 Vorsitzender der Prufungskommision: Prof. Dr. Gerhard Soff Gutachter: Prof. Dr. Wolfhard Moller Prof. Harry Bernas, PhD Prof. Dr. Sigismund Kobe Technische Universitat Dresden CNRS{CSNSM Orsay, Frankreich Technische Universitat Dresden
3 Physic ist wahrlich das eigentliche Studium des Menschen Georg Christoph Lichtenberg (Deutscher Physiker und Philosoph, 742 { 799)
4 iv
5 Contents Abbreviations ix Introduction 2 Ion beam synthesis of nanostructures 7 2. Ion implantation methods Principles of ionsolid interaction Formation of secondphase precipitates Impuritysubstrate phase diagram Homogeneous nucleation Nucleation in ion beam synthesis Growth, coarsening, and coalescence of nanoclusters Modeling and simulation approaches Atomic description Mesoscopic and continuum descriptions Kinetic 3D lattice MonteCarlo method 3 3. Basic description Energetics and jump probabilities Intrinsic properties of the model Analysis of simulation data Gauging of simulation parameters Length scale Diusion coecient, time scale, and ion ux Nearestneighbor bond strength, solubility, capillary length, and surface tension A simple approach to collisional mixing Simulation of ion implantation and annealing Applicability of the K3DLMC method and discussion General description of Ostwald ripening Characterization of Ostwald ripening and recent developments Fundamentals of the model v
6 vi CONTENTS 4.2. Evolution of a single nanocluster Evolution of an ensemble of nanoclusters Local meaneld approach to Ostwald ripening Numerical implementation Simulation of diusion and reaction controlled Ostwald ripening Nanocluster evolution during ion implantation Nanocluster formation at constant implantation conditions Nanocluster formation at varying implantation conditions On the inuence of collisional mixing Collisional mixing of a single nanocluster Nucleation, growth, and Ostwald ripening in the presence of collisional mixing Combination of K3DLMC and reactiondiusion equation methods 6. K3DLMC and reactiondiusion equation simulations of homogeneous Ostwald ripening K3DLMC simulations of homogeneous Ostwald ripening Comparison of K3DLMC and reactiondiusion equation simulations of Ostwald ripening Late stage evolution of asimplanted samples Focused ion beam synthesis of nanocluster arrays Applications of the K3DLMC method in ion beam synthesis 9 7. Impurity redistribution in a reactive ambient Experimental observations Modeling of redistribution of implanted Ge in the presence of an oxidizing atmosphere Ion beam synthesis of compound nanoclusters K3DLMC model for two types of interacting impurity atoms On core/shell nanocluster formation by sequential ion implantation Shiftedprole compound nanocluster synthesis Summary and outlook 39 A Bit encoding of MonteCarlo lattice 45 B Derivation of nanocluster source strengths 49 B. General formulation B.2 Monopole approximation B.3 Source strengths in monopole approximation List of Figures 55
7 CONTENTS vii List of Tables 59 Bibliography 6 Danksagung / Acknowledgements 79 Erklarung 8 Thesen / Major statements of the work 83
8 viii CONTENTS
9 Abbreviations An author of a (scientic) publication faces the conict of using acronyms versus writing technical or often repeated expressions always in full length. Some claim that acronyms facilitate reading while others complain about the problem memorizing them. By carefully balancing the convenience of using abbreviations versus the readability of this thesis, I nally decided to introduce the following ones which are partly standard in the physical literature: BC BCA bcc CA CBII CM CPU dpa fcc FIB GT IA IBS K3DLMC KIM lhs LSW MC MCS MD NC OR PRD RBS RDE rhs boundary condition binary collision approximation bodycentered cubic cellular automaton conventional beamline ion implantation collisional mixing central processor unit displacements per atom facecentered cubic focused ion beam GibbsThomson impurity atom ion beam synthesis kinetic threedimensional lattice MonteCarlo kinetic Ising model left hand side LifshitzSlyozovWagner MonteCarlo MonteCarlo step Molecular Dynamics nanocluster Ostwald ripening particle radius distribution Rutherford backscattering reactiondiusion equation right hand side ix
10 x CONTENTS sc SRIM TEM TRIM VG XTEM simplecubic Stopping and Range of Ions in Matter transmission electron microscopy TRansport of Ions in Matter VoorheesGlicksman crosssection TEM
11 Chapter Introduction Ever since the invention of particle accelerators energetic ions have been used to explore the physical laws of ionsolid interactions []. Besides these fundamental studies the potential of ions to modify selectively the properties of substrates has been recognized and thus found a wide area of technological applications. In modern microelectronics, for instance, current integrated circuit fabrication is based on the precise control of doping of Si wafers by implantation [2]. A further example is the hardening of steels with energetic nitrogen ions, which proceeds via the formation of nitrides close to the surface [3]. Depending mostly on the implanted uence F, ion beam modication of materials can be roughly grouped into three major ranges: For uences F. 4 cm ;2 the implanted ions are assumed to remain isolated within the substrate. Implanted into crystals these impurities may reside on regular lattice sites and thus change the electrical properties of the host material (doping range) For uences in the range 5 cm ;2. F. 6 cm ;2, in the course of implantation the deposited impurities start to exceed the solubility threshold. This causes the formation of isolated domains of a new phase [in general called nanoclusters (NCs), precipitates, quantum dots, or, if in a crystalline state, nanocrystals], which besides the mechanical may also change the optical properties of the substrate For uences F & 7 cm ;2 the second phase domains start to coalesce, which might result in the formation of a continuous buried layer of a new composition in a predened depth of the substrate. Ion beam synthesis (IBS) of nanostructures refers to items two and three of the above listing and consists usually of two independent steps. First, the implantation of a certain uence F is performed in a rather well dened parameter range, i.e. ion energy E, ion ux j, andsubstrate temperature T imp. Very often this step is followed by a thermal heat treatment because (i) radiation damage is annealed out and (ii) the thermally activated redistribution of the impurities can be tailored to a large extent. As evidenced by a vast literature, a huge variety of dierent NC/substrate systems has been achieved by IBS. For instance, the formation of Au [4, 5], Ag [6], Cu [7] or
12 2 CHAPTER. INTRODUCTION Ni [8] precipitates in silica glasses or other insulators has been reported (for a review of metallic NC formation by IBS see, e.g. Mazzoldi et al. [9]). The synthesis of elemental semiconducting NCs in neutral (chemically inert) matrices has been observed [], as well as compound nanocrystal formation in singletype implantations due to chemical reactions between impurity and substrate atoms, e.g. silicide formation for metal implantation into Si []. Additionally, in a neutral matrix compound NCs could be detected by co or sequential implantation of various atom types, e.g. IIVI, IIIV or IVIV semiconductor NCs in SiO 2 [2], Al 2 O 3 [3] orsi[4]aswell as metallic compound NCs in SiO 2 [5]. Further examples and applications of ion beams in materials science can be found in Proceedings of annual or biannual conferences in ion beam physics (for recent examples, see Refs. [6, 7]). This work concentrates on the synthesis of NCs by ion implantation, because a precise control of the formation of these essentially zerodimensional structures helps to use their unique physical properties in technological applications. Consisting of approximately to 5 single atoms, the properties of NCs are governed by a combination of eects known from atomic and solid state physics. Hence, for their description well established concepts from both of these branches of physics are used. Besides their attraction for conducting fundamental research, e.g. on quantum con nement [8, 9] or on hysteresis eects in structural phase transitions [2], the following examples should enlighten promising applications as well as the large technological potential of NCs: The nonlinear optical properties of metallic NCs embedded in insulators make them attractive for alloptical switching devices [2, 7] For opto and electroluminescence from semiconducting NCs in SiO 2 the understanding and controlling of the microstructure of the precipitates seems to be vital for a tailoring of ecient devices [22, 23] Within the challenges of miniaturization in microelectronics is the promising use of nanocrystals in nonvolatile memories [24] and even as singleelectron transistors [25]. Additional to conventional IBS, the formation of NCs can be achieved by ion beaminduced disintegration of buried (multi) layer structures due to collisional mixing eects [26, 27]. Furthermore, among others, the following preparation methods have been successfully applied to form NCs: (i) Colloidal chemistry [28] (ii) Solgel processes [29] (iii) In thin lm deposition processes specic (system and parameterdependent) growth modes favor threedimensional island formation (StranskyKrastanov regime) [3, 3]. All NC synthesis methods have their specic advantages and disadvantages and, therefore, their special elds of application. For instance, the synthesis of NCs by colloidal chemistry allows by subsequent dilution steps the study of fundamental properties of single NCs [32]. Furthermore, with this method the formation of core/shell nanocrystals has been achieved [33]. It is not within the scope of this work to discuss the details of the above mentioned synthesis methods. However, a few remarks should be made about the technological importance of IBS of NCs:
13 + The method is fully compatible with current microelectronics device fabrication, which allows for a convenient implementation of NCbased storage devices + Ion implantation can transform a system to a state far from equilibrium, e.g. very high supersaturations can be obtained (these states in the phase diagram are usually not accessible by other processes) + Specic NC distributions characteristic for high implantation uxes or high temperatures can be frozen in by rapid cooling of the system + The principles of NC formation by precipitation from a depth and timedependent supersaturated solid solution is widely independent of the ion/substrate combination + Specic isotopes of the impurity species can by selectively implanted by the use of mass lters + A proper choice of implantation parameters allows to a large extent to control the density, size, and depth distributions (which are, however, in general not independent of each other) of the synthesized NCs within the host material. These advantages are partly counterbalanced by certain disadvantages, among which the following should be mentioned: ; NC ensembles formed by IBS show a characteristic size distribution, whereas there is a need of monodisperse NCs for specic applications, which are based on sizedependent (quantum) eects ; Even by multiple implantations with cascading energies, (nearly) homogeneous spatial distributions of NCs are restricted to the rst micrometers of the substrate ; Beam line ion implantation is a technologically extensive process, and large scale implantation of high uences is a time consuming, and thus expensive, step. The formation of nanostructures by ion implantation is governed by various physical processes on multiple time and length scales, which range from basic ionsolid interactions to late stage phase separation phenomena. For a comprehensive understanding of IBS one needs a consistent description of the main stages, i.e. accumulation and supersaturation of impurities, nucleation of precipitates, their subsequent growth, and, if a postimplantation annealing is applied, Ostwald ripening (OR). Although the (homogeneous) nucleation stage of rstorder phase transitions is well understood and consistent (analytical) descriptions exist, which cover the evolution of a metastable state from nucleation of secondphase particles via their subsequent growth to coarsening (see e.g. [34][36]), the space and timedependent supersaturation inherent in highdose ion implantation imposes certain restrictions on their straightforward applicability to this process. Technological applications of IBS are based on an understanding and control of mesoscopic properties of the implanted samples, e.g. NC size and depth distributions (NC 3
14 4 CHAPTER. INTRODUCTION engineering) or characteristics of buried layers, rather than on a complete understanding and control on an atomic scale (defect engineering). This is reected by the respective modeling approaches. While in the latter case binary collision approximation (BCA) and Molecular Dynamics (MD) simulations are the method of choice to obtain detailed atomic descriptions of ion beam induced point defect generation, migration and stability of defect clusters, in IBS the redistribution of implanted impurities is of concern on quite dierent time and length scales. Here, descriptions are needed, which cover the redistribution of the impurities across the implantation prole during the complete process. As will be shown in this work, appropriate modeling approaches are MonteCarlo (MC) methods for the rst to intermediate stages governed by local kinetic processes and a thermodynamic description for the late stage of NC evolution. The motivation of this work is based on the higherthanever need for realistic modeling and accurate simulations of microstructural evolution in general and, due to their technological importance, of implantation phenomena in particular. For instance, with shrinking device dimensions in microelectronics, the design and conductance of crucial experiments in order to identify unambiguously the fundamental physical processes in charge of device performance becomes more and more complex. Therefore, any insight and predictions gained from theory or corresponding computer experiments becomes more and more important. Based on preexisting computational models used for many years in statistical physics as well as successfully applied in various areas of materials science, the task of this work was to develop and rene methods with respect to specic problems of NC formation and evolution by IBS. On an atomic scale eective particle models used in kinetic MonteCarlo simulations [37] have proven to yield accurate descriptions of critical phenomena and of microstructural evolution in phase transitions [38]. Thus, in order to obtain size and depthdistributions of ion beam synthesized NC ensembles, a kinetic threedimensional lattice MonteCarlo (K3DLMC) model has been developed. Due to its atomic nature, it is ideally suited to deal with systems being far from thermodynamic equilibrium as typical for ion implantation. On the other hand, (equilibrium) thermodynamic concepts are the method of choice for quasiequilibrium processes like OR of NCs, which is usually observed during subsequent annealing of implanted samples. Therefore, for the study of coarsening phenomena, a model is used, which is based on the numerical integration of the corresponding reactiondiusion equations [39, 4]. By combining both models, the IBS of NCs can be consistently described form the very beginning of ion implantation to the late stages of annealing. This work is organized as follows: In Chapter 2 the basic concepts of IBS are introduced and the physics of nucleation, growth, and OR of NCs discussed. Then modeling approaches to phase transitions in general and to ion beam induced phenomena in particular are shortly reviewed. The next two Chapters introduce the simulation methods used in this work in order to describe the evolution of ionbeam synthesized ensembles of precipitates: The details and intrinsic properties of the MC model are discussed in Chapter 3 followed by the description of the rateequation approach to OR in Chapter 4, where also the results of reactioncontrolled OR are presented. The next Chapter is devoted to
15 the study of NC formation during ion implantation in the cases of constant and varying implantation conditions and discusses corresponding Au + implantation experiments into SiO 2. Furthermore, modications of the NC evolution due to ballistic eects typical for irradiation are studied on the basis of an isotropic collisional mixing model. In particular, the inuence of the mixing parameters on the capillary length will be presented. Chapter 6contains examples of simulation results obtained by combining both simulation methods. Here, a detailed study of the similarities and dierences of both descriptions with respect to OR are presented. Furthermore, selforganization of ion beam synthesized NCs and specic aspects of focused ion implantation are addressed. Special applications of the MC method are discussed in Chapter 7, e.g. the redistribution of implanted impurities in the presence of an oxidizing annealing atmosphere or the extension of the model to two types of impurities in order to study the synthesis of compound NCs. Finally, a summary is given, further examples of promising applications of the MonteCarlo method are presented, and future approaches will be envisioned. It is naturally a dicult and challenging task to structure a thesis, in which (i) two conceptually dierent simulation methods are used, (ii) a good deal of theory concerning fundamental aspects of the formation and evolution of NCs is involved and should be presented, (iii) basic results of both simulation methods have to be checked with theoretical predictions and compared for similarities and dierences in their common range of applicability, and (iv) studies of the physics of real systems should be performed and comparisons to experiments should be made. Not to mention the problem of introducing the basic physical concepts beginning, for instance, with the smallest scale (here single atoms) and going bottomup to continuum descriptions as the characteristic length scales increase or to follow more the historical path and proceed vice versa. Rather than setting up Chapters dealing exclusively with one of the four points listed above, I found it more instructive to proceed on the basis of a "buildingup" strategy. By this I mean, that physical processes, concepts, or methods will be discussed upon their rst encounter appropriately within the actual context and extended later on if necessary. For instance, nucleation phenomena, theoretically introduced in Chapter 2, will play a major role in Chapters 57. A second example is the description of the K3DLMC method, which is introduced in Chapter 3 for one atomic species on the basis of thermally activated processes, and will appropriately be extended in Chapters 5and7inthe context of the ion implantation related physics to be considered there. May the rather extensive use of crossreferences help those, who would have favored a dierent ordering of the subjects! 5
16 6 CHAPTER. INTRODUCTION
17 Chapter 2 Ion beam synthesis of nanostructures Conventional IBS of nanostructures consists of the ion implantation step at low to moderate temperatures T imp which is usually followed by subsequent annealing. In this work the implanted substrate is considered as a solid host of a twophase system, namely dissolved impurity atoms (IAs, also in the following called monomers) and NCs, which either consist solely of precipitated IAs or of a chemical compound of impurities with matrix atoms (see Fig. 2.). The complex physical processes occurring during IBS can be roughly grouped into four to ve major stages [4] (see Fig. 2.2): Accumulation/Saturation: After the energetic ions have been slowed down to the average thermal energy of the substrate by nuclear and electronic interactions, they are incorporated into the host material. In a crystalline material, for instance, the IAs can be found either on substitutional or interstitial lattice sites. Depending on temperature the impurities may diuse through the surrounding matrix. Supersaturation/Nucleation: After a critical concentration has been exceeded the formation of precipitates is initiated either by thermal uctuations (homogeneous) or by heterogeneities (e.g. defects) of the substrate (inhomogeneous nucleation). precipitated IAs (NCs) implanted matrix monomer attachment/detachment dissolved IAs Figure 2.: Schematic denition of impuritysubstrate system and occurring impurity phases (dissolved monomers or precipitates). 7
18 8 CHAPTER 2. ION BEAM SYNTHESIS OF NANOSTRUCTURES implantation annealing sputtering substrate supersaturation nucleation growth Ostwald ripening coalescence mon. conc. nucleation threshold Figure 2.2: Scheme of major physical stages encountered in IBS of precipitates or buried layers for a system, where swelling due to secondphase formation exceeds sputtering. Note, that coalescence can also occur during implantation. In the bottom the corresponding evolution of the monomer concentration is shown. Growth: As long as the local monomer concentration around the nucleated NCs is above their equilibrium monomer concentration, all NCs grow at the expense of the surrounding reservoir of dissolved IAs. Ostwald ripening: After implantation, during annealing the monomer concentration decreases further, and in a competitive coarsening process large NCs grow at the expense of small ones which may nally dissolve. Coalescence: Neighboring NCs touch each other and merge to one (in solidsolid systems this stage is usually only met in very highdose implantations aimed at the formation of buried continuous layers). This scheme is, of course, to some degree articial, because sharp boundaries between successive stages can in general not be dened (see, e.g. the review of Wagner and Kampmann [34] on nucleation and phase transition phenomena). For instance, in very highdose implantations nucleation may be replaced by spinodal decomposition. Moreover, coalescence may set in already during implantation replacing OR as driving mechanism of impurity redistribution. Furthermore, the onset of individual processes depends in general on the ionsubstrate system as well as the implantation parameters. In principle, OR, i.e. the surface tensiondriven diusional mass transport form small to large NCs, is also present during implantation, but at this stage of IBS it can be regarded as a process of second order. time
19 2.. ION IMPLANTATION METHODS 9 2. Ion implantation methods A primarily used method for ion implantation is conventional beamline ion implantation (CBII). Here, ions are extracted from an ion source by an applied potential and focused into a beam which enters a mass analyzer, where one specic isotope is selected. The monoenergetic beam is then refocused by electromagnetic lenses and can be accelerated for a second time to reach a specic energy. Accordingly, for low energy purposes, e.g. implantation into ultrathin gate oxides, the last step can also be used to decelerate the ions. In the process chamber the beam is then scanned across the target (lineofsight process), which usually provides laterally homogeneous implants (heterogeneities. %). With conventional implanters NCs have been synthesized using ion energies from about kev [42] to several MeV [43]. A special version of CBII is the explicit use of the focused ion beam (FIB) for inhomogeneous patterning, e.g. the implantation of certain areas in maskless processes. Depending on the properties of the focus, the synthesis of quantum wires and quantum dots can be achieved. In this context an interesting application is the synthesis of periodic arrays of nanocrystals (see Section 6.3), where rst attempts have been made [44]. In CBII highpurity monoenergetic implants are achieved on the expense of long implantation times. An interesting alternative method is plasma immersion ion implantation suited for highux and large (also nonplanar) area implantations which do not have to meet such stringent requirements (see e.g. [45]). In this technique a plasma containing the implantation species is generated in the process chamber. Applying a negative high voltage pulse to the target, positive ions are accelerated out of the plasma and impinge onto the target. Since the plasma boundary follows the contour of the (smooth) substrate surface, this nonlineofsight method can be used for specimens with rather complicated topologies. 2.2 Principles of ionsolid interaction Since materials modications by energetic ion beams are based on irradiationinduced microstructural changes and/or the chemical nature of the deposited atoms much eort hasbeendevoted to understand fundamental ionsolid interactions []. Besides a particular interest in the basic mechanisms of damage creation as well as damage accumulation, a precise knowledge of the nal distribution of implanted impurities is mandatory for IBS of nanostructures. Energetic ions impinging onto a substrate successively lose their kinetic energy by complex interactions with the bulk atoms. On its stochastic track a penetrating ion is slowed down by elastic (nuclear collisions) and inelastic (electronic excitations, ionization,...) interactions (neglecting here nuclear reactions). Therefore, the energy loss per unit length (stopping power), which itself depends on energy, can be @x el = ; [S nuc (E)+S el (E)] = ;S(E) (2.)
20 CHAPTER 2. ION BEAM SYNTHESIS OF NANOSTRUCTURES where denotes the number density of atoms in the sample. For a given ion species both the nuclear S nuc and electronic S el stopping crosssections depend on the substrate and are usually assumed not to be correlated. Knowing precisely S nuc (E) and S el (E) would allow to predict the dependence of defect production in the substrate on the implantation parameters. Nuclear stopping power Within a ballistic model the nuclear energy loss is described by a sequence of independent binary collisions (binary collision approximation (BCA) []), by which energy is transferred to substrate atoms. The probability of such a collision is determined by the scattering crosssection d(e V ), where E is the energy of the projectile prior to the collision and V the interatomic potential. The nuclear stopping crosssection is then dened as S nuc (E) = Z Tmax T d: (2.2) The energy T transferred by a collision is given by (in the following, subscripts and 2 refer to the incident and resting particle, respectively) T = 4M M 2 (M + M 2 ) 2 E sin T max = T ( = ) (2.3) 2 where E is the incident energy and the scattering angle in the centerofmass frame. Due to this kinematic, in headon collisions ( = ) of two atoms of equal mass the complete kinetic energy can be transferred to a substrate atom. After the kinetic energy of the ion has fallen below a few tens of ev, which is a rough measure for the energy needed to displace a substrate atom, its excess energy with respect to the surrounding matrix is transferred into phonons, which gives rise to an intense local heating. Any attempts to understand the basic physical processes during ion implantation are based on a reliable description of the interaction potential. Even if the complex ionsolid interactions are decomposed into independent binary collisions, still an interatomic potential has to be found for a (N + N 2 +2)body problem, since the two nuclei and the corresponding electrons interact via Coulomb forces. Assuming that the interatomic potential is only a function of the distance R = j~r ;~r 2 j of the interacting particles, there has been much eort to generalize V (R) toan universal form, which is not depending on specic electronic congurations []. For this purpose the eective interaction is described with the help of a screening length a(z Z 2 ), which includes the essential parts of the Zdependences. Usually one assumes V (R) = Z Z 2 e 2 4 R R a (2.4) with an appropriately chosen screening function. With respect to experimental data the best choice is the universal potential based on the universal screening length a u =
21 2.2. PRINCIPLES OF IONSOLID INTERACTION :8854a =(Z :23 +Z :23 2 ), where a is the Bohr radius [46]. This potential has been the basis for binary collision codes like TRIM (SRIM) [47], which are frequently used to compute implantation proles. Electronic stopping power For high energies (MeVGeV regime) the electronic stopping crosssection S el (E) exceeds S nuc (E) and is reasonably described by the relativistic BetheBloch formulation []. For low energies, S el (E) is roughly proportional to the ion velocity in the regime v Z 2=3 e 2 =(4 ~). The intermediate regime is usually bridged by interpolation formulas. Whereas an accurate knowledge of the nuclear and electronic stopping powers are mandatory for a detailed understanding of ionsolid interactions, in IBS of nanostructures they are basically only considered in order to derive depth proles of implanted IAs. Implantation proles If the stopping powers are known, the R penetration length l of an ion can be calculated by integrating the energy loss, i.e. l = E [(de)=(dx)]; de. However, one is usually more interested in the average lateral and vertical distributions of the implanted species. In CBII of large plane areas, the lateral straggling is smeared out and the resulting depth prole (the number of IAs deposited in the interval between z and z +dz) is reasonably approximated by a Gaussian distribution F N(z) = p exp ; (z ; R p) 2 2Rp 2(R p ) 2 : (2.5) Here, F denotes the implanted uence, R p the projected range and R p is the width of the prole due to straggling. The radial straggling R r becomes important in FIB experiments [48] if the beam size is of the order of R r or smaller. Furthermore, radial straggling has to be considered if a FIB is used for lateral patterning (see e.g. [49]) and for implantation in nonplanar substrates [5], where it gives rise to lateral concentration variations. Irradiation damage The nuclear stopping of energetic ions creates collision cascades, in which a fraction of target atoms are set in motion. If the energy transferred to a target atom exceeds a critical value, i.e. the displacement threshold energy E d, it will not return to its original site prior to the collision. In this case, a stable Frenkel (i.e. vacancyinterstitial) pair is created. Depending on its energy the recoiling atom, in turn, can then displace further substrate atoms adding to the irradiation damage. The number of stable Frenkel pairs (E) produced by an energetic ion of energy E has been rst approximated by Kinchin and Pease [5]: (E) = E=(2E d ). This
22 2 CHAPTER 2. ION BEAM SYNTHESIS OF NANOSTRUCTURES expression was later modied by Sigmund [52] to (E) = (E E d)e n 2E d (2.6) where E n denotes the fraction of the ion's energy lost in nuclear collisions. The numerical factor (E E d )varies with energy and reads =:8 for E 2:5E d (see also [53]). For low substrate temperatures the defects are essentially immobile. Thus in the course of implantation the damage accumulates, which in the case of crystalline targets can cause their amorphization. At elevated temperatures point defects become mobile and start to recombine, thus, depending on the ratio of irradiation to recombination, a certain damage state will not be exceeded. 2.3 Formation of secondphase precipitates The formation of nanocrystals from a supersaturated solid solution of IAs can be described within the framework of a rstorder phase transition. For this purpose for simplicity the IAs are regarded as eective particles interacting with each other within a neutral matrix. The resulting evolution of the system can be understood with respect to the corresponding phase diagram Impuritysubstrate phase diagram The phase diagram of Fig. 2.3a qualitatively describes the impuritysubstrate system. At a given temperature T for low impurity concentrations c the physically stable state consists of dissolved monomers. If the concentration exceeds the corresponding value c () coex(t ), 2 the system is in a metastable state and tends to decay via nucleation and growth to impurity NCs embedded in the substrate. In cases, where the systems is quenched into the spinodal region of the phase diagram [here, the (classical) spinodal is dened as the curve, where the second derivativeofthegibbs free energy G with respect to the concentration of impurities vanishes [55], 2 2 = ], the phase transition proceeds via spinodal decomposition (for reviews see, for instance, Langer [56] and Binder [57]). In thermal equilibrium, the onephase region is homogeneous, whereas the twophase region is inhomogeneous. In the last case, according to the lever rule (see e.g. [54]), for a given point (c T ) in phase space a fraction [c;c () coex(t )]=[c (2) coex(t );c () coex(t )] is in precipitated domains of concentration c (2) coex(t ). The remaining fraction [c (2) coex(t );c]=[c (2) coex(t );c () coex(t )] has composition c () coex(t ). In Fig. 2.3b various process paths occurring in IBS of nanostructures are shown. In the general case (path ), as implantation proceeds the (depthdependent) concentration of impurity monomers increases, and the system gradually transforms from a stable to a metastable state and starts to decay via nucleation and growth of secondphase precipitates. However, several dierent scenarios are possible: (i) if the implantation temperature 2 Superscript () denotes here the phase of dissolved impurities, whereas superscript (2) denotes the clustered phase.
23 2.3. FORMATION OF SECONDPHASE PRECIPITATES 3 a) T c b) T c 2 4 temperature 2 ms 3 us ms temperature ms 3 3b 3a us ms composition composition Figure 2.3: Schematic drawing of the phase diagram (see e.g. [54]). For temperatures larger than T c no phase transition from disorder to an ordered state is observed. The solid line denotes the two branches of the coexistence curve and the dashed line is the spinodal. The metastable (ms) part is located between the coexistence curve and the spinodal, whereas the unstable (us) part is conned by the spinodal. In a) the points 3 refer to stable, metastable and unstable states of the system. In b) arrows 3 denote process paths during ion implantation, whereas arrow 4 indicates a quench from innite temperature. is too high and/or the ion uence too low 3 (path 2), no NCs will form (ii) if the implantation temperature is very low and the uence high enough (path 3), the system could be transformed into the unstable part of the phasediagram. Depending on the temperature of a subsequent annealing step, the resulting phase transition would then occur either via spinodal decomposition or via nucleation and growth. The chemical potential per IA = k B T ln c + ' serves as an useful quantity todescribe the state of the system, where the thermodynamic potential ' does not depend on the monomer concentration c [54]. The location of the phase transition (coexistence curve) is characterized by the critical chemical potential c = (c () coex(t )). Homogeneous nucleation caused by thermal uctuations starts, if the supersaturation expressed by := (; c ) > is maintained on the order of the time scale of the inverse nucleation rate [I()] ; Homogeneous nucleation The basics of the nucleation behavior of nanocrystals formed by IBS can be understood in terms of the classical kinetic nucleation theory developed by Volmer and Weber for equilibrium [58] and Becker and Doring for steadystate conditions [59]. Applied to supersaturated gases of undercooled liquids and glasses this theory can successfully describe several features of observed nucleation phenomena. 3 Atypical example is doping of Si via lowuence implantation in electronic device technology.
24 4 CHAPTER 2. ION BEAM SYNTHESIS OF NANOSTRUCTURES In general, the nucleation rate can be written as I = A exp f;wg ==(k B T ) (2.7) where W is the thermodynamical nucleation barrier and A a dynamical factor which describes the rate of nucleation. The following overview relating W min and A to physical quantities encountered in IBS is based mainly on reviews of various experimental and theoretical aspects of homogeneous (with a few excursions to inhomogeneous) nucleation phenomena given by Langer [56], Kelton [6], Gunton et al. [6], Binder [62], Wu [63], and recently Spinella et al. [64]. For simplicity only spherical isotropic NCs with sharp interfaces are considered and any inuence of strain elds is neglected. Assuming a nite mobility (either during implantation or during a subsequent heat treatment) diusing IAs can interact and thus form tiny agglomerations, e.g. dimers, trimers,.... According to thermodynamic principles the equilibrium size distribution U per unit volume for clusters consisting of i IAs formed by thermal uctuations is given by U eq (i>) = U() exp f;w min (i)g U() = c: (2.8) Here, W min (i) denotes the minimum reversible energy needed in order to form a cluster of size i and c is the impurity monomer concentration. The transition from a solid solution to precipitates involves the formation of an energetically unfavorable phase boundary, thus the corresponding change of the Gibbs free energy per IA G can be written as [56] G(i) =;()i + i 2=3 : (2.9) In the last equation the rst term denotes the bulk and the second the interface contribution which is proportional to the surface tension [i.e. = (36Va 2 ) =3, where V a is the atomic volume]. In the standard framework of classical nucleation theory, the surface contribution is assumed to be independent of size, i.e. 6= (i) (for a discussion of modications due to a sizedependent surface tension see [65]). The underlying capillarity approximation of Eq. (2.9) is, of course, only applicable for reasonably large clusters which possess clearly distinct bulk and surface energy states. Fig. 2.4 shows typical examples of the dependence of G on the cluster size. It is obvious that as long as <, all clusters are unstable. However, for > there exists a critical size i? associated with a maximum of G 3 W min =G(i? )= () 2 for i? = (2.) 3 which denotes the nucleation barrier (see Fig. 2.4). According to classical nucleation theory the higher the supersaturation the lower is the corresponding critical cluster size. 4 In general clusters with i >i? can lower their free energy per atom by attachment of further monomers, whereas ones with i<i? prefer detachment of monomers. 4 Note, that close to the spinodal W min k B T, and spinodal composition itself is characterized by the absence of any nucleation barrier [57].
25 free energy 2.3. FORMATION OF SECONDPHASE PRECIPITATES 5 i? 2 i? < 2 size Figure 2.4: For three dierent cases ( <, < 3 < 2 ) the dependence of the Gibbs free energy G on the size i of a precipitate is plotted according to Eq. (2.9). In the absence of supersaturation, i.e. <, precipitates of any size are unstable. For metastable systems, i.e. >, the nucleation barrier depends on the degree of supersaturation (here i? 2 3 denotes the corresponding cluster size). In order to obtain the rate of nucleation I concepts from nonequilibrium statistical mechanics have to be applied. For this purpose it is assumed that NCs grow or shrink only by bimolecular steps, i.e. evaporation or condensation of one monomer at a time. This implies, that coalescence of NCs can be neglected which is a reasonable assumption for nucleation in a condensed matter system, because the cluster diusivity rapidly decreases as a function of size. The derivation of the nucleation rate is usually done in the steadystate regime, where one assumes, that supercritical NCs of size i > i? are removed and the i monomers are brought back into solution such as to keep constant. Within this approach, which ignores depletion eects, the steadystate nucleation rate is independent of time and cluster size, i.e. I s 6= I(i t) Let I(i) be dened as the rate at which NCs of size (i ; ) are transformed to size i, then the NC distribution U in size space is given = I(i) ; I(i +): (2.) The nucleation rate can be expressed as I(i) =k + (i ; )U(i ; t) ; k ; (i)u(i t) (2.2) where the coecients k + (i) and k ; (i) denote the rate of attachment and detachment, respectively, of one monomer with respect to a NC of size i. The dierence between the VolmerWeber [58] and BeckerDoring [59] approaches is the use of the equilibrium U e or steadystate U s size distributions, respectively.
26 6 CHAPTER 2. ION BEAM SYNTHESIS OF NANOSTRUCTURES By applying the principle of detailed balance (which is strictly valid only for equilibrium conditions) the kinetic coecients can be related k + (i ; ) k ; (i) = U eq(i) U eq (i ; ) = exp f;[g(i) ; G(i ; )]g : (2.3) From this it can be shown, that the dynamics of the system can be expressed in terms of a FokkerPlanck t) k t) U(i t)+ Eq. (2.4) can be interpreted as the diusion equation for NCs in onedimensional NC size space [62] with a sizedependent "diusion coecient" [k + (i)] and a term accounting for a "drift" [k + The details of the kinetics of this stochastic process in size space are determined by k + (i). On the basis of physically reasonable approximations of Eq. (2.4), e.g. saddlepoint integration [56], the steadystate nucleation rate is given by I s = U()k + (i? )Z exp f;g(i? )g (2.5) where the Zeldovich factor Z [66] accounts for the fact, that not all precipitates which reach size i? actually continue to grow. For a complete description of homogeneous nucleation it remains to determine the kinetic coecient k + (i? ) for special systems. Nucleation in condensed systems For nucleation within a condensed system the forward and backward rate constants can be calculated assuming that the system passes through an activated complex [67] k + (i) = 4i 2=3 expf;g(i)=2g (2.6) k ; (i) = 4(i ; ) 2=3 expfg(i)=2g: (2.7) Here, g(i) = G(i + ); G(i) and is the atomic jump frequency at the nanocrystal interface. If is assumed to be equal to the jump frequency of bulk diusion, then the relation = 6D= 2, where is the atomic jump distance, can be used to rewrite the steadystate nucleation rate [6] I s = U() 24Di?2=3 2 Z exp f;g(i? )g : (2.8) Thus I s is explicitly proportional to the monomer concentration c = U(), but nonlinearities arise due to the additional dependence of the critical NC size i? [Eq. (2.)] on the supersaturation (and thus on c). Furthermore, the steadystate nucleation rate is characterized by the total thermodynamic energy barrier given by the sum E A +G(i? ), where E A is the activation energy for diusion. Thus it is obvious form Eq. (2.8), that although
27 2.3. FORMATION OF SECONDPHASE PRECIPITATES 7 a system can be in a highly supersaturated state, there might benonucleation, if thermal uctuations are too weak to make atoms mobile. In cases, where there is a lattice mismatch between the precipitated phase and the surrounding matrix or where elemental nanocrystals are formed, nucleation depends on the associated elastic potential. This can be described by adding a volumedependent term to the change in G [Eq. (2.9)]. Furthermore, the NC growth rate is modied in a sense that monomer diusion in the strained vicinity ofa NC is inuenced Nucleation in IBS Before discussing the applicability of classical homogeneous nucleation theory to NC formation in IBS, some additional aspects of nucleation should be mentioned briey. Inhomogeneous nucleation While homogeneous nucleation is completely due to thermal uctuations of the metastable system heterogeneities within the system can catalyze the phase transition. For nucleation within a condensed system, such catalytic sites can be grain boundaries, impurities, or defect complexes like dislocations or vacancy clusters [68]. In such an environment, the eective nucleation rate can dier substantially form the homogeneous one [Eq. (2.8)] and can be written as I i = A i exp f;w i g : (2.9) Usually, the relation W i < W can be assumed which is due to an eectively lower interface energy contribution to the nucleation barrier. Since the dependence of I i on W i is exponentially, a reduction of the energy barrier can greatly enhance the nucleation rate. Timedependent nucleation Classical nucleation theory is often applied to systems which are rapidly quenched from the stable to the metastable state, e.g. the expansion of a cloud chamber. It is obvious that nucleation does not start instantaneously, rather, after a time lag (an incubation period), a transient nucleation rate is observed, which asymptotically tends to the steadystate value provided that depletion eects can be neglected. According to various analytical treatments within the classical nucleation theory, i.e. for = const >, the transient regime can be approximated by I(i? t)=i s ( ; expf;t= t g) t = =(k + (i? )Z 2 ) (2.2) where Z denotes the Zeldovich factor and the numerical constant depends on the particular derivation (see [69, 6] and further references therein). The transient time t decreases with increasing temperature as well as with increasing supersaturation. In general, also depletion eects have to be taken into account during the nucleation stage, which, in turn, inuence the nucleation rate. This can be done by considering the
28 8 CHAPTER 2. ION BEAM SYNTHESIS OF NANOSTRUCTURES normalized volume v(t), which is available for the formation of supercritical clusters [7]. However, while for solidtosolid phase transitions v(t) is simply given by ; v (t), where v = is the volume fraction of the (nucleated) new phase, in IBS nucleation is restricted to the volume fraction characterized by >. Depending on the size of the depletion zone (i.e. the volume for which < holds) around each NC, which is no longer available for nucleation, v can considerably exceed. During implantation, v is a function of the ratio of the deposition to the diusion rate. Discussion of nucleation in IBS In highdose ion implantation nucleation of NCs can be encountered at two quite dierent stages of the process. The phase transition occurs either during implantation and/or during a postimplantation heat treatment. For a given ionsubstrate system the primary nucleation stage can roughly be classied with respect to the diusion length L Di = p 2Dt of impurity monomers during implantation, where the implantation time t for a nominal uence F and an ion ux j is given by t = F =j. Furthermore, the local accumulation of impurities is a function of the ratio j=d. The comparison of L Di with R, ~ which is the radius of a hypothetical sphere dened by 4=3 R ~ 3 c(f ). i? (c(f ) denotes the averaged local concentration after a uence F has been implanted), and R p allows the following phenomenological categorization: (i) L Di < ~ R: This condition states that thermal uctuations do not initiate precipitation. For instance, this situation is assumed to be encountered for Ge implantation into SiO 2 at or below room temperature [7]. 5 (ii) L Di R p > ~ R: Nucleation starts during implantation, when the monomer concentration exceeds the nucleation threshold ( > ). Due to the implantation prole the rst stable precipitates appear close to R p. Since the concentration increase is proportional to the implantation prole, a larger supersaturation is reached in the center of the prole than in the tails. Accordingly, the critical NC size is supposed to increase from the center to the tails. In the course of implantation, the nucleation region spreads outside, whereas behind the nucleation front the growth stage sets in. In this case NCs are formed essentially across the whole deposition range with a density roughly proportional to the impurity prole. (iii) L Di R p > ~ R: NCs formation starts close to R p, where the highest concentration of IAs is achieved. Due to the high mobility of the impurities, during the ongoing implantation those deposited in the tails of the distribution either diuse away from the implantation region or diuse into the center, where the already formed NCs act as sinks. The resulting monomer uxes prevent a spreading of the nucleation region across the prole, because in the tails the critical monomer concentration will not be exceeded. Therefore, the nucleation region is restricted close to R p. 5 If tiny NCs have been formed during implantation they are below the TEM detection limit.
29 2.3. FORMATION OF SECONDPHASE PRECIPITATES 9 Implantation modes (ii) and (iii) are usually met for metal implantation into insulators. However, classical nucleation theory as described above is based on several assumptions which can not be expected to be met in IBS of nanocrystals: Due to the depthdependence of the implantation prole [Eq. (2.5)], there are spatial inhomogeneities in the layer of phase transition, i.e. = (~r ). In contrast to a homogeneous supersaturation background the modication of the nucleation behavior in presence of concentration gradients is not clear. Since a certain uence is implanted, depletion eects have to be considered, at least at the end of the nucleation stage, i.e. (~r )=(~r t). In case (iii) additionally the evolution of the supersaturation in the course of implantation inuences the phase transition. Thus it is not clear, if the steadystate nucleation rate I s is reached at all. Furthermore, in the case of precipitation during implantation collisional mixing modies the nucleation rate by enhancing the rate of dissolution of a NC which can be written as [64] I CM (i) =k + (i ; )U(i ; t) ; [k ; (i)+k CM (i)]u(i t): (2.2) As a consequence, for a given implantation temperature the critical NC size shifts to a higher value, i.e. i? CM >i?. However, assuming a xed ion ux, i? CM decreases to i? for increasing temperature [64]. Note, that this is in line with the model of Martin [72], according to which the eect of an ion ux can be cast to some extent into an eective higher temperature T e = T +T CM. Classical nucleation theory assumes isotropic spherical precipitates, whereas NCs may be crystalline having an anisotropic faceted shape. Thus, not all surface positions are equivalent with respect to attachment and detachment of monomers, which, in turn, modies the kinetic growth parameters k + and k ; [69]. The distribution of damage in the substrate caused by ion implantation is depthdependent. Thus, if heterogeneous nucleation has a major inuence, the nal NC distribution should be correlated to the damage prole. It is obvious from this listing that for IBS the eective supersaturation (~r t) is dicult to compute, and hence the number of nucleated NCs, given by N NC = ZZ I(~r t)d 3 rdt (2.22) can hardly be predicted analytically.
30 2 CHAPTER 2. ION BEAM SYNTHESIS OF NANOSTRUCTURES a) c b) monomer concentration c GT 2R x monomer concentration c c GT 2R x Figure 2.5: Schematic drawing of the monomer concentration eld of a single NC of radius R in one dimension. The NC grows (a), if the surrounding average concentration c is larger than its own equilibrium concentration. In the opposite case (b), it shrinks. 2.4 Growth, coarsening, and coalescence of nanoclusters A single isolated secondphase precipitate interacts with the initial phase by monomer exchange via the common phase boundary. In general this interface is curved and the explicit monomer attachment and detachment rates depend on this curvature. Accordingly, the equilibrium concentration in a volume V above a surface segment A is also a function of the local curvature (for simplicity the following discussion is restricted to the diusion controlled case a more general discussion will be presented in Chapter 4). For a spherical isotropic NC of radius R this relation is given in a thermodynamic description by the GibbsThomson (GT) relation [73] c GT (R) =c exp Rc R c =2V a : (2.23) R Here, c denotes the impurity equilibrium concentration at a at (R!) phase boundary (i.e. the solidus), and the capillary length R c is given by the material parameters surface tension and the atomic volume V a. If the average surrounding concentration c is larger than c GT, this NC acts as a sink for monomers and will grow (see Fig. 2.5a). In the opposite case, i.e. c < c GT, it behaves like a monomer source and will shrink (see Fig. 2.5b). Although the evolution of diusionally interacting NCs is a complex manybody process, a good basic understanding can be achieved by studying the behavior of a single precipitate in a meaneld approach. Restricting this description furthermore to the adiabatic limit, which implies that the growth rate of a NC is slow compared to the resulting adjustment of the concentration prole of IAs, the stationary diusion equation has to be solved. In the presence of a constant positionindependent volume source term G 6= G(~r t) of monomers, which approximates the eect of impurity deposition due to the ion beam, one obtains for
31 2.4. GROWTH, COARSENING, AND COALESCENCE OF NANOCLUSTERS 2 a spherical isotropic precipitate of radius R at site r 2 r c(r) =; ~ G G D : (2.24) For the dierent stages encountered during IBS a solution of the last equation has to be sought with respect to the boundary conditions (BCs) c(~r )j j~r;~r j=r =^c and either one of the two following (2.25) lim c(~r )=c u =: (2.27) j~r;~r j=s>r Usually, one assumes (i) that the monomer concentration at the curved phase boundary is given by the GT relation [Eq. (2.23)], i.e. ^c = c GT, and (ii) that the monomer concentration at innite distance can be identied with the average concentration, i.e. c u =c. Growth stage The NC growth stage is encountered during implantation when nucleation has ceased, i.e. after the monomer concentration has fallen below the eective nucleation threshold. Due to the continuous impurity deposition, the monomer concentration may stay above the equilibrium values of all supercritical NCs, i.e. c > c GT (R min ) of the smallest stable precipitate. In this case OR due to the inevitable size dispersion is only a second order process since the concentration eld eectively screens competitive coarsening (see Fig. 2.6a). The growth law of a single NC is then related to the available volume for which it acts exclusively as a sink for diusing monomers. If n denotes the NC density after the nucleation stage, then this monomer reservoir is of the order s 3 n ;. To proceed further it is assumed, that there is no monomer ux [see BC Eq. (2.27)] between adjacent cells containing one precipitate ("mun tin" conguration). Neglecting collisional mixing [i.e. ballistic eects of ion irradiation which would add an additional source term on the rhs of Eq. (2.24)], the concentration eld is given by G c(r) =^c + ~ ; R 3 +2s 3 Gr ; ~ 2 6R 6 ; Gs ~ 3 for R r s: (2.28) 3r By evaluating the monomer ux through the NC surface the growth law reads dr dt = V ag ; s 3 3R 2 ; R 3 : (2.29) The last equation simply states, that the rate of growth is proportional to the available volume of monomer deposition. In the case s 3 R 3, one obtains a constantvolume growth rate dv NC =dt. It should be noted, that Eq. (2.29) is not explicitly temperature dependent. Rather, the temperature enters indirectly via the value of s, because the density of NCs is determined in the (temperaturedependent) nucleation stage.
32 22 CHAPTER 2. ION BEAM SYNTHESIS OF NANOSTRUCTURES a) b) c monomer concentration monomer concentration c x x Figure 2.6: Scheme of the monomer concentration in an onedimensional ensemble of NCs. In (a) all NCs grow, because the average concentration c fed by continuous monomer deposition is larger than the corresponding equilibrium concentrations. In (b) the situation for OR is shown. Here, the NC equilibrium concentrations are such, that the two largest grow while the three smaller NCs shrink. Coarsening stage After implantation, the monomer concentration rapidly decreases and its local value is determined by the surrounding NCs rather than by feeding through the ion beam. Now, c GT of the smallest NCs will be above the average concentration, which, in turn, initiates their dissolution (see Fig. 2.6b). This process of diusional material redistribution from small to large NCs is known as OR. The driving force is the minimization of the surface energy of the whole ensemble of secondphase particles. With respect to the BCs Eqs. (2.25) and (2.26) the solution of Eq. (2.24) in the case G =is given by c(r) =c u ; R[c u ; ^c(r)] r for r R: (2.3) After substituting the average local concentration c for c u and assuming ^c = c GT, the corresponding growth law reads dr dt = ;DV a R c GT (R) ; c (2.3) which is obtained by integrating the monomer ux through the NC surface. A more detailed discussion of OR, including the inuence of diusion and reaction control, will be given in Chapter 4. There it will be discussed that this NC description is a good approximation for highly dilute systems, i.e. for vanishing volume fraction of the second phase. However, typical systems in IBS have volume fractions of the impurity phase of several percent. In this case, NCs are not embedded independently in an uniform background sea of dissolved monomers. Rather, NCs interact via monomer diusion and the local monomer concentration is now a function of the NC size and space distributions.
33 2.5. MODELING AND SIMULATION APPROACHES 23 time Figure 2.7: Schematic drawing of coalescence of two growing NCs in the course of implantation. As a consequence, in a local meaneld approach Eq. (2.3) is modied by a term taking into account the diusional NC interactions. Coalescence stage In systems with very high precipitate densities and/or continuous monomer supply during implantation, neighboring NCs may touch each other and start to merge (see Fig. 2.7). For these coalescence events the touching zone is characterized by surfaces with negative curvature which have a lower equilibrium concentration than the solidus. Therefore, IAs will preferentially migrate in this area either by surface or bulk diusion and a rodlike precipitate will evolve in a transient stage. The formation of a continuous buried layer by IBS proceeds on the basis of coalescence of smaller precipitates. 2.5 Modeling and simulation approaches Progress in Materials Science is driven by a thorough qualitativeaswell as accurate quantitative understanding of basic physical and chemical processes. Supported by the tremendous increase of computing power, modeling and simulation of system properties starts to compete with conventional experiments in gaining knowledge of complex systems. This has created the new discipline of Computational Materials Science with the ultimate goal to give precise predictions of the physics and chemistry of materials. In the area of ion beam modication of materials (simulation) models describing the implanted impurity redistribution as well as defect generation are of general interest. Using the BCA of ionsolid interactions, TRIM (SRIM) [47], for instance, is widely used to calculate implantation proles as well as to obtain defectrelated data, e.g. vacancy or interstitial distributions. Special developments of BCA codes include the treatment of channeling eects in crystals (CRYSTALTRIM [74]) and the consideration of dynamical changes of the substrate composition in the course of implantation (TRIDYN [75, 76]). However, these approaches do not include (i) the phase transition to precipitates usually observed in highdose implantations and (ii) defect evolution. Thus a consistent model describing all processes of IBS starting from a BCA description of ionsolid interaction to latestage annealing phenomena is not yet available. The traditional way of modeling phase transitions given a particular supersaturation is based on two complementary descriptions due to the experimental observation methods:
34 24 CHAPTER 2. ION BEAM SYNTHESIS OF NANOSTRUCTURES Information about phase separation can be obtained by (small angle) Xray and neutron scattering (see, e.g. [34]), where one measures the structure factor S( ~ k t) of the system (with respect to the scattering wave vector ~ k ). The structure factor is dened as the Fourier transform of the twoparticle (or local concentration) correlation function G(~r t) =hc(~x + ~r t)c(~x t)i and reads S( ~ k t) = X ~r expfi ~ k~rgg(~r t): (2.32) The evolution of the system can be studied by seeking a solution to the highly nonlinear equation of motion for the structure factor [56, 77] " = ;2Mk ~ k + X n=3 (n ; )!! Kk 2 2 S( ~ k t) c n n c S n ( ~ k t) +2Mk 2 ; (2.33) where M denotes the mobility of single particles and K is proportional to their squared mean interaction range. The coarsegrained free energy f of the system is expanded around the (macroscopically) averaged concentration c of the minority component and S n ( ~ k t) are Fourier transforms of higherorder paircorrelation functions. This description is especially suited to study spinodal decomposition. A more direct method is to determine the distribution function of NCs f(s t) via TEM, where s is a measure of the NC size (either the radius R or the number of particles i). In principle the evolution of the phase separation is completely dened by the general kinetic equation of the time evolution of f(i t) = X i = ; 2 k ; (i + i i )f(i + i t)+ 2 Xi; i = k ; (i i )f(i t) ; X i = Xi; i = k + (i ; i i )f(i t)f(i ; i t) k + (i i )f(i t)f(i t): (2.34) Taking additionally into account the splitting of NCs into smaller fragments (rst term on rhs) as well as coagulation of NCs of sizes i and i (third term), the last equation is a generalization of Eq. (2.), where only monomer evaporation and condensation have been considered. The fundamental problem is to determine the rate coecients k (i i ). Various aspects of IBS of precipitates and the corresponding redistribution of implanted IAs have been modeled on a wide range of time and length scales. Whereas Molecular Dynamics (MD) studies deal with detailed atomic interactions on time scales of picoseconds
35 2.5. MODELING AND SIMULATION APPROACHES 25 and MonteCarlo (MC) methods stochastically describe the dynamics of large numbers of particles, several mesoscopic and continuum (thermodynamic) approaches allow to model phase transitions starting from nucleation or spinodal composition to latestage coarsening phenomena of large ensembles of NCs Atomic description On an atomic scale two simulation methods are commonly used, which are based on quite dierent footings. Since MD studies are only of marginal and supporting use with respect to IBS of nanostructures, the emphasis in this work will be on MC methods. Molecular Dynamics approach In MD simulations (see e.g. [79]) the evolution of a set of interacting atoms is followed by solving the corresponding Newtonian equations of motion. At a given instant the positions f~r i (t)g and momenta f~p i (t)g are known. Then, according to the chosen interaction potential, the forces acting on each atom are computed. This species the evolution of the system within a time interval t, after which the algorithm is repeated. The most important part of MD simulations is the choice of the interaction potential. Depending on the size of the model system and the accuracy needed, interaction potentials range from rst principles quantum mechanical based to semiempirical and empirical potentials. Since typical time scales of atomic motions within a condensed matter system are on the order of picoseconds this computationally intensive method is only applicable for phenomena at best on the order of a few nanoseconds. Thus, at present MD is restricted to the study of fundamental ionsolid interaction processes, for instance the physics of damage creation (see e.g. [53]). However, MD simulations have proven to be very valuable in computing structural and electronic properties of materials. For instance, energy barriers for diusion can be computed and equilibrium properties of small to medium nanoclusters like congurationdependent binding energies and geometries can be obtained. MD results are often used as input parameters for other simulation approaches like MC methods. MonteCarlo approach The MC method has been proven to be an ecient means to describe complex systems with very large degrees of freedom, as they are characteristic for problems in condensed matter physics [37, 8]. Since for such systems the exact computation of physical observables is impractical, one relies on statistical methods like MC simulations in order to get numerical approximations. Based on specic physical models, MC simulations allow for direct comparisons to experiments as well as they can bridge the gap between experiment and theory by exploring the consequences of particular theoretical assumptions and approximations.
36 26 CHAPTER 2. ION BEAM SYNTHESIS OF NANOSTRUCTURES In a statistical model the state of a system is described by a corresponding conguration X in phase space. Let S = fx g denote the set of all possible congurations and P (X t) their timedependent probability distribution, where d = dim(x ) denotes the microscopic degrees of freedom. If a system is described by a model Hamiltonian H then the thermodynamic equilibrium value of an observable O at time t is given by hoi (t )= Z S O(X t )P (X t )dx P (X t)= exp f;h(x t)g (2.35) Z where Z denotes the partition function. The underlying idea of MC simulations is to compute average values of observables based on stochastically chosen phase space congurations. For this purpose one can randomly choose N congurations, weigh them according to their thermodynamic probability, i.e. their Boltzmann weight, and calculate their average. The problem of this "simple sampling" method is the highdimensionality of the phase space which makes it dicult to pick out the important congurations. This problem can be circumvented by the method of "importance sampling", where only statistically signicant states enter the calculation of expectation values hoi. This is achieved by constructing a Markovian chain of con gurations X k k = ::: M, which tends to converge to the thermodynamic probability distribution P eq in the limit k!. Starting with the Master equation describing the evolution of the = X X W (X!X )P (X t)+ X X W (X!X)P (X t) (2.36) where the transition probabilities W connect two states, the principle of detailed balance P eq (X k )W (X k!x k+ )=P eq (X k+ )W (X k+!x k ) (2.37) is used to generate the congurations X k. While the application of Eq. (2.37) is sucient to guarantee convergence of the Markovian chain [37] the explicit form of the transition probability W is not xed. Whereas any choice satisfying W (X k!x k+ ) W (X k+!x k ) = exp f;hg H = H(X k+) ;H(X k ) (2.38) is permissive, the Metropolis method [8], where ; exp f;hg H > W (X k!x k+ )= ; otherwise (2.39) has gained considerable attention. The constant in Eq. (2.39) is an arbitrary constant, which isinterpreted as a time scale in dynamic MC simulations (see Section 3.5.2). Usually the Metropolis algorithm corresponds to the local change of one degree of freedom, but also cluster algorithms changing many degrees of freedom at one instant are frequently used [82, 83]. The acceptance of transitions to states with higher energy can be understood by noting, that the free energy rather than the internal energy is subjected to minimization.
37 2.5. MODELING AND SIMULATION APPROACHES 27 Standard MC is used to calculate thermodynamical equilibrium values, thus the transition probabilities have not to be related to the explicit dynamics of the system. In contrast, in kinetic MonteCarlo simulations the emphasis is on relaxation or nonequilibrium processes. Thus the Markovian chain to be generated has to represent a possible evolution of the system, i.e. conguration changes have to correspond to actual physical processes. Since each event in real systems, e.g. a thermally activated single diusion step of a particle, happens with some probability per unit time, this provides a means to couple physical time scales to the time scale of kinetic MC events. 6 Besides the dynamical part MC simulations are characterized by the geometry. In general MC simulations are used for continuum as well as for discrete models. If the particles are dened on lattice positions then the system is usually called a lattice model. MC methods have been extensively applied to study the properties of magnetic systems. A frequently used model Hamiltonian for uniaxial ferromagnets is based on the Ising [84] model, where interactions are restricted to nearestneighbor spins Here S i H = ;J X hi ji nn S i S j ; H NX i S i S i = : (2.4) corresponds to the spin of lattice site i (pointing either up or down), J is the exchange energy (J > for ferromagnetic and J < for antiferromagnetic systems, respectively), H denotes an external magnetic eld, and the summation is to be taken once over all nearestneighbor pairs and N lattice sites, respectively. By the transformation C i =(; S i )=2 this system is isomorph to a lattice gas model [85, 8] (binary alloy), where each site is either occupied or empty (either occupied by ana or B atom). Thus, the average magnetization per lattice site given by hmi = N ; P i S i is now equivalent to the concentration c = N ; P i C i. Furthermore, the chemical potential, measured from its temperaturedependent critical value c, replaces the magnetic eld as driving force of phase transitions. The correspondence between Ising ferromagnet and lattice gas can be summarized as hmi! ( ; 2c) and 2H! ( ; c ): (2.4) In magnetic systems, the number of, say, upspins is not xed, thus the state of the systems is described by the nonconserved order parameter magnetization M. Accordingly, in MC studies the evolution of such systems is modeled by single spinip attempts (known as kinetic Glauber model [86] usually referred to as model A). In lattice gas models, the density of particles is usually xed and described by the conserved order parameter c. Therefore, a MC simulation consists of moving a particle to an empty neighboring site, which is equivalent to the spinexchange formalism of Kawasaki [87] (usually referred to as model B). 6 This coupling is justied, if at any time instant only one event takes place, and all events are Poisson processes [83].
38 28 CHAPTER 2. ION BEAM SYNTHESIS OF NANOSTRUCTURES MonteCarlo studies of phase transformations Parallel to the increase of available computing power, MC studies of phase transition phenomena were rst performed to check analytical models, only to take later on the lead in certain areas of statistical physics, where now analytical theories are to be checked with respect to simulation results. Due to the simplicity of the Ising model it has frequently been used to describe eective interactions in manybody systems. For instance, phase diagrams of alloys have been simulated [88], and meanwhile MC calculations of critical temperatures T c (see Fig. 2.3) of Ising models [89] can be considered to be more accurate than analytical approximations [9]. Concentrating in this work on systems with conserved order parameter, the rst comprehensive MC studies on phase transitions of binary alloys in three dimensions were performed in the seventies [9, 92]. Dealing with concentrations of the minority phase 7 up to c = :5, these simulations were primarily intended to study concepts of spinodal decomposition. One important result has been the observation of dynamical scaling of the structure function S( ~ k t) [93][95], which can be expressed as [62, 96, 97] S(k t) / [k m (t)] ;d F (k=k m (t)) (2.42) in d dimensions. Here, k m (t) is the position of the maximum of S and the scaling function F (x) becomes asymptotically independent of time. Note, that studies of the evolution of S( ~ k t) are not restricted with respect to the volume fraction of the minority phase, whereas a characterization in terms of the size distribution function f(s t) becomes meaningless as the percolation threshold c p is approached (c p :3 for the sc lattice). The BeckerDoring theory of nucleation [59] has been the focus of simulation studies [98, 99] for systems of low concentrations quenched into the metastable part of the phase diagram close to the coexistence curve. Additionally, simulations of growth and coarsening of NCs have been performed []. However, in three dimensions these simulations barely exceeded a few 4 jump attempts per IA, thus doubt arises, if the late stage of phase separation has been approached Mesoscopic and continuum descriptions Besides the direct atomic approach there exist several eldtheoretic descriptions of phase separation (for reviews, see Gunton et al. [6] and Langer [56]). The CahnHilliard Cook [55, ] formulation is widely used to study phase transitions, especially those proceeding via spinodal decomposition. The evolution of the system is expressed in terms of a conserved concentration eld (~r t) and a timedependent (coarsegrained) free energy functional F [ (~r (~r = M ~ r 2 F + (~r t): (2.43) 7 Note, that the Ising Hamiltonian Eq. (2.4) shows particlehole symmetry.
39 2.5. MODELING AND SIMULATION APPROACHES 29 Here, M denotes the mobility of monomer components and is a thermal noise term taking into account thermal uctuations (Langevin approach [56]). The free energy functional is usually assumed to have the GinsburgLandau form F = R d 3 r(kj ~ r j;a 2 + b 4 ). Combining both equations leads to a nonlinear partial dierential equation, for which analytical approximations successfully describe early stages of phase separation. The late stages of the evolution can be studied by numerical integration of the governing equation [2] and has been applied to spinodal composition in binary mixtures [3]. This method does not pose any restriction on the volume fraction of the domains of the second phase. More advanced eldtheoretic approaches try to solve the equation of motion [Eq. (2.33)] of the structure factor S via analytical approximations and/or numerical integrations [56, 57]. Another widely used approach describing the decay of a metastable state after the nucleation stage is based on thermodynamic considerations. In the multiply connected space between the secondphase domains a solution for the monomer concentration eld c subject to suitable BCs is sought. The classical theory of the late stage of phase separation has been formulated in a global meaneld manner for vanishing by Lifshitz and Slyozov [4] and Wagner [5] (LSW theory). They succeeded to derive a stationary particle radius distribution f(s t) = f(s) and a power growth law for the characteristic system size, i.e. s / t m (see Chapter 4). In general, in a more realistic local meaneld approach for nite, the evolution of secondphase domains is given by the multidroplet diusion = D ~ r 2 c(~r t)+ X i Q i (~r ; ~r i )+G(~r t): (2.44) Here, for a system with monomer diusion coecient D the eect of an external source term G as well as modications due to the clusters are considered, which are assumed to be pointlike objects characterized by a source strength Q. Recent approaches additionally allow to include nucleation [6, 35, 36]. Other descriptions of the evolution of second phase precipitates are based on a numerical integration of the basic kinetic equations [7][9]. Starting with the balance equation for the cluster distribution function [Eq. (2.)] and determining the kinetic coecients k for monomer condensation and evaporation in the limits of diusion or interface reaction control, the evolution of NCs can be followed from the early nucleation to the latestage coarsening regime. This method [] allows also to show the connection between the kinetic approach of Becker and Doring [59] the thermodynamic approach of Lifshitz and Slyozov [4] and Wagner [5]. Furthermore, systems of coarsening secondphase precipitates have been described in statistical approaches by appropriate multiparticle distribution functions [, 2]. Here, the evolution of individual domains is determined selfconsistently by averaging the multiparticle distribution functions over the positions and sizes of the precipitates. The resulting description in terms of a hierarchy of equations of manyparticle distribution functions is usually truncated at the lowest level. A meaneld approach based on a singleparticle distribution function can be used to model selforganization in nite systems [3].
40 3 CHAPTER 2. ION BEAM SYNTHESIS OF NANOSTRUCTURES
41 Chapter 3 Kinetic 3D lattice MonteCarlo method This Chapter introduces the main simulation tool used in this work in order to study the evolution of nanostructures. Besides presenting some principles and technical details of the MC method, the focus will be on the characteristics of the model with respect to thermally activated processes, i.e. the solubility properties and the validity of the GT relation [Eq. (2.23)]. The incorporation of ballistic eects typical for ion irradiation will only be briey sketched a more detailed description of collisional mixing eects will be given in Section Basic description The IBS of nanostructures involves stages like the nucleation of precipitates out of a timeand spacedependent supersaturated solid solution of IAs which can hardly be modeled with statistical equilibrium concepts. A more appropriate method is an atomic description and, therefore, a kinetic 3D lattice MonteCarlo (K3DLMC) method in the tradition of lattice gas models has been developed [4], which allows to study the evolution of the implanted IAs. In this model the positions of the impurities are dened on a 3D periodic lattice and for their kinetics eective nearestneighbor interactions between impurities are taken into account. This simplied eectiveparticle approach assumes, that the impurity atoms are embedded in a positionindependent potential of the substrate, which includes all the complex interactions between impurity and matrix atoms. For a particular simulation the crystallographic structure of the nanocrystals under investigation determines the type of lattice within the K3DLMC method. For this purpose three lattice types have been implemented in the computer code: (i) the simple cubic (sc), (ii) the bodycentered cubic (bcc), and (iii) the facecentered cubic (fcc) lattices. However, for most of the results presented in this work a fcc lattice description has been used for several reasons: avariety of metals can be found in this crystal structure, e.g. Au or Ag precipitates 3
42 32 CHAPTER 3. KINETIC 3D LATTICE MONTECARLO METHOD z y a x Figure 3.: Construction of the main fcc lattice (grey circles) out of the underlying sc lattice. The remaining nonoccupied sc sites (small circles) build up an additional fcc lattice. The conguration for an arbitrary jump in [] direction is indicated together with the four nearestneighbor positions (black circles) common to the initial and nal site of the jump. formed by IBS in SiO 2 the Co subsystem in CoSi 2 forms a fcc lattice [] the fcc structure is one of the most isotropic lattices and thus suited to describe precipitation in amorphous matrices since Si is composed of two fcc sublattices, the simple fcc description is compatible with directional precipitation eects in this technologically most relevant material. These advantages outweigh the technically (numerically) more expensive treatment compared to simpler lattices like the sc or bcc structures. Since some metals show a bcc geometry of their unit cell, this lattice type is appropriate for corresponding material systems, whereas no elemental NCs crystallize in the sc lattice. The crystallographic structure of a compound of stoichiometry X i Y j for a system of impurities of types X and Y determines the choice of the appropriate lattice for K3DLMC studies. By IBS mostly compound NCs of equal stoichiometry, i.e. of XY composition, have been studied. In this case a fcc lattice is not suited due to its intrinsic phase diagram, which includes X 3 Y, XY, and XY 3 phases, respectively [5]. This becomes clear, because any two nearestneighbor sites have four other nearestneighbor sites in common (see Fig. 3.). For a nearestneighbor pair XY this implies, that it is energetically more favorable for atom X (Y ) to have these four sites occupied by Y (X) atoms. The corresponding degeneracy of the ground state gives rise to a frustrated system. Therefore, this geometry
43 3.. BASIC DESCRIPTION 33 does not lead automatically to a periodic arrangement of both components, if their uctuating local concentrations determine the nanocrystal formation and composition. For the study of the IBS of compound NCs (see Chapter 7.2) corresponding K3DLMC simulations are thus performed using either the sc or bcc lattices, which correspond to the NaCl or CsCl structures, respectively. In this K3DLMC method eective atomic interactions among IAs are incorporated on the basis of a probabilistic stochastic Cellular Automaton (CA) approach [6, 7]. Although the description in terms of a CA supports the consideration of congurationdependent interactions among IAs, the results presented in this work are based on the Ising model [84, 8, 9] as the most simple implementation of a CA. In the Ising model, the potential energy of an IA is just proportional to the number n l of nearestneighbor bonds, where l denotes the coordination number, i.e. maximum number of nearestneighbor bonds. Depending on the lattice type l, the coordination numbers are l =6 8 and 2 for the sc, bcc, and fcc lattices, respectively. As the fcc lattice has been most widely used for simulations the corresponding geometry of a jump conguration is shown in Fig. 3. in order to discuss the method. In the course of the simulation for every jump attempt an IA is chosen stochastically and one out of its l (here fcc = 2) jump directions is determined randomly (if the corresponding lattice site is occupied a new IA is chosen). Next, for both the initial ~r i and nal ~r f sites the number of occupied nearestneighbor sites is counted. Based on this local conguration the jump probability is determined, and, accordingly, the jump will be either performed or rejected. Since each lattice site is completely dened by its occupation state, only a single bit is needed to represent each position. Thus the K3DLMC method can be implemented very eciently on the basis of bit manipulations [4, 9] in order to perform jump attempts of IAs, the core procedure of the code. Furthermore, using a double bookkeeping strategy in bit and coordinate space to keep track of the positions of the impurities (for details see Appendix A), this code (not parallelized) allows the simulation of reasonably sized systems on current toplevel workstations. In particular, depending on the emphasis of the simulation { either large simulation volumina for dilute systems or dense nanostructure distributions { lattice sites of the order of 9 and/or up to several 5 IAs can be modeled for 5 { 7 MonteCarlo steps (MCSs) on acputime scale of several days. Technically, the basic fcc lattice is constructed from an underlying simple cubic one (see Fig. 3.). This approach hasthe advantage of having an additional fcc lattice shifted by ( 2a ) with respect to the rst one. Due to the fact, that a bit representation gives only information about the occupation state but not about the type of occupying species, simulation involving dierent types of atoms need a further criterion for distinguishing atom types. Thus the second fcc lattice can be used to model special problems of IBS, e.g. the eect of an indiusing reactive component of the annealing atmosphere on the redistribution of the implanted impurities (see Chapter 7.). Since the diamond lattice is also composed of two fcc lattices shifted by ( 4 a 4 a 4a), the division of a sc lattice into For all possible local congurations of IAs the jump probabilities are computed once (at the beginning of the simulation and after each temperature change) and then tabulated.
44 34 CHAPTER 3. KINETIC 3D LATTICE MONTECARLO METHOD two independent sublattices used in this approach would provide an eective way for the implementation of the diamond lattice. The loss of coincidence of geometrical relation and internal representation by this conformal mapping is of no relevance, because in the K3DLMC method the lattice type is cast into the properly constructed jump conguration. The chosen geometric implementation of the lattice is especially suited to study systems with () boundaries. However, by topological distortions also () boundaries can be mapped directly into the cubic simulation cell of this approach [2]. 3.2 Energetics and jump probabilities If J l > denotes the energy (bond strength) of a nearestneighbor bond with respect to lattice type l, then the total potential energy of the impurities within the Ising model is given by the Hamiltonian X H = ;J l C i C j : (3.) hiji nn Here, C i denotes the occupation state of site i (C i =for an occupied and C i =for an empty lattice site, respectively) and the sum is to be taken once over all nearestneighbor pairs. Obviously, by establishing a nearestneighbor bond the energy gain of the system is J l. Since any bond is shared by two atoms the potential energy of one IA is E = 2 nj l, where n is the number of occupied nearestneighbor sites. Thus the binding energy of a bulk IA (sublimation energy) is E b = 2 lj l : (3.2) In the schematic drawing of Fig. 3.2a the energetics of an IA in the averaged potential within the Ising model is shown. The activation energy E A denotes the diusion barrier governing a single nearestneighbor jump of an IA. In this model both the matrix diusion of a free monomer and the surface diusion of an adatom on a precipitate surface are subjected to the same activation energy E A. The cluster properties are dened by the bond strength J l between two nearestneighbor IAs. If necessary an additional energy barrier E R at the precipitatematrix interface (whichisbeyond the Ising model, but within the CA approach) can easily be incorporated for a more accurate treatment of monomer attachment and/or detachment rates, i.e. the interface reaction kinetics. Thus the transition probability W if for one atom to jump from the initial site i to an empty nal site f [see also Eq. (2.39)] is given by W if = ; exp f;e A g n f n i ; exp f; [E A +(n i ; n f )J l ] g n f <n i (3.3) where ; = ; denotes the frequency of jump attempts, and n (i f) represents the number of nearestneighbor bonds at the two sites.
45 3.3. INTRINSIC PROPERTIES OF THE MODEL 35 a) b) E R E A E R energy substrate energy substrate E=f(n,E B ) E=f(n,E B) cluster cluster x x Figure 3.2: Energetics of the simulation model. In a) the physical model is schematically shown, where the activation energy E A governs diusion and the energy gain E for monomer attachment is a function of the nearestneighbor bond strength E B. Additionally, an interface energy barrier E R is shown. In b) the renormalized model E A! isshown. In order to reduce simulation time it is convenient to allow every diusion attempt, i.e. ~W if = W if =( ; exp f;e A g), which renormalizes just the time scale of the model (see Fig. 3.2b). Dening l = J l this leads to the dimensionless transition probability nf n ~W if = i exp f;(n i ; n f ) l g n f <n i (3.4) and the quantity = expfe A g gives a measure for the time scale during a single MCS (see Section 3.5.2). In cases where n i > n f, (i.e. transitions, which are energetically not favored), the jumps are nevertheless allowed if a random number chosen from the interval [ ] is less than Wif ~. In this work a MCS is dened by a sequence of N jump attempts of statistically independently chosen IAs out of the full set of N IAs. If for a single jump attempt the randomly determined nearestneighbor site ~r f is already occupied, another randomly chosen IA is checked for a possible jump. For all the simulation results presented in this work the Metropolis algorithm [8] guaranteeing local relaxation dynamics has been used. Neither Glauber dynamics [86] nor cluster updating methods have been applied. Within the Ising model the extension to two dierent interacting types of IAs is straightforward and will be dealt with in Section Intrinsic properties of the model According to the phase diagram (see Fig. 2.3) above a critical temperature T c no phase transition from the disordered to the ordered state is expected. For the nearestneighbor
46 36 CHAPTER 3. KINETIC 3D LATTICE MONTECARLO METHOD Ising model used in the K3DLMC simulations, the critical point depends on the lattice type. Table 3. summarizes the critical properties, which have been obtained either by hightemperature expansions in the case of the bcc and fcc lattices [2] or by extensive MC simulations in the case of the sc lattice [89] (see e.g. Kobe [9] for a survey of critical temperatures and exponents), respectively, since analytic solutions in three dimensions are not known. Based on hightemperature series expansions, the spontaneous magnetization (H! ) near below the critical point is known quite accurately [22] hmi = K l ( ; T=T c ) = 5=6: (3.5) The amplitudes K l depend on the lattice type (K fcc :49, K bcc :5, K sc :57 [23]), whereas the exponent is believed to be universal in three dimensions. Since the critical chemical potential c corresponds to the spontaneous magnetization (see Section 2.5.), with the help of Eqs. (2.4) and (3.5) the phase diagram of the lattice gas close to T c can be determined (see Section 3.5.3). From Eq. (3.3) follows that the K3DLMC model exhibits some general intrinsic properties, which depend only on the value of the dimensionless simulation parameter l and the value of the activation energy for diusion E A, if the number N of IAs is kept constant. In particular, in the renormalized model, NC systems with diering binding energies will evolve similar provided that besides J (2) l = J () l also the relation T (2) = T () holds. The physical time scales, of course, will be usually dierent. For temperatures considerably below T c the shape of a (quasiequilibrated) NC depends on the choice of the simulation lattice. In the case of a sc lattice, the surface of a reasonably large NC consists mainly of () surfaces (Fig. 3.3a), whereas for a bcc nanocrystal the () surfaces are energetically favored (Fig. 3.3b). In the case of a fcc lattice the corresponding NCs tend to have a faceted octahedrallike shape with dominating () surfaces (see Fig. 3.3c). With increasing temperature the pronounced faceting starts to be smeared out [24] and the interface morphology gradually changes from a sharp to a diuse phase boundary. The characteristic NC shapes can be understood in terms of the surface energies of the principal crystal surfaces. Within the nearestneighbor Ising model, the internal energy part of the surface tension I (hkl) is proportional to the number of bonds n(hkl) which Table 3.: Critical points of the threedimensional Ising model expressed per nearestneighbor bond [ c =(k B T c ) ; ]. l sc bcc fcc J l c
47 3.3. INTRINSIC PROPERTIES OF THE MODEL 37 a) b) c) Figure 3.3: Quasiequilibrated shape of a NC at T :5 T c consisting of roughly atoms condensed into the (a) sc, (b) bcc, and (c) fcc structures (the darker the blue (grey) scale, the higher the energy state). In each case, the lineofsight is the [] direction. have to be broken in order to bring a bulk atom to the (hkl) surface layer. Thus I (hkl) = J ln(hkl) 2S(hkl) (3.6) where S denotes the surface area per atom, and the factor =2 accounts for the fact, that per nearestneighbor bond only the energy J l =2 is associated with each atom (by cutting through a crystal, two new surfaces are created). Table 3.2 lists the surface energies for the three principal surfaces of each of the three lattices. For instance, since for a fcc structure the () planes are energetically most favored, the surface of a single NC consists to a large fraction of the eight geometrically dierent () planes. Resulting sharp edges are usually smoothed to () planes. This specic shape is predicted by constructing a fcc nanocrystal according to the Wulff plot Table 3.2: Characterization of the lowindexed surfaces of the sc, bcc and fcc lattices in terms of the number of broken bonds n per surface area S of an atom belonging to a (hkl) surface [25, 26]. l sc bcc fcc hkl n(hkl) S(hkl) I (hkl) I () n(hkl) S(hkl) I (hkl) I () n(hkl) S(hkl) I (hkl) I () p a 2 4 a =2 a 2 2= p 3 p p p p p 2 2 a a 2 6 2=2 a 2 6=2 p p p p p 3 3 a a =4 a 2
48 38 CHAPTER 3. KINETIC 3D LATTICE MONTECARLO METHOD a) b) c) Figure 3.4: Scheme of the transition from atomicscale to spherical cluster representation. In a) an ensemble of fcc NCs is shown. In b) each NC is superimposed by a sphere, whose radius is given by Eq. (3.7). In c) only the spheres representing the NCs are drawn. (see e.g. [27]). Recently, Huang et al. explicitly compared the shape of fcc NCs obtained by a similar lattice MC method with the corresponding Wulff construction and found very good agreement [28]. 3.4 Analysis of simulation data For the extraction of simulation data (mainly the size and space distribution of the NCs) after a certain number of MCSs the whole simulation volume is scanned for the lattice positions of the IAs. For instance, if a llattice site is occupied a recursive procedure checks all l nearestneighbor positions for further IAs. After the scan the numbers of monomers, dimers, trimers,..., or any agglomeration of interconnected IAs are known. In this work the size of a cluster is given by the number i of atoms it consists of. This standard Ising droplet model is justied at low temperatures and concentrations close to the coexistence curve, but fails close to T c (diverging correlations) or beyond the percolation threshold. Furthermore, the position of each NC is calculated, which isdened as the center of mass of its IAs (with appropriate translations at periodic boundaries of the simulation box). Since the system is completely dened by the coordinates of the IAs, more advanced data analysis, e.g. pattern recognition, can be done. Since TEM micrographs are the main method for the analysis of NC distributions formed by IBS, a characterization in terms of the number of IAs is not adequate. Hence, in this model the size of one (equilibrated) NC is approximated by the radius of the smallest possible sphere which allows to accommodate the number of its atoms on regular lattice sites (see Fig. 3.4). This relation is given by 4 3 R3 = iv a = i a3 l p l i (3.7)
49 3.4. ANALYSIS OF SIMULATION DATA 39 a) b) t ( 3 MCS) 2 Figure 3.5: K3DLMC simulation of coalescence of two NCs consisting of N 46 and N 2 5 IAs at fcc =2. Snapshot a) shows both NCs shortly after merging. In b) the evolution of as dened in Eq. (3.8) is plotted. where p l denotes the number of atoms per unit cell (p sc =, p bcc = 2, and p fcc = 4, respectively). However, the problem arises to dene a lower limit i l of NC size, because a monomer can hardly be considered as a NC. Unless otherwise stated, in this work the (arbitrary) choice i l = 6 has been used. It should be noted that this procedure of a spherical cluster approximation does a very poor job in the case of two coalescing precipitates. In this case the analysis of the radial inhomogeneity of a NC helps to some extent to reveal its shape. For this purpose the normalized mean square distance from the center of mass of the NC has been introduced, which is dened as (analogous to the moment of inertia) = MR 2 Z V NC r 2 dm: (3.8) Here R denotes the radius of the NC [as determined by Eq. (3.7)], M its mass, and the integration is to be carried out over the whole volume V NC of the NC. 2 The evolution of for two coalescing NCs can be seen in Fig For comparison it should be noted that for an equilibrated octahedrallike NC NC :54, which is only approximately % o the value of a homogeneous sphere ( sphere = :6). Recording for each NC during the K3DLMC simulation provides a means to check, for instance, the ion uence threshold of NC coalescence during ion implantation, or the relative contribution of coagulation to NC coarsening (see Section 6.), because in the case of two touching precipitates considerably exceeds the value of a homogeneous sphere. 2 In this discrete lattice model for the evaluation of the integral is replaced by the sum over all interconnected IAs.
50 4 CHAPTER 3. KINETIC 3D LATTICE MONTECARLO METHOD 3.5 Gauging of simulation parameters The K3DLMC method allows to give predictions of the nucleation and growth behavior of NCs of specic ionsolid systems if the parameters of the simulation are chosen according to the applied implantation parameters and the material properties of the NC/substrate system. The free simulation parameters of the model, i.e. the lattice constant a l, the activation energy for diusion E A and the energy J l of a nearestneighbor bond between IAs, can be deduced from the implantation parameters and the material constants Length scale The basic length scale of this K3DLMC model is the lattice constant a l of the lattice, on which the IAs diuse and may condense to precipitates or form other kinds of nanostructures. For corresponding K3DLMC simulations the value of a l is accessible by Xray diraction measurements at samples containing reasonably large NCs or simply by taking tabulated bulk values. The sizes of the simulation box are hence expressed in terms of the lattice constant a l, i.e. L i = 2 n i a l, i = x y z. The discretization of the box volume in powers of 2 has advantages concerning the implementation of periodic BCs. Since each lattice point is stored as a bit, the determination of the coordinates of the nal site of a nearestneighbor jump can be performed merely by bit manipulations, even if the jump of an IA takes place across the boundaries of the simulation volume. Besides the implantation temperature, the main parameters of IBS of nanostructures are the projected range R p of the impurity prole (related to the ion energy E) and the ion ux j and ion uence F. Since all three quantities are related to a length scale they are derived in the K3DLMC model with respect to the lattice constant a l of the specic NCs under investigation Diusion coecient, time scale, and ion ux Time dependent quantities like the diusion coecient D sim or the ion ux j are transformed to corresponding K3DLMC quantities via the intrinsic lattice diusion coecient. Diusion coecient The diusion coecient D sim of the K3DLMC method as well as the time scale of a MCS [see Eq. (3.3)] are coupled to the experimentally measured diusion coecient D exp = D expf;e exp A g, where Eexp A denotes the activation energy for diusion. Both D sim and are derived within the framework of the random walk theory of diusion (see, e.g. [29]), which assumes independence of successive diusion steps. The diusion coecient for particles on a lattice, which are only allowed to migrate to nearestneighbor positions,
51 3.5. GAUGING OF SIMULATION PARAMETERS 4 is given by [29] D latt = l ;a 2 l (3.9) where ; = ; is the eective jump frequency, a l is the lattice constant, and l = f6 8 2g denotes the corresponding coordination number of the three lattices used for the simulations. Note, that the jump frequency is the product of the frequency of jump attempts ; times a temperaturedependent probability, i.e. ;=; exp f;e A g. Since it is convenient in kinetic MC simulations to normalize the event with the highest probability to unity, which in the current model corresponds to allow every diusion attempt, the normalized K3DLMC diusion coecient is given by D sim = D latt ; = a2 l : (3.) l By the last equation a jump frequency of one is implied, i.e. ; =(jump attempt), and accordingly D sim is expressed in units of a 2 l per MCS. With the help of the Einstein relation [29] the diusion lengths are related by p 2Dexp t = x = p 2D latt k = p 2D sim k (3.) where k denotes the number of MCSs. Eq. (3.) is valid in the asymptotic limit, i.e. for very large numbers of MCSs. Time scale With the help of Eq. (3.) the time constant, or, equivalently, the jump frequency ;, can be obtained = l a 2 l D exp f;e exp A Thus, due to the temperaturedependent diusion coecient, one MCS can correspond to time intervals, which may dier by orders of magnitude. The total number of MCSs times the duration of a single MCS determines the physical time scale which can be modeled by the K3DLMC method, i.e. t = k. It should be noted that the common choice [37] for the (normalized) transition probability W ~ = [+tanh(h=2)]=2 rescales the diusion coecient, and hence the time scale, by a factor two, because now not every diusion step is performed [ W ~ (H =)==2]. Ion ux g: (3.2) The ion ux j is dened as the number of ions crossing an unit area element per second. In MC terms this corresponds to the number of ions crossing the area a 2 l of an unit cell per MCS. Since the duration of a MCS is temperaturedependent [Eq. (3.2)] the corresponding dimensionless K3DLMC current is given by a 4 l j MC = ja 2 l = j : (3.3) l D exp
52 42 CHAPTER 3. KINETIC 3D LATTICE MONTECARLO METHOD Nearestneighbor bond strength, solubility, capillary length, and surface tension Within the framework of the lattice gas model the value of the nearestneighbor bond strength J l can be gauged by the solubility of the IAs in the substrate and/or by the surface tension. If the solubility (solidus) is known, the bond strength J l can be derived via the intrinsic dissolution properties at a at interface of the bulk phase, whereas the GT relation [Eq. (2.23)] is used to connect J l to the surface tension. In the following it is assumed that the solubility can be described by anarrhenius law c = c expf;e S g, where E S is the activation energy for the dissolution of one monomer. Flat interface solubility The underlying idea is to determine the concentration c of dissolved IAs which are in equilibrium with a at interface of the bulk phase of this material. If c is known for dierent values of l, an Arrhenius plot allows to relate the parameters c and E S to simulation parameters. The initial setup for this simulation approach consists of a layer of atoms, which acts as the condensed phase [3]. If the layer extends from z to z 2, its "bulk" behaviorisachieved by keeping the atoms at z = z 2 xed at their positions (see Fig. 3.6a). Additionally, simulations have been performed for the sc and bcc lattices, where in the initial conguration a quarter of a monolayer was randomly deposited on top (z = z ;) of the bulk layer. Applying periodic BCs in the x and y directions and preventing diusion through the boundary at z =, the minimization of the corresponding thermodynamic potential drives the evolution of the system. This particular setup represents a canonical ensemble (xed simulation volume, number of atoms and temperature), thus the free energy F = U ; TS will be minimized. However, the evolution of both subsystems ("gas" of dissolved monomers and bulk) is determined by achieving the same chemical potential, thus the concentration of monomers is related to the phase equilibrium. For the three lattice types in a series of simulations for dierentvalues of l the averaged number of dissolved IAs 3 is determined after the conguration has reached equilibrium. For this purpose, the evolution of the system was followed for 4 6 MCSs. This period was divided into 5 equidistant time intervals, where at the end of each of the last 4 intervals the number of dissolved IAs was determined. The corresponding averaged concentrations normalized with respect to the available volume within the unit cell of the sc, bcc, and fcc lattices are given in Fig. 3.6bd, respectively. The relation between concentration and scaled temperature has been established with the help of the Arrhenius form c (l) ( l )=A l expf;b l l g: (3.4) The tted values of the pairs of constants A l and B l are listed in Table 3.3. For each 3 In this context, all IAs are counted, which are not connected to the bulk layer. This includes very tiny clusters like dimers, trimers,....
53 c (=a 3 sc) c (=a 3 bcc ) c (=a 3 fcc ) 3.5. GAUGING OF SIMULATION PARAMETERS 43 a) b) c) d) E3 E3 =4 ML FIF t =4 ML FIF t E3 z z 2 FIF t E4 E5 E4 E5 E4 E5 E6 E6 E sc bcc fcc Figure 3.6: Intrinsic solubility properties of the K3DLMC model for the three lattice types. The snapshot of a) obtained after 2 6 MCSs for fcc =:75 indicates the simulation setup in () geometry. The Arrhenius plots in b)d) show the temperature dependence of the solubility of monomers for the sc, bcc and fcc lattices, respectively (labels 'FIF' and '=4 ML' refer to initial conditions of the interface either perfectly at or decorated randomly with a quarter of a monolayer). In the case of the sc and bcc lattices, only high temperature ts have been performed, where the four lowest simulation points have been omitted. lattice type, the tted slope B l is l =2. Therefore, the total binding (i.e. sublimation) energy [Eq. (3.2)] of a monomer E b = B l J l is equivalent to the activation energy E S for its dissolution. This allows to gauge the nearestneighbor bond strength and thus to introduce an absolute temperature into the K3DLMC model. Furthermore, in the limit T!, the bulk density is reached, because the parameter A l for each lattice type is equal to the corresponding number of atoms per unit cell. Since Eq. (3.2) has been veried (at least in the "hightemperature" parts of the simulated l regimes) for all three lattice types, equilibrium conditions independent of the () phase boundaries have been achieved.
54 44 CHAPTER 3. KINETIC 3D LATTICE MONTECARLO METHOD a). b).8.8 T=Tc c (fcc) T=Tc c (fcc) ~c(k fcc = :487) ~c(k fcc = ) E7 E6 E5 c E4 E c.6.8 Figure 3.7: Phase diagram of the fcc Ising model. Using B fcc = 6 and T c as given by Table 3. in a) the solubility according to Eq. (3.4) is plotted. Combining Eqs. (2.4) and (3.5) in b) the hightemperature approximation ~c =[; K fcc ( ; T=T c ) 5=6 ]=2 is plotted as well. Physically, the extrapolation towards T! is only dened for temperatures below the critical temperature T c, because any condensed substance vaporizes above this point. The nature of the coexistence of phases is dened by the thermodynamic properties of the interface. Since it is known, that at a certain temperature T R T c =2 there is a roughening phase transition from a smooth to a rough interface (with diverging interface correlation length) (see e.g. [3, 32] and references therein), the above analysis is furthermore restricted to the regime T <T R. According to the critical temperature of the fcc KIM in Fig. 3.6d the c(t ) phase diagram has been computed in the (normalized) temperature range :48 T c <T < :87 T c far below any critical phase transition (see Fig. 3.7a). While in this temperature regime physically reasonable solubility properties are observed, the limited validity of Eq. (3.4) becomes obvious in Fig. 3.7b, where this relation has been extrapolated into the hightemperature part of the phase diagram. Obviously, at T = T c the particlehole symmetry of the Ising lattice gas Hamiltonian is violated, i.e. c(t = T c ) 6= :5. It should be noted, that measured values of solubilities (c E S) are usually restricted to certain temperature regimes. Therefore, values of c exceeding the bulk density by Table 3.3: Values of the solubility constants of Eq. according to the ts of Figs (3.4) for the three lattice types l sc bcc fcc A l (a ;3 l ) :4 :3 :9 : 4:2 :7 B l 2:98 : 3:94 :3 5:993 :3
55 3.5. GAUGING OF SIMULATION PARAMETERS 45 orders of magnitude (e.g. the solubility of Co in crystalline Si has been determined to c = 26 expf;(2:83 ev)g /cm 3 [33]) are not contradictory, but prevent an exact gauging of K3DLMC parameters. Within the regime of the simulation parameters, in the low temperature range dierences arise with respect to the initial condition (see Fig. 3.6). For instance, starting with a perfect () surface in the case of the sc lattice leads to solubility properties in the low temperature range, which are not in accordance with an Arrheniuslike behavior. Very likely, the system has not yet reached equilibrium, which is due to the special interface kinetics. Adetachment event from a perfect () surface is only permitted by breaking ve out of the six nearestneighbor bonds, whereas an (diusing) adatom has just one eective bond. Thus a large time lag is expected before an equilibrium of the chemical potential has been reached. In the case of the fcc lattice two points should be noted: (i) at most seven out of twelve bonds can be broken in any nearestneighbor jump, and (ii) due to the relatively high isotropy interface mass transfer is supposed to happen via cascade processes involving the break of only a few bonds, which gives a smooth kinetics. Thus even for low temperatures equilibrium conditions should be reached quickly. It would be interesting to compare the solubility with computed values of the chemical potential for the lattice gas [34]. However, this was beyond the scope of this work. GibbsThomson relation A connection between atomic and thermodynamic quantities is established by the GT relation Eq. (2.23), which denes the equilibrium concentration around a (spherical) NC of size 2R with respect to the materialsdependent capillary length R c. In order to exploit Eq. (2.23) it has rst to be shown that the K3DLMC method reproduces the GT relation. This has been done by a series of simulations, where a NC of a specic size ("radius" R) is put in a simulation box of volume V =2 nx+ny+nz a 3 with V =3 R (Fig. 3.8a shows the simulation setup). Like in the case of the at interface simulation, this highly articial initial conguration will evolve at nite temperatures to a state with phase equilibrium between dissolved monomers and the curved bulk phase boundary (see also [35]). For the analysis, averaged over aperiodof2:5 6 MCSs (for the three highest values of fcc in Fig. 3.8b the averaging was over 7:5 6 MCSs) the number of dissolved monomers is determined, which are in equilibrium with this precipitate [36, 37]. For the following analysis the radius of the NC is derived according to Eq. (3.7). In the case of a fcc lattice Fig. 3.8b shows the averaged simulated equilibrium monomer concentrations for several xed MC parameters fcc for various cluster sizes. For each value of the simulation results are approximated reasonably well by the GT relation. Thus two properties of the model can be deduced: The K3DLMC method excellently reproduces the GT relation even for very small NCs
56 c (=a 3 fcc ) 46 CHAPTER 3. KINETIC 3D LATTICE MONTECARLO METHOD a) b) E3 E4 E5 E =R (=a fcc ).6 Figure 3.8: Check of the validity of the GibbsThomson relation within the K3DLMC method. In a) the simulation setup is shown. For the fcc lattice in b) the normalized monomer concentration is plotted versus the inverse NC radius. From top to bottom, the simulations have been performed for fcc =:25 to fcc =2:5 in steps of fcc =:25. By extrapolating for a given the GT relation to a at interface (i.e. R!) the intersection of a t with the yaxis determines the solidus concentration. Furthermore, by plotting the values of the solidus versus the simulation parameter (Fig. 3.9a) the solubility can be derived. Applying Eq. (3.4) to the simulation results one obtains A GT fcc =(3:64 :8) a;3 fcc and BGT fcc =(5:93 :2), which is in good agreement with the results of the at interface analysis (Table 3.3). While one could argue, that the at interface simulations are inuenced by the specic choice of () phase boundaries, the agreement of both simulation results is evidence that the interface orientation of the phase boundary does not eect intrinsic properties of the K3DLMC model. It should be noted, that the GT relation is supposed to be valid also for concave interfaces. For instance, the monomer concentration in a spherical cavity of radius R within the bulk phase should be given by Eq. (2.23) after performing the transformation R!;R (see Fig. 3.). In the particle picture, a positive (negative) curvature corresponds to a convex (concave) phase boundary. In the vacancy picture, the eective surface curvatures are reversed, i.e. convex $ concave. Furthermore, due to the symmetry of the Ising Hamiltonian Eq. (3.) with respect to a particlevacancy interchange [i.e. C i! ( ; C i )], 4 the surface tension transforms appropriately. This particlevacancy symmetry is reected in the GT relation of Fig. 3.. As an implication, the product of the averaged monomer 4 Neglecting a constant term J(L x L y L z ; 2N V ), which xes just the total energy of a lattice containing N V unoccupied sites.
57 3.5. GAUGING OF SIMULATION PARAMETERS 47 Rc (afcc) a) b) c (=a 3 fcc ) E3 E4 E5 c GT R GT c E c fcc fcc Figure 3.9: In a) the solubility properties are derived using results of the solidus obtained by the GT simulations. In b) the tted capillary lengths are plotted versus fcc, where c denotes the critical point (see Table 3.). c p c V ccv c=c R c =R 2 4 Figure 3.: Generalized GT relation of the Ising model relating the equilibrium monomer and vacancy concentrations c and c V to convex and concave phase boundaries, respectively. and vacancy concentrations outside and within a NC is constant, i.e. cc V = c 2. However, up to now the kinetics of phase transitions has been predominantly studied on the basis of the linearization of the GT relation. For instance, cluster growth in the sc KIM has been discussed by Penrose et al. [6, ] in terms of the monomer concentration c. Without referring directly to the GT relation they use as expression for the equilibrium monomer concentration c i of ancconsisting of i particles c i = c + (i ; 2) =3 i>2 (3.5) where is related to the surface tension.
58 48 CHAPTER 3. KINETIC 3D LATTICE MONTECARLO METHOD Capillary length and surface tension A further analysis of the GT data allows an explicit determination of the eective surface tension, which according to the standard terminology denotes the interface free energy per unit area. Plotting the capillary lengths Rc GT versus the scaled bond strength fcc (see Fig. 3.8b) a linear dependence is observed R c ( fcc )=R (fcc) c + fcc a fcc fcc : (3.6) According to the leastsquare t the constants are given by R (fcc) c =(;:32 :9) a fcc and fcc = (2:9 :5). The oset is based on the fact, that at T = T c the surface tension (and thus the capillary length) vanishes (see e.g. [38, 39]). 5 With the help of the relation R c =2V a =(2V a =J l ) l [see Eq. (2.23)] for the capillary length, the surface tension is coupled to the nearestneighbor bond strength J fcc according to = J fcc (R (fcc) c + fcc a fcc fcc )= 2J fcc 2V a fcc a 2 fcc! R (fcc) c + fcc (3.7) a fcc fcc where 4V a = a 3 fcc has been used. The last equation establishes a spherically averaged eective surface tension of a NC, while usually macroscopically measured surface tensions are dened with respect to a specied interface orientation. Moreover, the temperature dependence of (at least in the simulated temperature regime see also Footnote 5) is given by Eq. (3.7), indicating a limiting value! T = 2 fcc J fcc =a 2 fcc for vanishing temperature. In comparison with the surface energies of the principal surfaces (see Table 3.2), T is slightly above the zerotemperature value of I (). Relations similar to Eq. (3.7) also hold for the sc and bcc lattices, but will not be presented in this work. It should be noted, that the surface tension can not simply be obtained by counting the average number N J of broken bonds of the cluster surface atoms and dividing this value by the mean (spherical) surface area A. Having in mind, that the surface tension is composed of an internal I and entropic E part (i.e. = I + E ), this approach would just specify I. The entropic part E = ; ; =A ln S(N J ) accounting for the number of dierent states S(N J ) in phase space is not accessible by this method. An alternative method to obtain the surface tension is the use of Eq. (2.9), i.e. by plotting ln(i);()i versus i 2=3, if the discrete size of the critical cluster and the (constant) supersaturation are known [4, 4] (note that these authors used the spinip kinetic Glauber model, where agiven magnetic eld translates to a corresponding supersaturation via 2H $ ). Although Eq. (2.9), the basic assumption of classical nucleation theory, is usually referred to as capillarity approximation, the capillary length R c is not related to the critical radius of nucleation. This becomes obvious in Fig. 3., where both quantities are plotted. 5 This condition is reasonably satised by the linear extrapolation of the simulation results. However, close to the critical point the surface tension is known to vanish like / ( ; T=T c ) 2 with a critical exponent :6 [39].
59 c (=a 3 fcc ) 3.6. A SIMPLE APPROACH TO COLLISIONAL MIXING 49 E3 R nuc R c E4 E5 E =R (=a fcc ).6 Figure 3.: Replot of Fig. 3.8b, where the nal points in the limit R! of the GT curves give a good approximation of the temperature dependence of the critical NC size. For comparison the temperaturedependent capillary length has been added. For this comparison it has been used, that in general the nal point of the GT curve in the limit R! denotes the critical cluster size i? for nucleation (Section 2.3.2). Although this simulation series was not aimed at determining i? ( l ) exactly, the dependence of the critical size on simulation parameters can roughly be guessed in Fig. 3. (upper right part of the plot a smooth dependence on temperature is expected). Eqs. (3.4) and (3.7) reect intrinsic properties of the nearestneighbor KIM. Combining both relates the surface tension directly to the solubility. Thus care should be taken if for a specic system discrepancies arise in gauging of J l according to reliably measured values of the solubility and the (eective) surface tension. This could be a hint, that the nearestneighbor KIM might fail to give a reasonable description of the system and other approaches like the use of more sophisticated manybody potentials (e.g. embedded atom model) are more appropriate. 3.6 A simple approach to collisional mixing Ion implantation is inevitably accompanied by a specic intensity of collisional mixing (CM), because decelerating ions displace host atoms or previously implanted impurities. In this process both primary knockons (recoil mixing) and interactions with the collision cascade (cascade mixing) determine the displacement probability and contribute to the mean displacement length [42, 43]. Therefore, in order to model NC formation during ion implantation or irradiation, the basic eects of CM, i.e. the displacements of atoms, should be incorporated into the K3DLMC method. From the statistical point of view, CM can be considered as an exter
60 5 CHAPTER 3. KINETIC 3D LATTICE MONTECARLO METHOD nal force, which in addition to thermal forces introduces a further dynamical component. Hence, thermally activated processes, e.g. monomer diusion or evaporation steps, characterized by a nite temperature > compete with ballistic processes, e.g. atomic displacements, independent of temperature ( = ). For binary systems, irradiationinduced (dis) ordering phenomena have been studied for many years [44], and are usually referred to as driven alloys (for a recent review, see Martin and Bellon [45]). The incorporation of CM into the K3DLMC model uses some simplifying assumptions: a displacement probability (displacements per IA per implanted impurity) related to the nuclear energy deposition of the ion and a systemspecic displacement length are assumed the displacement distribution is chosen to be isotropic (which is a rather good approximation of cascade mixing but does not treat correctly the anisotropic nature of recoil mixing [46]) and exponentially decaying, i.e. f(r) / expf;r=g due to the lattice nature of the model, only discrete displacements to (regular) lattice sites are considered the displacements of IAs are not correlated in time and space. In particular no cylindrical region around a hypothetical ion or energetic recoil track is assumed, within which the displacements take place (thermal spike model) if for a statistically chosen IA the nal site for a displacement attempt is occupied, no displacement is performed (e.g. for a displacement of a "bulk" IA within a NC). Furthermore, no replacement cascades are considered. The displacement parameters for specic systems can be estimated by corresponding TRIM (SRIM) simulations [47]. Note, that this approach does not account for the displacement of substrate atoms into a NC and, as a consequence, their evolution within an (compound) impurity NC. Because this Chapter is devoted to the intrinsic properties of the K3DLMC model, which are based on thermally activated processes, a more detailed discussion of the modi cations due to ballistic eects will be postponed to Section Simulation of ion implantation and annealing In the most general case the evolution of IAs during implantation has to be simulated by taking into account deposition, CM, and diusion steps: Deposition: For each single implantation step the new IA is set in the simulation box ata position, which x and y coordinates have been chosen randomly and the z coordinate according to a specied depth distribution, usually a Gaussian. Reasonable choices of the corresponding parameters R p and R p can be obtained by TRIM (SRIM) calculations [47].
61 3.8. APPLICABILITY OF THE K3DLMC METHOD AND DISCUSSION 5 Collisional mixing: According to the number of impurity displacements per atom (dpa) statistically chosen impurities are checked for a displacement Diusion: The implantation parameters then determine the ratio of implantation to diusion steps. For instance, for a xed implantation current, the higher the implantation temperature the more diusion steps occur between two single implantation events. For simulations in cases, where no NCs can be observed in asimplanted samples, steps two and three of the above scheme are simply skipped. In this case a subsequent simulation of annealing starts with the asimplanted prole (this corresponds to a quenched system see process path 4 in Fig. 2.3). However, a detailed modeling of NC formation according to the above scheme, i.e. taking into account CM, has not yet been accomplished. So far, only general aspects of CM have been studied (see Section 5.3.2). For all simulations periodic BCs have been applied in the x and y directions, i.e. perpendicular to the ion beam. In the z direction either periodic, reecting, or absorbing BCs have been used depending on the particular materials system under investigation. In the case of a reecting interface, for instance at z = (the surface), a chosen jump direction across the surface terminates the jump attempt for this atom. A successful jump attempt across an absorbing interface (the virtual lattice sites in the layer directly adjacent to this interface are dened to be empty) causes the removal of this IA. For the simulation of annealing, simply no new IAs are deposited and usually the temperature is increased, i.e. l is decreased. All temperature changes are performed instantaneously (this approximation is justied, since usually the annealing time is much longer than the time the system needs to achieve the new temperature, but may cause problems with respect to the number of nucleated NCs). 3.8 Applicability of the K3DLMC method and discussion To conclude this Chapter, some aspects of the K3DLMC model should be discussed before presenting applications of this method in Chapters 57. By IBS two distinct classes of NCs can be formed. One distinguishes between mixed compound NCs consisting of impurity and substrate atoms, e.g. CoSi 2 nanocrystals observed after Co implantation into csi, and pure precipitates solely built up by IAs, e.g. Au NCs embedded in SiO 2 (impurity compound NCs consisting of two or more implanted atom species also belong to the second class). The approach to assume an averaged positionand congurationindependent potential, which describes an IA within the host matrix, has to be discussed with respect to the two NC classes. For nanocrystals belonging to the rst group, this simplied attempt to model the energetics is justied, if for the precipitation and further growth of these compound NCs only local rearrangements of the bulk atoms occur, which preserve the density of host atoms. For instance, in the phase transition from dissolved Co in csi to CoSi 2 precipitates
62 52 CHAPTER 3. KINETIC 3D LATTICE MONTECARLO METHOD the number of Si atoms per unit cell remains the same (8 Si atoms in a diamondlike cell as well as 8 Si atoms in the CaF 2 like CoSi 2 cell, which both have nearly the same lattice constant a), but they reside on dierent positions. This implies, that the number of host atoms, with which an IA interacts, is constant, and thus this absolute contribution to its energy state can be to rst order neglected. For NCs of the second class, the attachment of an additional monomer is also achieved only by local (on a length scale of the order of an unit cell) rearrangements of (host) atoms, but now the density of the substrate atoms is not preserved, since they are pushed out of the volume, where the precipitate grows. As a consequence, the IAs within this NC do not directly interact with the atoms of the substrate. In this case, the use of an averaged, positionindependent potential is not a priori justied and deserves for thorough studies a further discussion. Associated with the work to be spent tomove the host atoms (radially) away from the NCs of the second type, the resulting densication in the shell surrounding the precipitate is likely accompanied by the development of a strain eld. This inuences the monomer diusion [29] in the vicinity of the NCs, and could result in a sizedependent growth law with a possible upper limit for the NC size. The experimental observation of strong strain elds around NCs would clearly restrict the use of the above described K3DLMC method (for a MC modeling of domain growth in the presence of strain see e.g. Fratzl and Penrose [47, 48]). However, the eect of strain elds can be neglected in systems, where the lattice mismatch between nanocrystals of the rst type and the (crystalline) matrix is negligible. Furthermore, if the substrate is viscous enough at implantation and annealing temperatures, strain is also not supposed to inuence the impurity redistribution considerably. As indicated in Fig. 3.2, a more precise treatment of precipitatematrix interface reactions can be achieved by the introduction of an additional energy barrier E R, which inuences the attachment and/or detachment of monomers. It is known from OR, that for an ensemble of precipitates the evolution depends on the relative strength of diusion and interface reactions [5, 49]. The value of E R controls the degree of diusion to reaction controlled coarsening with large values delaying absorption/desorption events, which then causes a more and more homogeneous monomer concentration in the substrate. An energy barrier eective only for attachment attempts might be a possible way for a simple modeling of the eect of a strain eld around a NC. On the other hand it had been shown, that the evolution of Au NCs in SiO 2 depends on the annealing atmosphere. White et al. [5] found, that coarsening in an Ar + H 2 atmosphere proceeds much slower than in an oxidizing atmosphere. It is reasonable to assume, that hydrogen diusing into the sample passivates the Au/SiO 2 interface, which reduces the driving force for OR. This could be simulated by assuming an additionally energy barrier eective only for detachment. For all simulations homogeneous and constant conditions throughout the simulation volume have been assumed. No attempt has been made to include damage eects caused by ion implantation, thus possibly preferred heterogeneous nucleation of NCs in areas of large damage is neglected, which could inuence the NC distribution. Furthermore, the eect of radiation enhanced diusion is not explicitly taken into account as well as a possible
63 3.8. APPLICABILITY OF THE K3DLMC METHOD AND DISCUSSION 53 trapping of single IAs at lattice defects, which by an articially increased solubility delays the formation of NCs. For the description of diusion, no other diusion channels than nearestneighbor jumps are considered, irrespective, if the modeled impurity redistribution takes place in a crystalline or amorphous substrate. Due to the lattice description the detailed atomic diusion mechanisms (e.g. interstitial diusion, direct exchange, vacancymediated diusion, etc [29]) are not taken into account. The K3DLMC method rather resembles interstitial diusion of impurities in crystals. For modeling of binary alloys the use of the direct XY exchange mechanism is questionable because atomic movements are most likely caused by vacancy diusion (recent simulation attempts of phase separation compared vacancy dynamics with the conventional Kawasaki model [5]). It is assumed, that diusion of impurities can be described either by coupling to experimentally observed diusion coecients or by using the activation energy E A of the most eective diusion channel as obtained by MD simulations. The use of the Ising model to describe nearestneighbor interactions among IAs is a good basis for an ecient description of the evolution of NCs. Despite its simplicity it correctly reproduces the GT relation [Eq. (2.23)], and thus allows a coupling to a thermodynamic treatment of the late stage of the phase transition. However, more sophisticated interaction potentials may be needed in order to model specic problems, e.g. an embedded atomlike potential for the understanding of stressinduced sub nm patterning of CoSi 2 layers, where a modied version of this K3DLMC method has been successfully applied [2]. One inherent property of this K3DLMC method is the xed bonding length between two IAs, irrespective, if it is a dimer or one out of l bulk bondings. However, agglomerations of a few impurities are presumably not positioned on regular lattice sites, rather they are supposed to be in an amorphous order. Hence, this model is not suited to study the properties of very small embryolike NCsas well as of precipitates, which condense in the amorphous state. Within an ensemble of NCs, the diusional screening length [] D (t) = p 4n(t) R(t) (3.8) where n(t) denotes the density of NCs, is an important quantity, because it sets the length scale of NC interactions. Since a monomer detaching from a NCs is very likely to migrate to a nearby precipitate on his random walk, D denotes the distance beyond which the diusional interaction is screened by the remaining ensemble a NC is embedded in. Thus the K3DLMC simulations have to be checked, that selfinteractions of NCs are avoided in cases, where periodic BCs are applied. Due to the lattice description all ordered phases have the same orientation. This provides a good description for a phase transition in a single crystal, but fails to model the random orientation of NCs in amorphous substrates like SiO 2. Furthermore, since in this K3DLMC model all ordered domains are in phase (all IAs are located on the same lattice) no grain boundary eects can be studied. By appropriately extending the model, e.g. by
64 54 CHAPTER 3. KINETIC 3D LATTICE MONTECARLO METHOD using the qstate Potts model [52, 53] or assigning a further parameter to each lattice point [28] grain boundary studies have been performed. Furthermore, systems with dierent coexisting NC types can not be modeled in detail, for instance IBS of CoSi 2 precipitates in Si, where A and Btype clusters are formed (the plateletshape of Btype CoSi 2 NCs is not caused by intrinsic lattice properties rather by a rotated () surface with respect to the Si lattice). Phase transformations characterized by dierent crystallographic structures of the ordered domains (e.g. FeSi 2 phase diagram) are also not directly accessible by the current K3DLMC model.
65 Chapter 4 General description of diusion and reaction controlled Ostwald ripening 4. Characterization of OR and recent developments The last stage of IBS consists usually of a thermal heat treatment of the implanted sample because of two major reason: (i) the radiation damage within the substrate can be (at least partially) annealed out (ii) the mean NC size can be increased and, therefore, be adjusted to a predened value. In case (ii) the physical process governing the evolution of an ensemble of precipitates is known as Ostwald ripening (OR) [54]. More precisely, OR controls the late stage of a phase transition of a closed twophase mixture (either dissolved monomers or secondphase precipitates) within a chemically neutral matrix (see Fig. 2.). Since a considerable amount of energy is associated with the phase boundary, i.e. the precipitate/matrix interface, the system is not in its lowest energy state. Therefore, the minimization of the surface contribution to the total energy is the driving force governing the dynamics of the material redistribution. Accordingly, small NCs (characterized by a high surfacetovolume ratio) will dissolve and the corresponding material mass transfer to larger precipitates is mediated by diusion. A measure of the instability of the system is the degree of supersaturation of monomers, which is dened as the dierence between the average concentration due to the presence of NCs and the equilibrium solubility. From the theoretical point of view OR can take place in between two limiting kinetic regimes: (i) diusion controlled ripening or (ii) reaction controlled ripening. For specic systems the coarsening characteristics is determined by the ratio of the monomer diusion coecient D and the interface reaction rate k, which isgiven by the transfer velocity of impurities across the phase boundary [5]. The latter quantity takes into account the concept of a reaction barrier by xing the reaction rate of dissolved impurities at the precipitate/matrix interface. The ratio D=k relates the time scales of diusion jumps to monomer attachment/detachment rates. In ripening mode (i) the limiting process is the diusion of monomers between precipitates assuming that monomer attachment/detachment events take place on a much shorter time scale. Therefore, rather large concentration gradients 55
66 56 CHAPTER 4. GENERAL DESCRIPTION OF OSTWALD RIPENING should be established between welldened equilibrium monomer concentrations of shrinking and growing NCs. In reaction controlled ripening, diusion is fast compared to mass transfer across the interface, which results in much less pronounced concentration gradients between NCs. A comprehensive theory of OR in 3D was rst developed by Lifshitz and Slyozov [4] and independently by Wagner [5] (LSW theory) for the limit of vanishing volume fraction! of the impurity phase. In the regimes of pure diusion or reaction controlled coarsening, they derived the time dependence of OR in the asymptotic limit, i.e. the growth law for the mean NC radius R / (t=)m, where is a characteristic time constant and m is determined by the mode of ripening. Furthermore, they showed, that the particle radius distributions (PRDs) have a timeindependent stationary shape, if the NC sizes are scaled by R. Although being qualitatively very successful in describing coarsening phenomena, a serious shortcoming of the LSWtheory is the inherent global meaneld approach. Since each precipitate is treated as an isolated particle, diusional interactions between individual precipitates are not taken into account. In order to extent the limited validity of the LSW theory, much eort was devoted to study the eect of nite volume fractions and, as a consequence, spatial correlations on particle coarsening. Using dierent approaches, among others Brailsford et al. [55], Tsumuraya et al. [56], Marqusee et al. [57], and Mardar [58] derived a dependence of OR on. While there is agreement that a nite volume fraction does not change the time exponent m but increases the rate of coarsening [() <( = )] and gives rise to a broader PRD than compared to the LSW theory, the precise dependence on (usually expressed as an expansion in p ) seems still to be controversial (see, e.g. [59, 6] and further references therein). Very recently, Alkemper et al. [6] have shown for a solidliquid system (with %) satisfying all assumptions of the LSW theory the importance of transient eects [62] during phase separation. While most theories assume steadystate coarsening, they have pointed out that such conditions are usually not met in experiments and, therefore, give a reasonable explanation of the observed discrepancies. Computer simulations based on meaneld descriptions have been performed mainly in the diusion controlled limit. Pioneering work was done by Voorhees and Glicksman (VG) [39, 4], who treated the interacting precipitates as xed pointlike sources characterized by a (ctitious) radius. By dening a dimensionless supersaturation (~r t) = [c(~r t);c ]=c they solved the modied timeindependentmultidroplet diusion equation ~r 2 (~r )=;4 X i Q i (~r ; ~r i ) (4.) with respect to BCs given by the linearized GT equation [Eq. (2.23)]. In their approach the individual source strengths Q i (corresponding to a monopole approximation of a full treatment of NC interactions) determine the evolution of NCs (dr i =dt / Q i ) within the P i Q i =. While the VG method is computa restriction of material conservation, i.e. tionally very extensive due to the included mutual interaction of all precipitates, dierent simulation approaches by Beenakker [63] and Enomoto et al. [64] explicitly used diusional screening properties present in an ensemble of NCs. By restricting the range
67 4.. CHARACTERIZATION OF OR AND RECENT DEVELOPMENTS 57 of NC interactions they were able to model larger and thus statistically more signicant systems. With the rapid increase of computer power, it has later been possible to include higherorder (dipole,...) terms of NC interactions which account for migration and spherical shape deviations of precipitates [65, 66]. Whereas most of the theoretical and simulation studies considered fundamental properties of (at least on a large scale) homogeneous coarsening systems, special attention was paid also to the mechanisms of pattern formation [67, 68]. In a theoretical study Venzl found rst indications of selforganization of precipitates by OR [69, 7]. Later on Reiss et al. [7, 72] developed a model based on VG, which allowed to study properties of spatially inhomogeneous systems. A typical example are precipitates formed by ion implantation which evolve in a thin lm with explicit boundaries (e.g. the surface of the sample) and show a depthdependent size distribution. In particular, they could explain the selfstructuring of NCs by OR into bands parallel to the surface as has been observed in IBS. A more general study of OR has shown that selforganization of spatial patterns is an inherent property of an inhomogeneous ensemble of clusters [3]. Other widely studied areas of OR are theoretical descriptions of 2D systems (see, e.g. [73, 74] and references therein), with special attention to the evolution of dislocation loops [75, 76] and the coarsening behavior of clusters on surfaces [3]. Since in a lot of cases the evolution of NCs in solids is inuenced by elastic forces (e.g. lattice mismatch between nanocrystals and crystalline substrate), the description of OR in the presence of strain elds is also a vividly studied part of materials science (see, e.g. [77, 78] and references therein). After Wagner's treatment of reaction controlled OR, in meaneld approaches the inuence of interface kinetics on particle coarsening appears to have been studied only occasionally. Based on the growth behavior of an alloy, which was not conform with the diusion controlled regime of OR [79], White derived a description for competing inuences of diusion and reaction control [8]. On an atomic level Lavine et al. set up amcmodel, where they explicitly included an escape probability of monomers from NCs in order to simulate dierent regimes of coarsening [8]. In this Chapter the model of Reiss [7, 4, 72, 82] has been extended from the diusion controlled limit to the whole range of the quantities D and k. In addition to demonstrating that this local meaneld approach reproduces the basic results of the LSW theory in the two limiting cases, this general description is applied to study intermediate coarsening processes. Furthermore, this approach allows to model open systems, e.g. growth of NCs during implantation, as well as the correct treatment of external sinks, e.g. absorbing interfaces. In what follows, at rst the basic physical concepts are introduced by considering a single isolated NC, and results of the LSW theory are presented. Then a general expression for the source strengths of interacting NCs is derived and, nally, typical results will be discussed.
68 58 CHAPTER 4. GENERAL DESCRIPTION OF OSTWALD RIPENING monomer concentration c u c c^ GT 2R x Figure 4.: Schematic drawing of the monomer concentration eld around a single NC of radius R due to diusion and interface reaction inuences. In the general case, ^c adjusts between the diusion controlled (c GT )andreaction controlled (c u )values. 4.2 Fundamentals of the model 4.2. Evolution of a single nanocluster In an extension of the discussions of Section 2.4 rst the evolution of a single NC is described in the general case of diusion and reaction controlled OR. Considering the adiabatic limit (i.e. neglecting the time derivative of the concentration eld, which is justied if the growth rate of a NC is slow compared to the resulting changes of the impurity concentration) the stationary homogeneous diusion equation ~ r 2 c(~r ) = (Laplace equation) has to be solved. With respect to BCs Eqs. (2.25) and (2.26) the solution of Eq. (2.24) in the case G = is repeated here for convenience c(r R) =c u ; R[c u ; ^c(r)] : (4.2) r Material conservation requires, that the reaction ux "through" the precipitate/matrix interface, i.e. the net attachment and detachment rate for growing or shrinking NCs, is equal to the diusion current ~ di = ;D rc(~r ~ ) evaluated at this interface. Assuming a linear ansatz [5] ~ reac = k c GT (R) ; ^c ~e (r) (4.3) where k is a radiusindependent reaction rate describing both monomer attachment and detachment, c GT (R) the radiusdependent equilibrium solubility [Eq. (2.23)], and ~e (r) the radial unit vector pointing outward, the monomer concentration at the interface (see Fig. 4.) can be evaluated as ^c(r) = krcgt (R)+Dc u : (4.4) kr + D Thus, the evolution of a precipitate consisting of N atoms is given by the growth rate dn dt = ; I ~ j r=r d ~ S = ; 4R2 kd kr + D c GT (R) ; c u : (4.5)
69 4.2. FUNDAMENTALS OF THE MODEL 59 Obviously, a shrinking NC acts as a source of monomers and thus feeds the surrounding concentration eld c(~r t). Therefore, a precipitate is characterized by its source strength, given by Q = ;dn=dt, which is dened as the number of atoms it puts into solution per second. Thus Eq. (4.2) can be expressed as c(r R) =c u + Q 4D r : (4.6) As a result, for a single NC one obtains for the interface monomer concentration and source strength in the two limiting regimes: Diusion control: kr D ^c(r) =c GT (R) Q =4DR c GT (R) ; c u : (4.7) Reaction control: kr D ^c(r) =c u Q =4R 2 k c GT (R) ; c u : (4.8) Evolution of an ensemble of nanoclusters An ensemble of NCs is described by the timedependent PRD f(r t), where f(r t)dr denotes the number of particles per unit volume whichhave a radius between R and R+dR. Accordingly, the NC density, normalized to unit volume, is given by n(t) = R f(r t)dr. In the limiting case of a highly dilute system, a growth law can be derived, where all NCs are embedded in the same average concentration c. This growth law is given by Eq. (4.5) after substituting c for c u dr dt = ; kdv a kr + D c GT (R) ; c : (4.9) According to the GT relation [Eq. (2.23)], for a given (materialsdependent) capillary length R c the mean concentration c is associated with a specic NC radius R? R? = R c ln(c=c ) : (4.) This radius is called the critical radius because precipitates larger than R? will grow, whereas those being smaller will shrink. With the help of the linearized GT equation c LSW (R) =c ( + R c =R) (4.) Eq. (4.9) can be written as dr dt = ; kdv a c R c kr + D R ; RR? : (4.2)
70 6 CHAPTER 4. GENERAL DESCRIPTION OF OSTWALD RIPENING The evolution of NCs can be expressed as a continuity equation for f in size @R =: (4.3) For closed systems, the amount c per unit volume of minority phase(impurities) consists of dissolved monomers and precipitates. Both parts are related according to material conservation c = (t)c NC +[; (t)]c(t) = const. (4.4) where (t) =4=3 R R 3 f(r t)dr denotes the precipitated volume fraction per unit volume and c NC is the concentration of monomers within a NC. Combining Eqs. (4.2)(4.4) and introducing a normalized radius = R=R?, Lifshitz, Slyozov [4] and Wagner [5] have derived the following distribution functions, characteristic time constants and time dependences of the critical radius R? (t) (the mean radius R, respectively) and the NC density n(t): Diusion control f( t) / 8 >< >: 2 R? (t) =R? (t =) 3 4=3 + t 3+ di 7= ; =3 exp n o ; 3 2 ; LSW max = 3 2 > LSW max + t di =3 (4.5) di = 9[R? (t = )] 3 4c DV a R c R? = R (4.6) n(t) / t ; for t di (4.7) Reaction control f( t) / 8 < : R? (t) =R? (t =) 2 (+ t reac )2 2; 5 n o exp ; 3 2; > LSW max + t reac =2 LSW max =2 (4.8) reac = 2[R? (t = )] 2 c kv a R c R? = 9 8 R (4.9) n(t) / t ;3=2 for t reac (4.2) Both PRDs are shown in Fig. 4.2a. Note, that theoretical descriptions of OR for nonvanishing volume fraction predict max > LSW max. Furthermore, it should be stressed, that the LSW theory is based on the linearization of the GT relation [see Eq. (4.9)]. Thus care has to be taken by applying the LSW theory to systems, where R Rc is not valid. As Fig. 4.3 indicates, the exact GT relation gives much higher equilibrium concentrations for R. R c, thus NCs in this regime tend to dissolve more rapidly than the LSW theory predicts. As a consequence NC ensembles with R. Rc can not be described by Eqs. (4.5)(4.2). Rather, they will exhibit a quite dierent dynamics (see Section 6.).
71 f() f() 4.2. FUNDAMENTALS OF THE MODEL 6 a) b) LSW di LSW reac? = :? = :? =? = Figure 4.2: In a) the normalized PRDs of both limiting cases of the LSW theory are shown. In b) the normalized PRDs of four intermediate cases according to Eq. (4.2) are plotted [for comparison both LSWPRDs (solid lines) of Fig. a) have been added]. 8 GT LSW c=c R=R c Figure 4.3: Comparison of the equilibrium monomer concentration of a NC of radius R according to the exact [Eq. (2.23)] and linearized [Eq. (4.)] GT relation. Intermediate regime Using the parameterization? = R r =R?, where R r = D=k, White [8] derived an expression for the PRD in the intermediate regime between pure diusion and reaction controlled OR b(a + f() / (? + )(a ; ) (;c ; )? ) exp (4.2) a ; c a ; where the parameters are given by =[ba(a;2c);2(a;c) 2 ;bc? ]=(a;c) 2, =[bc(c+? ); (a ; c) 2 ]=(a ; c) 2, a =2=(2 + ), b ;3, c = ;=2, and =3+? + p (9 +? )( +? ). Here, the parameter a denotes the maximum allowed NCs size.
72 62 CHAPTER 4. GENERAL DESCRIPTION OF OSTWALD RIPENING In the above description, the quasistationary PRD depends on?, and thus changes shape during OR. Thus Eq. (4.2) is only valid, if changes within the distribution occur much more rapidly than changes in?. It should be noted, that in the limiting cases?! and?!eq. (4.2) reduces to the LSW limits Eqs. (4.5) and (4.8), respectively. In Fig. 4.2b the PRDs of the LSW theory are plotted as well as four PRDs characterized byvarious values of? according to Eq. (4.2). Distributions with parameters? & are essentially indistinguishable from the PRD of the reaction controlled limit. Interestingly, for small but nite? the relative contribution of NCs smaller than R? to the PRD rst decreases with respect to the LSW distribution for the diusion limited case. This property (not discussed in [8]) might be due to the approximations made for deriving f() in closed form and will be discussed in Section Local meaneld approach to diusion and reaction controlled Ostwald ripening As mentioned above, for nonvanishing volume fractions the LSW theory is no longer strictly valid simply because the longrange diusion elds start to overlap. As a result, the monomer concentration around one NC is inuenced by the presence of neighboring precipitates. Thus an appropriate framework for simulation studies of OR is a local mean eld description. The following derivation is in line with the VG approach and is aimed as an extension to the work of Reiss [82] and Reiss et al. [7, 72] towards a full coverage of the LSW theory. As in the single NC case, the starting point for this approach to model the evolution of coarsening NCs is to seek a solution of the stationary diusion equation r ~ 2 c(~r t) = dened in the multiply connected space outside the precipitated phase [equivalent to Eq. (4.)]. Considering an ensemble of N NCs, the BCs for the monomer concentration at each phase boundary c(~r )j j~r;~ri j=r i = ^c i are now a function of c and therefore have to be determined selfconsistently. Like in electrostatics, an exact solution to the stationary diusion equation subject to N BCs may be found by the method of mirror sources. Replacing the (innite) number of mirror sources inside the precipitates by an (innite) series of multipole moments at each center gives an equivalent solution. Thus the concentration eld can be expressed as a sum over the individual multipole expansions (with multipole moments M m) il c(~r )=c u + 4D NX i= X lx l= m=;l Yl m ( i i )Mil m j~r ; ~r i j l+ (4.22) using the common notation Yl m to denote the spherical harmonics. It should be noted, that in the case of a single isolated isotropic NC all but the monopole term Q = Y M vanish and Eq. (4.6) is retained. The actual boundary values ^c i can be derived by equating the reaction current [Eq. (4.3)] with the diusion current evaluated at the ith interface, ~ (i) (i) di = ~ reac, from which
73 4.3. LOCAL MEANFIELD APPROACH TO OR 63 immediately follows ^c i = D k ~ rc(~r ) j~r;~rij=ri ~e (r) i + c GT (R i ): (4.23) The multipole moments M m il can be obtained by integration of Eq. (4.22) over the (spherical) surface of the ith precipitate using the orthogonal properties of the spherical harmonics involved. However, in order to keep things simple, only monopole terms are considered, which is a reasonable approximation for small volume fractions of the second phase (usually the monopole approximation is acceptable as long as <: [83]). After some straightforward algebra (see Appendix B) one ends up with a coupled system of N linear equations for the N source strengths Q i = Y M i Q i = " 4DR2 i c GT (R R i + R?? i ) ; 4D NX j6=i Q j + R?? j~r i ; ~r j j j~r i ; ~r j j ; c u # : (4.24) Here, the dimensionless parameter? = D=(kR? ) denotes the degree of diusion and reaction control during ripening. In the case? =, i.e. the diusion controlled coarsening mode, Eq. (4.24) is equivalent to formerly derived expressions [39, 72]. The local meaneld character of this approach is clearly seen in Eq. (4.24), since the source strength of the ith precipitate is proportional to the dierence between its own equilibrium concentration and the superposition of the external concentration c u and the concentration elds caused by all other NCs. The evolution of individual precipitates is mainly determined by the diagonal elements of Eq. (4.24), whereas the odiagonal elements account for the coupling of NCs. Thus the onset of reaction control primarily reduces the absolute value of the source strengths, while additional modications of the NC coupling become only relevant for large?. More precisely, the inuence of reaction control on mutual NC interactions can not be neglected if D=k is of the same order as the average distance d between NCs. However, in the course of OR the NC density decreases, thus the ratio of both types of coupling decreases like =d. As other studies suggest [3], the correct treatment of odiagonal terms inuences the time behavior of the ensemble. It should be noted that in the limit!, i.e. j~r i ; ~r j j!, the LSW growth law is obtained. Within the monopole approximation, the concentration eld is given by c(~r ) ' c u + 4D NX i= Q i j~r ; ~r i j (4.25) and the individual source strengths Q i determine the evolution of the precipitates 4 R 2 i (t) dr i(t) = ;Q i : (4.26) V a dt Eq. (4.26) together with the diusion equation form a coupled system of dierential equations controlling the evolution of the precipitates. Considering the characteristic time scales
74 64 CHAPTER 4. GENERAL DESCRIPTION OF OSTWALD RIPENING one generally loses no information in neglecting the time derivative of the diusion equation. This is due to the fact that the time scale involved in the precipitate growth is usually much larger than that of the diusional accommodation of the impurity concentration to the existing precipitate pattern. 4.4 Numerical implementation Here, a short sketch of the numerical implementation will be given are more detailed discussion can be found in [82]. At the beginning of the simulation, geometrical (e.g. shape of basic simulation cell, assignment of physical properties of ensemble boundaries, like periodic, absorbing, or re ecting boundaries, respectively) and physical (materials parameters, NC size and space distributions) aspects have to be specied. In order to obtain dimensionless quantities, the following (to some extent arbitrary) transformations are performed: all lengths are scaled by the ensemble size L ens (in the case of a cubic geometry L ens is the size of the unit cell of the simulation) a supersaturation = (c ; c )=c according to VG is dened a time scale is introduced via sim = L 2 ens =(V adc ). Within the scaled system of equations, the only remaining explicit dependence on physical parameters is the capillary length R c. Since besides the N unknown quantities Q i also the BC c u has to be specied, one has to solve a linear system of equations P of dimension N +. Several choices for c u are possible: (i) via the closure condition Q i = Q ext (material conservation), where Q ext is an external source strength, c u is determined selfconsistently (ii) c u can be dened directly. In case (ii) the choice c u = c together with the linearized GT relation [Eq. (4.)] allows to transform R c =L ens into the time scale. Thus, in this special case, OR depends just on geometry (f~r i g fr i g), whereas all physical constants only inuence the time scale of coarsening. Note, that if not otherwise indicated, in simulations presented in this work the exact GT relation [Eq. (2.23)] has been used. Usually, the generation of the initial ensemble is to a large extent arbitrary. The simulation input, the NC density and mean radius, are by denition average values and thus do not provide any specication of spatial correlation between precipitates. A reasonable setting algorithm [82] starts by randomly distributing nonoverlapping spheres (halos) with a constant radius (R halo > R max ) throughout the simulation volume, i.e. the unit cell. Then the NCs are placed into the centers of the halos and their radii are chosen statistically according to a predened PRD. This procedure tries to mimic the nucleation of precipitates during IBS, since a new nucleus decreases the supersaturation of impurities in its vicinity and thus decreases the probability of a close second nucleus to come into existence. With respect to the generation of the initial ensemble the transfer of K3DLMC simulation results to the rateequation approach to OR seems to be a promising option [84] (see Chapter 6). Although there remains an ambiguity about the minimal NC size to be transferred, K3DLMC generated input data have the advantage, that they already characterize a coarsening system. If initial data have beenchosen solely statistically, the articial
75 4.4. NUMERICAL IMPLEMENTATION 65 a) IF IF2 Q Q b) Q Q c) Q Q Q Q Figure 4.4: Construction of basic unit cell for Ewald summation for various BCs of interfaces IF and IF2. In (a) both interfaces are reecting (i.e. prevent monomer ow out of the system), in (b) both interfaces are xed to c u, and in (c) IF is xed to c u, whereas IF2 is reecting. In each gure, the solid box denotes the physical NC ensemble, the dashed boxes contain auxiliary ensembles and the dotted box is the resulting unit cell for 3D Ewald summation. system will nevertheless evolve toward a state conform with the LSW or extended theories. This has been proven by Chen et al. [62], who showed that for homogeneous systems the LSW distributions represent attractors in the space of all possible distributions. The more articial the initial distribution the longer is the transient time this unphysical system needs to converge to the behavior of real systems. This may lead to bad statistics of the remaining independent precipitates. In the case of inhomogeneous systems, however, an unphysical choice of initial data may have a major inuence on the evolution of coarsening precipitates (see also Section 6.2) In OR simulations BCs deserve a closer investigation. For fundamental studies one wishes to use ensembles which are not distorted by boundary eects. Thus a natural choice are periodic BCs. As demonstrated earlier by other groups [39], Ewald's summation method provides an analytical way to incorporate =r interactions between precipitates in spatially periodic unit cells. However, as already pointed out, the description of ion beam synthesized NCs requires the correct treatment of a heterogeneous NC distribution as well as absorbing and reecting interfaces. For instance, in Si + implantation into a thin SiO 2 lm on a at Si substrate, the SiO 2 /Si interface absorbs the Si monomer supersaturation in SiO 2, because the bulk Si maintains the solidus concentration c at the interface. On the other hand, if the implanted impurities do not segregate on the surface or are nonvolatile, the surface prohibits any monomer ow out of the system and is thus equivalent to a reecting interface. Both BCs can be achieved by the proper use of mirror sources (see Fig. 4.4). While the 2D Ewald summation with respect to a unit cell containing mirror
76 66 CHAPTER 4. GENERAL DESCRIPTION OF OSTWALD RIPENING sources by Reiss et al. [72] allowed them to describe one absorbing interface (analogous to Fig. 4.4b), they remarked, that the second interface has not been treated correctly. This shortcoming is circumvented simply by a full 3D extension of the appropriately extended simulation cell. However, the Ewald summation method fails to treat =r 2 interaction terms [Eq. (4.24)], which are present in the case? 6=. But considering the eective screening by surrounding precipitates [2], the actual range of inuence of one NC is restricted and quantitatively described by the diusional screening length D [] given by Eq. (3.8). Based on this property of the system, Yukawalike interaction terms among the precipitates can be applied, i.e. the expression for the source strengths [Eq. (4.24)] is modied according to the substitutions j~r i ; ~r j j ;! expf;j~r i ; ~r j j=l scr g n = 2: (4.27) n j~r i ; ~r j j n Choosing for the Yukawa screening length l scr > D this model gives in the diusion controlled limit physically reasonable results comparable to results obtained by Ewald's summation method (for a discussion, see Section 4.5). Additionally, it provides a method to incorporate higher order interactions. Since the interaction matrix is calculated once at the beginning of the simulation and because of the increase of D (t) during the ripening process, the initial value for l scr has to be chosen high enough to ensure l scr > D during the whole simulation. One shortcoming of this approach is the relative increase of damping during the simulation due to the increase of the average NC distance d. An improved, but computationally more extensive approach would be to keep the ratio d=l scr xed by subsequently updating the interaction matrix for an appropriately increased screening length. In practice, only a nite number s of surrounding shells of unit cells can numerically be included to achieve quasi3d periodic BCs. For the simulation results presented in the next section s =6has been used. The simulation is discrete in time, i.e. at each time step t rst the linear system of equations (4.24) extended by one equation xing c u is solved. Then the change in radius due to the actual value of the source strengths is evaluated with the help of a linear approximation of Eq. (4.26). With the new radii obtained the procedure is repeated. The time interval t can be chosen to some extent arbitrarily. However, it should be noted, that special care has to be taken not to violate material conservation. This situation easily arises, if an almost dissolved NC would lose in the next time interval more material than it contains. An eective solution is rst to check all NCs which will dissolve, and in a second step to adjust their computed source strengths by their total remaining material content. For further details concerning second order corrections see [82]. Combining Eqs. (3.8), (4.6) and (4.7) one obtains D (t) / t =3 in the asymptotic limit.
77 4.5. SIMULATION OF DIFFUSION AND REACTION CONTROLLED OR Computer simulation of diusion and reaction controlled Ostwald ripening In this section the evolution of homogeneously distributed ensembles of NCs is simulated for various values of?. In particular, the parameter set? = f g is used to study the ripening regimes of pure diusion control, intermediate mixed processes, and reaction control, respectively. Typical ensembles consist of up to several thousand precipitates located randomly in a cubic unit cell and periodic BCs are applied in three dimensions. As a rst check of the validity of Yukawalike screened interactions [Eq. (4.27)], simulations have been performed for? =. Starting with an ensemble described by the stationary PRD of the diusion limited case [Eq. (4.5)] no deviations have been observed with respect to the evolution of the number of particles, N(t), and the critical radius, R? (t), as compared to numerical results using Ewald's summation method. In particular, the time dependences of the critical radius and the NC density are observed to be in accordance with the LSW predictions [Eqs. (4.6) and (4.7)]. However, the proportionalitybetween these quantities and the time t depends on the choice of the screening length l scr. This is illustrated for the evolution of R? (t), where the relative dierence to the analytical result is given by the coecient R? 3 (t) ; R? 3 (t )= R? 3 (t ) di t: (4.28) In the case? = the results are shown in Table 4. for four dierent values of l scr and Ewald's summation method. Due to nite volume eects mentioned above, in general the observed coarsening rates are larger than the value = predicted by the LSW theory. This increase is systematic with decreasing l scr andcanbephysically understood by noting, that the Yukawalike screening causes a damping of the mutual interactions. The implication of reaction control, i.e.? 6=, on the ripening kinetics is pointed out for a simple D model system in Fig A plot of the scaled concentration eld is shown for two precipitates with dierent radii in an eective eld c u =:2c, e.g. generated by other clusters of an ensemble not visible in Fig For this pair of NCs the concentration eld is evaluated using Eqs. (4.22) and (4.24) with arbitrary materials parameters. Obviously, the larger the value of? the weaker is the gradient ofthe concentration eld. From the point of view of simulations, for a xed diusion coecient D the higher the parameter? is chosen, the slower will the evolution of the system takes place. This is Table 4.: Relative coarsening rate [see Eq. (4.28)] of precipitates during diusion controlled ripening for four dierent ratios of the Yukawa screening length l scr [see Eq. (4.27)] to the system size L ens and in the case of using Ewald's summation method (ESM). l scr =L ens ESM
78 68 CHAPTER 4. GENERAL DESCRIPTION OF OSTWALD RIPENING scaled concentration scaled location scaled concentration scaled location scaled concentration scaled location Figure 4.5: Scaled monomer concentration eld of two interacting NCs embedded in a global eld c u =:2 c for three dierent degrees of diusion and reaction control. From left to right, the NC pairs are characterized by? = f g. The equilibrium concentrations c GT are indicated by the corresponding columns. based on the fact that individual IAs have to overcome a nite reaction barrier, which obviously hinders their redistribution. This eect is clearly seen in Eq. (4.24), because for high values of? the source strengths are roughly proportional to =?. In order to compare systems characterized by dierent values of? it is useful to scale the ripening time by a time constant (? ). Since analytical expressions for characteristic ripening times [Eqs. (4.6) and (4.9)] are only known in the LSW limits [5], a reciprocal interpolation should serve as a reasonable approximation for the intermediate range = 8 9 R? R 3 "? R R? 3 # di : (4.29) Thus for? the ripening time scale is proportional to? di, which implies that an ensemble characterized by? = ripens approximately times slower in real time than it would in the diusion controlled regime. The dependence of the evolution of homogeneous ensembles of precipitates on the degree of diusion and reaction control is shown in Fig In each of six runs of a series of simulations the coarsening of N = 36 nanoclusters has been studied, where their initial PRDs obeyed the stationary PRD of the diusion limited case. The volume fraction of the precipitated material is = :76, with a mean radius R = :5nm at t =. In the logarithmic plot of Fig. 4.6a the averaged remaining number of ripening precipitates is shown in the cases? = f g. In the case? =, i.e. pure diusion controlled ripening, N(t) tends to be proportional to =t as predicted by the LSW theory. The ensembles characterized by? = and? =, respectively, exhibit a stronger time dependence. In particular, in the limit?!, coarsening systems are found to have a time dependence N(t) / =t 3=2. The evolution of the critical radius is pointed out in Fig. 4.6b. Depending on?, the time dependence for t for R? (t) lies in between the two asymptotic results R? (t) / t =3 for diusion limited coarsening and R? (t) / t =2 for the reaction limited process, respectively. The dierences in the ripening behavior for the three ensembles are also visible in their PRDs. In the case? =, the PRD does not change its scaled shape during the
79 N R? (nm) 4.5. SIMULATION OF DIFFUSION AND REACTION CONTROLLED OR 69 a) b) 5 5? =? =? = / =t / =t 3= ? =? =? = / t =3 / t =2 5 t () 2 5 t () 2 Figure 4.6: Time dependence of the number of coarsening particles (a) and the critical radius (b) in the time interval t 2 for the three ensembles discussed in the text. For comparison, the corresponding analytically derived results (Section 4.2.2) for the two limiting cases of diusion and reaction controlled ripening are plotted as well. t = t =5 t =5.2 N=Ntot Figure 4.7: Evolution of the PRD in the case of diusion controlled OR (? = ). Here, the normalized number of NCs belonging to a size interval is plotted versus the normalized radius = R=R?. For comparison the two stationary PRDs of the LSW theory are included (dashed: diusion control, dotted: reaction control). simulation in accordance with the LSW theory. This can be seen in Fig. 4.7, where for comparison also the analytically derived LSW distributions [Eqs. (4.5) and (4.8)] are shown. As expected, the shape of the PRD starts to deviate from this specic initial choice for systems having a non zero degree of reaction control. This is visible in Fig. 4.8, where the evolution of the PRD in the case? = is shown. With increasing reaction control, the simulated distribution becomes broader and less peaked than in the pure diusion limited case. Especially the fraction of NCs with < starts to increase with respect to the PRD of the diusion limited case. This behavior is not predicted by Eq. (4.2). Moreover, the
80 7 CHAPTER 4. GENERAL DESCRIPTION OF OSTWALD RIPENING t = t =5 t =5.2 N=Ntot Figure 4.8: Evolution of the PRD for competing inuences of diusion and reaction controlled OR (? = ). Additionally to the stationary PRDs of the LSW theory (dashed: diusion control, dotted: reaction control), the PRD for? = according to Eq. (4.2) is plotted (dasheddotted line). t = t =5 t =5.2 N=Ntot Figure 4.9: Evolution of the PRD in the case of (basically) reaction controlled OR (? = ). scaled maximum size of the precipitates increases, as may be seen more clearly in Fig. 4.9, where coarsening is shown for? =. Obviously, in the limit?!, the PRD is found to match the stationary PRD of the reaction controlled limit derived by Wagner [5]. The coarsening of precipitates can also be monitored with respect to the evolution of the width! of the PRD dened as!(t) =q (R= R(t) ; ) 2 : (4.3) The time behavior of! can be seen in Fig. 4. for three values of?. After a coarsening duration of a few time constants (? ), also systems being initially in an articial state reach a stationary OR stage. This observation is in accordance to ndings of Chen et al. with respect to attractor states in the space of size distributions [62]. However, as already indicated in Fig. 4.8, the simulated PRD for? =is signicantly broader as compared
81 Q (=s) Q (=s) Q (=s)! 4.5. SIMULATION OF DIFFUSION AND REACTION CONTROLLED OR ? =? =? = t () 5 Figure 4.: Averaged widths! of the PRDs for a set of ensembles characterized by? = f g, which possess initially the LSW size distribution of diusion control. The two dotted lines denote the analytic results for the stationary PRDs of the diusion and reaction controlled limit of the LSW theory, which read! di = :25 and! reac = :333, respectively. The dasheddotted line is obtained from the analytic form of the intermediate PRD [Eq. (4.2)]. 4? = 5? = 3? = Figure 4.: Source strengths Q i of precipitates plotted versus the scaled radius = R=R? for the set of NC ensembles characterized by? = f g after coarsening for a time t = 5. Note that positive source strengths belong to shrinking, whereas negative ones belong to growing precipitates. to the prediction of White [8]. Additional insight into the physics of OR is gained by plotting the source strengths Q i versus the scaled radius (t) =R=R? (t) for the three characteristic ensembles of coarsening precipitates (see Fig. 4.). While in a global meaneld theory the source strengths have to lie on a single curve, the scattered data for particular cluster sizes reveal the local
82 72 CHAPTER 4. GENERAL DESCRIPTION OF OSTWALD RIPENING interaction character of the simulation approach. The concentration eld at the site of a precipitate depends considerably on the specic conguration of neighboring precipitates. As can be seen in Fig. 4. the eect of mutual interactions due to overlapping diusion elds decreases with increasing degree of interface controlled OR. This can be understood due to the weaker concentration gradients between neighboring NCs of dierent sizes, since for basically reaction controlled OR the detailed nearestneighbor conguration tend to be smeared out by the fast diusion. Another interesting point is the size of the NC characterized by the largest source strength. In the diusion controlled limit there is a linear dependence of the source strength with respect to the NC size. Thus precipitates about to vanish have the largest detachment rate. However, if reaction control becomes important, intermediate shrinking precipitates show a larger dissolution potential than very small ones. Within the global meaneld approximation the maximum source strength Q max can be determined by combining Eqs. (4.2) and (4.26), taking the derivative with respect to, and solving the equation 2 + 2? ;? =,from which follows Q max =4Dc R c +2? ; 2 p? (? +) for = p? (? +);? : (4.3) In the reaction controlled limit, i.e.?!, NCs of half the critical size have the largest monomer detachment rate, which, in turn, tends to zero. The fact, that within this local meaneld description for nite? the maximum dissolution rate is associated with a nite precipitate size, interesting consequences arise with respect to the validity of Eq. (4.2). The deceleration of dissolution of NCs being smaller than the size corresponding to Q max causes them to remain slightly longer alive. Thus the consequence of this small retardation of dissolution should be a tendency of accumulation of small NCs. This, in turn, explains the relative abundance of small NCs in the simulated PRD with respect to the PRD of the diusion controlled limit of the LSW theory and is in clear contrast to the prediction of Eq. (4.2). Thus it can be concluded, that the approximations made by White [8] for?. 5 deserve a closer inspection. All of the results presented above have been obtained on the assumption, that the reaction rate k does not depend on size. However, it is reasonable to assume, that the monomer ux through the precipitate/matrix phase boundary is a function of the local curvature. A more detailed study of these eects remains to be given in future approaches. Essentially all experimental data for aging of secondphase particles are in accordance with the time dependence of diusion limited OR [85, 6]. Good candidates for the observation of reaction controlled coarsening are solidsolid systems, which possess incoherent phase boundaries and/or very high diusion coecients for impurity monomer diusion. Recently, evidence has been reported for 2D ripening of 3D selfassembled quantum dots located on a substrate according to the reaction controlled limit [86]. In this experiment the density of CdSe quantum dots grown on ZnSe showed a time dependence of n(t) / t ; rather than n(t) / t ;3=4 as would be expected for ripening in the diusion controlled regime for this geometry [3].
83 Chapter 5 Nanocluster formation and evolution during highdose ion implantation The formation of secondphase domains in systems transferred to the thermodynamically metastable region of the phase diagram is usually described by classical nucleation theory (see Section 2.3). As pointed out earlier, the application of this standard theory to IBS is not straightforward, because in this process precipitation is due to a depth and timedependent supersaturated solid solution of IAs. Furthermore, for nucleation occurring during implantation, a correct treatment should take into account the eects of CM, not to mention the inuence of radiation damage, e.g. the depthdependent interaction of IAs with point defects and defect clusters. This Chapter rst presents K3DLMC results of simplied (neglecting CM) simulations of NC formation at constant and varying implantation conditions and discusses corresponding experiments for the AuSiO 2 system [87]. Then, in the last section, the eect of CM on the state of a single NC is described and consequences of CM on the evolution of NC ensembles are pointed out. 5. Nucleation and growth of NCs at constant implantation conditions General considerations The basic physical stages of IBS briey introduced at the beginning of Chapter 2 can easily be identied in K3DLMC simulations. Fig. 5. presents results of a model simulation of a nite homogeneous system, where monomers have been added at a constant (volume) deposition rate up to a total dose of F. For constant (implantation) parameters the evolution of the system is governed by: Accumulation/Saturation (I): Immediately after the start of ion deposition, the rst IAs can be found as (dissolved) monomers. Depending mainly on the substrate temperature, the implanted atoms either remain "frozen" in their nal position, or they may diuse through the substrate. Initially, the concentration of monomers 73
84 74 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION a) b) c nuc n c R? nuc R? I I II III.5 F=F.5 F=F Figure 5.: K3DLMC simulation of homogeneous phase transformation indicating the physical regimes of accumulation/saturation (I), nucleation (II), and growth (III). In a) the evolution of the monomer concentration c and the NC density n is shown. The eective concentration threshold for nucleation c nuc is indicated for clarity. In b) the (discrete) nucleation rate I is directly compared to the critical radius R? given by the inverse GT relation [Eq. (4.)]. c increases linearly with time (or, equivalently, with uence F ). In the case of sucient impurity mobility,asc increases further and reaches the solubility threshold (saturation is given by = ), small agglomerations of IAs (i.e. dimers, trimers,...) start to form by thermal uctuations. The appearance of these subcritical nuclei slows down the increase of c. Supersaturation/Nucleation (II): Supersaturation sets in, when c exceeds the solubility limit (i.e. > ). By thermal uctuations some subcritical nuclei start to grow beyond the critical size i? forming stable precipitates. At later times, these supercritical precipitates act as sinks for diusing monomers, which reduces the volume available for nucleation [7]. Despite the continuing deposition of IAs c starts to decrease, thus eventually dropping below the threshold for nucleation. Further NC formation becomes very unlikely. Growth (III): No additional NCs are formed and the existing ones grow by attachments of newly implanted IAs rather than competitive ripening. Hence, the density of precipitates essentially remains constant, while the concentration of monomers further decreases. In Fig. 5.b the nucleation rate I is given by the derivative of the NC density n with respect to the implanted uence, which is proportional to t (the discrete implementation I = n=f of the results of this single run for a nite system explains the observed oscillations of the nucleation rate).
85 5.. NC FORMATION AT CONSTANT IMPLANTATION CONDITIONS 75 T> T T< j < j j > Figure 5.2: Scheme of parameter range of ion ux and implantation temperature of K3DLMC study of NC formation during ion implantation. The appearance of the three stages relative to the implanted uence depends on the implantation parameters and the materials constants. For instance, for very low uences the monomer concentration might completely remain below the nucleation threshold. For very low T imp the monomer mobility might be negligible, thus, although a considerable degree of supersaturation might have been reached, nucleation is essentially retarded to a subsequent heat treatment. Furthermore, due to the depthdependent deposition prole, the above described sequence of stages sets in rst around R p and shifts later on gradually to the tails. Simulation of NC formation during implantation In order to understand the evolution of NCs during implantation, the dependence of the (depthdependent) size distribution on the main implantation parameters, i.e. the implantation temperature T imp and the ion current j, was studied qualitatively for a xed ion energy E (see Fig. 5.2). In a series of simulations for a xed ion uence F 3 a ;2 fcc (in the case of Co implantation into csi, this would correspond to a uence of F 6 cm ;2 ), the NC formation was studied at three dierent implantation temperatures ft < T T > g for a xed ion ux j and at three dierent ion uxes fj < j j > g for a xed T imp. The three ion currents fj < j j > g diered one another by one order of magnitude, whereas the implantation temperatures were chosen according to the K3DLMC parameters fcc = f2 3 4g. Here a few comments should be made concerning the corresponding physical values of the simulation parameters chosen for this general study. The ion current in the case of the reference parameter pair was j (T j) =2:44 ;4 a ;2 fcc ;. Since the physical time scale of a MCS is temperaturedependent [see Eq. (3.2)], simulations for constant j at dierent T have to be specied with respect to a particular value of the activation energy for diusion E A. Taking for this study (the arbitrarily chosen, but typical values) E A = :5eV and E S = :5 ev, the simulation currents are related approximately by (in units of a ;2 fcc ; ): j (T< j) : j (T j) : j (T> j) =7::(=7). It should be noted, that the higher E A the higher are the ratios of the simulation currents normalized with respect to a MCS. The corresponding physical ion currents, however, depend still on the preexponential D of the diusion
86 76 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION (T < j) (T j > ) (T j) (T j < ) (T > j) Figure 5.3: K3DLMC simulation results of NC formation during implantation as recorded immediately at the end of ion deposition. All NCs are represented as spheres (see Fig. 3.4) and the blue (grey) scale is chosen according to their size (within each gure the blue (grey) scale increases with size). constant. In a simulation volume of size fcc unit cells (about :7 7 lattice sites) IAs have been deposited symmetrically according to a Gaussian with R p = 256 a fcc and R p = 75 a fcc. For this particular series of simulations reecting BCs have been applied at z =, whereas the opposite boundary acts as an absorbing interface. However, as the results to be presented will indicate, this specic choice of BCs has no pronounced inuence on the nucleation results due to diusional screening eects and the restricted diusion length during implantation (it will be shown in Section 6.2, however, that BCs do have an inuence during long time annealing.). In this simulation series CM was not included. For the ve parameter pairs f(t < j) (T j > ) (T j) (T j < ) (T > j)g Fig. 5.3 shows the corresponding NC distributions. Increasing the implantation temperature or decreasing the For nonperiodic BCs in the z direction used in this work, positive depths point totheright.
87 n (=a 3 fcc )! 5.. NC FORMATION AT CONSTANT IMPLANTATION CONDITIONS 77 a) b) E3 E4 (T j) (T > j) (T j <) (T < j) (T j >) (T j) (T j < ) (T j > ) E F=F F=F Figure 5.4: In a) the evolution of the NC densities (normalized with respect to the simulation volume) for the ve parameter pairs is shown. In b) the evolution of the widths! of the PRDs is plotted. Here, the widths of the LSW distributions (see Fig. 4.) have been added for comparison. ion ux with respect to the reference parameter pair results in similar NC distributions. This observation is also reected in Fig. 5.4a, where the evolution of the NC density in the rst half of the respective implantations is shown. The evolution of the width! [see Eq. (4.3)] referring to three parameter pairs can be seen in Fig. 5.4b. Experimental observations and discussion The IBS of Au nanoclusters in SiO 2 is wellsuited for fundamental precipitation studies, because (i) Au does not tend to form an oxide or silicide [88] (Au atoms are chemically inert with respect to the constituents of the host material), (ii) Au is observed to precipitate during the implantation stage, and (iii) no collective shift of the implanted IAs inuences the NC formation. 2 The temperature dependence of Au nanocrystal formation in fused silica can be seen in Fig Here, Au NC distributions recorded immediately after 2.75 MeV Au + implantations (projected range about.9 m) at current densities of approximately A/cm 2 are shown. The K3DLMC simulations for a xed ion current presented in Fig. 5.3 reproduce these observations. This qualitative dependence of the NC distribution on T imp has been reported also for other NC/substrate systems [89]. For a xed T imp the increase of the NC density with increasing ion current has been observed, for instance, in the case of Co implantation into Si [6]. Both simulated and experimentally observed NC distributions can be understood in terms of the classical nucleation theory presented in Section 2.3 (neglecting for a moment inhomogeneities due to the implantation prole). However, in contrast to standard studies 2 For instance in the case of Ag implantation into fused silica at elevated temperatures, a net movement of the IAs towards the surface has been observed [6].
88 78 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION Figure 5.5: Crosssection TEM micrographs of 2.75 MeV Au + implantation into fused silica for a uence of :5 7 cm ;2 (from Ref. [87]). Figs. a) { c) refer to implantation temperatures of 6 C, 4 C and room temperature, respectively. of nucleation phenomena starting with a particular supersaturation level, here in addition the dynamical concentration increase has to be considered. Constant implantation current: Given a specic supersaturation, Eqs. (2.7) and (2.) state, that the nucleation probability increases with increasing temperature (Boltzmannfactor). Therefore, the decay velocity of a supersaturated state also increases with increasing temperature (transient eects). While for a xed implantation current the supersaturation increase is temperatureindependent, the decay of the metastable state into precipitates does depend on T imp. Thus an increased thermal activity leads for high T imp to nucleation on a lower supersaturation scale, with a correspondingly larger critical NC size. After growing beyond the critical size, a NC acts as permanent sink for diusing monomers, thus decreasing the monomer concentration in its vicinity. The ratio of the deposition to diusion rate then determines the range of the eective depletion zone around each NC, where the nucleation of an additional precipitate is unlikely. Since both the critical size of nucleation increases and diusion becomes more eective with increasing temperature, less stable NCs will be formed, onto which the subsequently implanted impurities condense (see Figs. 5.3 and 5.5).
89 5.2. NC FORMATION AT VARYING IMPLANTATION CONDITIONS 79 Constant implantation temperature: For a given T imp it is obvious, that supersaturation increases more slowly as j decreases. This implies, that the systems remains the longer at a specic supersaturation level the lower the ion ux is (for constant temperature the time lag of nucleation depends on ). Thus on the average larger NCs are nucleated for low j than for high j. The corresponding ratio of deposition to diusion denes again the range of the depletion zone around a successful precipitation. Since here the size of the depletion zone, where no additional nucleation is expected, is proportional to =j, the smallest NC density is observed for the lowest ion current (see Fig. 5.3). As Fig. 5.4a indicates, the NC density essentially remains constant after the end of the nucleation stage. During the ongoing implantation all NC can be expected to grow approximately at the same rate, because both the deposition and NC density distributions are similar (Gaussianlike). This is reected in the evolution of the widths of the PRDs shown in Fig. 5.4b, which tend to decrease during the growth stage. From the viewpoint of homogeneous nucleation similar NC size distributions can be obtained either by increasing the implantation temperature or by decreasing the ion ux (or vice versa) (see Fig. 5.3 and also Fig. 5.6 below). This behavior suggests, that the mean NC size can be described according to a function f(g=d(t )), where D is the (strongly temperaturedependent) diusion coecient and G the generation rate of IAs per unit volume, which is proportional to j. No unique form of f could be deduced from the K3DLMC results, which might be related to the depthdependence of G. The ratio G=D also explains the observed vertical spread of the nucleation region. A small deposition to diusion ratio prevents a signicant increase of the impurity concentration in the very tails of the implantation prole. In this case the nucleation region lies close to R p (compare microstructures in the cases (T < j) and (T > j) of Fig. 5.3). 5.2 Nucleation and growth of NCs at varying implantation conditions Simulation of NC formation at varying implantation conditions Most studies of IBS of NCs reported so far have been conducted for constant implantation parameters (excluding here multienergy implantations). Therefore, K3DLMC studies have been performed in order to give predictions of NC distributions to be expected for a controlled variation of parameters during implantation. Fig. 5.6 shows simulation results, where one parameter (either T imp or j) has been (instantaneously) changed for the second half of the implantation. The results for the changes (T < j)! (T j), (T j)! (T < j), (T j > )! (T j), and (T j) $ (T j > ) not shown here yield qualitatively similar results with respect to the direction of the parameter variation. Fig. 5.7 shows the NC density evolution during implantation and relates the observed bimodal PRDs to the onset of a second nucleation stage after an appropriate parameter change.
90 8 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION.4 N=Ntot.3.2. R= R R= R 2 3 R= R 2 3 R= R Figure 5.6: K3DLMC simulations of NC formation for the following changes of parameters at F = F =2 (from top to bottom): (T > j)! (T j), (T j)! (T > j), (T j < )! (T j), and (T j)! (T j < ). All NCs are represented as spheres (see Fig. 3.4). The corresponding NC size distributions are shown from left to right in the lower row. The predicted bimodal PRD (for the implantation sequences (T > j)! (T j) and (T j < )! (T j), respectively) has not previously been observed. Therefore, a set of experiments was conducted to verify these results. Experimental observations and discussion The TEM micrographs of Fig. 5.8 show the eect of changing T imp during Au + implantation into SiO 2. Clearly, the size distribution depends on the sequence of the temperature change. A rather broad PRD (possibly the overlap of two individual distributions as suggested by
91 n (=a 3 fcc ) 5.2. NC FORMATION AT VARYING IMPLANTATION CONDITIONS 8 2E4 E4 (T > j)! (T j) (T j)! (T > j) (T j <)! (T j) (T j)! (T j <).5 F=F Figure 5.7: Evolution of the NC densities for a parameter variation during implantation. the simulation results of Fig. 5.6) is obtained by decreasing T imp in the second implantation period. The change in size distribution due to a signicant change in j has not been measured in this experiment. Like in Section 5. the simulation results of Fig. 5.6 can be explained in terms of classical nucleation theory. For a given monomer concentration c the transition to a lower temperature increases the eective supersaturation, which, in turn, corresponds to a smaller critical radius R? [Eq. (2.)]. Furthermore, due to the larger ratio G=D, the eective monomer ux to the NCs is reduced, which causes an increase in c. Thus c might now again exceed the nucleation threshold and a second generation of NCs can form leading to a bimodal size distribution. On the other hand, by increasing T imp during implantation, a narrow PRD is observed with very tiny NCs missing. A reasonable explanation for this behavior is the corresponding shift of R? (the higher temperature increases the monomer ux to the NCs, thus c decreases), which can be so large, that previously formed NCs are now smaller than the critical size and thus dissolve. Variations in the ion current j cause changes in the ratio G=D opposite to the respective temperature changes. Like in Section 5. increasing (decreasing) j during implantation results qualitatively in the same microstructure as decreasing (increasing) T imp. Considerable changes of the implantation parameters can lead to even more dramatic eects. For instance, if a Au + implantation into SiO 2 at 6 C is followed by a second implantation at room temperature, no large Au precipitates, which have been certainly formed in the rst part of the experiment (see also Fig. 5.5a), can be detected [5]. Rather, the resulting NC size distribution resembles the distribution obtained by the experiment, where the complete uence was implanted at room temperature (see also Fig. 5.5c). Therefore it can be concluded, that in the experiment shown in Fig. 5.8a the previously formed NCs probably decreased in size by ballistic losses during the second implantation step concurrently with the development of new NCs precipitating from the supersaturation. Thus CM, which will be discussed in the next Section, might prevent the
92 82 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION a) b) c) T imp : 6 C ;! 25 C d) T imp : 25 C ;! 6 C N=Ntot N=Ntot diameter (nm) diameter (nm) 8 Figure 5.8: TEM micrographs for 2.75 MeV Au + implantation into SiO 2 : a) 3 6 cm ;2 at 6 C+3 6 cm ;2 at 25 C, b) 3 6 cm ;2 at 25 C +3 6 cm ;2 at 6 C (from Ref. [87]). The corresponding size distributions are shown in Figs. c) and d). formation of a clearly separated doublepeaked PRD. 5.3 On the inuence of collisional mixing For systems, where NCs are forming during implantation, the continuous ion bombardment not only causes damage to the substrate, but also interacts with previously formed precipitates. For each impact in a NC by a decelerating ion or an associated recoil, IAs may be knocked out and deposited in the surrounding matrix according to a distribution function. This has not been taken into account in the simplied procedure of ion deposition used for the simulations described in the previous two sections. A promising approach to describe irradiation inuences on the NC evolution is the concept of CM briey introduced in Section 3.6.
93 5.3. ON THE INFLUENCE OF COLLISIONAL MIXING Collisional mixing of a single nanocluster K3DLMC simulation and results In order to obtain a qualitative understanding of the eect of CM, in a series of simulations similar to the determination of the GT relation in the pure thermal case (see Section 3.5.3), the steadystate monomer concentration c as a function of NC size is studied in the presence of temperatureindependent ballistic jumps. 3 For this isothermal series of simulations (for fcc = :75) the mixing length (an isotropic displacement distribution / expf;r=g is assumed see also Section 3.6) as well as the number of displacement attempts per IA per MCS is varied. In the following, will be given in units of [ ; ], where denotes the duration of one MCS [see Eq. (3.2)]. Regardless of the chosen value of, due to the lattice nature of the model the smallest possible discrete displacement r if = j~r i ; ~r f j is given by r = ( p 2=2) a fcc (i.e. a nearestneighbor displacement) in the case of a fcc lattice. Since the continuously chosen displacement length is projected onto the lattice, 4 the minimum radial distance of a successful jump attempt is r m = :35 a fcc p :25 2 +: a fcc causing a nearestneighbor displacement of length r. Within the K3DLMC method the length of a displacement is determined by r = ; ln w, w 2 [w ], where the cuto parameter w corresponds to a maximum distance of a ballistic jump. For the simulations to be presented in this Section the (arbitrarily chosen) cuto value w = ;6 has been used. Therefore, the probability of a discrete displacement of length r if is given by r<rm P = P(r! r if )( ; C f ) r r m (5.) where the projection operator P determines the nal lattice site ~r f. The last factor in Eq. (5.) takes into account that a displacement to an occupied lattice site (i.e. C f = ) is not performed. In the case of a fcc lattice Fig. 5.9 shows the normalized displacement distributions for three mixing lengths. In general, the assumed exponentially decaying displacement distribution for jump attempts will dier from the (continuous) distribution of performed jumps, which cause discrete displacements within the K3DLMC model. Fig. 5. shows the dependence of the steadystate monomer concentration on the NC size for various mixing lengths and mixing intensities. Obviously, also in the presence of competing dynamics a GTlike behavior [see Eq. (2.23)] is observed c (CM) (R) =c (CM) exp (R (CM) c R ) : (5.2) 3 Note, that in this study for each simulation the number of IAs within the simulation volume is kept constant. This corresponds to irradiating a NC consisting of impurities of type A with ions of type B. 4 The nal lattice site of a displacement attempt is determined by the coordinate transformation ~r f (r )! ~r f (x y z) and subsequent rounding to the next nearest integers, i.e. projection onto the next nearest lattice site. If ~r f belongs to the shifted second fcc lattice (see Fig. 3.), this jump attempt is discarded and, retaining r, a new pair ( ) ischosen.
94 c (=a 3 fcc ) 84 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION ~P. E2 E3 E4 E5 E6 E7 +? b b +? +? b? ++? b b? + +? b b b?? b??? ++? b b b b b b b? ?? b b?? b b b bb? + +????? b b b b b b?? ++?? b b b bb b b???? b b b b b b +?? b? bbb b b b bb?????? r m r r (a fcc ) = :25 a fcc + = :375 a fcc? b = :5 a fcc b bbb b b b b b b b b bb b b b b b bb b b b bbb b Figure 5.9: For three values of the normalized radial distributions ~ P of discrete displacements are plotted for CM simulations of a single NC of radius R 4:75 a fcc. The underlying continuously chosen displacement distances (r r m ) of these successful ballistic jumps have been included (solid lines). Furthermore, the distance r of a nearestneighbor jump is indicated. E3 E4. = 5 ;3 = = 5 ;4 ; ;.2.3 =R (=a fcc ).4.5 Figure 5.: For isothermal conditions ( fcc = :75) the GTlike c(r) behavior is shown for various mixing parameters (: = :25 a fcc, : = :375 a fcc, 4: = :5 a fcc ). For comparison results for pure thermally activated processes ( = ) are added [dotted lines from bottom to top: fcc =(:75 :5 :25) see Fig. 3.8b]. However, as compared to the pure thermal case (see Fig. 3.8), in addition to an overall solubility increase c (CM) = c (CM) ; c also the eective capillary length R c (CM) changes as a function of the CM parameters. An analysis of the eect of mixing can be done by determining the slope (i.e. R c (CM) ) and the intersection in the limit R!(i.e. c (CM) ) employing leastsquare ts. Table 5.
95 5.3. ON THE INFLUENCE OF COLLISIONAL MIXING 85 summarizes the simulation results. As one would intuitively guess, the higher the mixing intensity, the larger is the solubility increase, whereas simultaneously the capillary length decreases. For a xed value of, the results depend furthermore on the mixing length. In real systems the mixing length of an atomic component X is xed with respect to irradiation by ions Y ; at a given energy E. The mixing intensity depends then on the irradiation ux. For instance, assuming a displacement probability / expf;r=g a t to TRIM (SRIM) calculations of 5 kev Co + irradiation of a thin CoSi 2 layer buried in Si yields a mixing length :28 nm :52 a fcc with respect to Co displacements [9]. It should be noted, that Soisson et al. [9] have performed similar simulations for a bcc binary alloy in an essentially twodimensional model (system sizes up to 8 8 bcc unit cells). Restricting their ballistic jumps to nearestneighbor XY exchanges, they also derive a GTlike c(r) relation. However, although an overwhelming fraction of successful ballistic jumps is to nearestneighbor sites (in the regime. a fcc, see Fig. 5.9), the tails of the displacement distribution have a considerable inuence on the (dynamical) equilibrium conditions (see Table 5.). According to an idea of Martin [72] the eect of CM can be approximated by assigning a higher temperature T (CM) >Tto the system. Assuming that the changes in the observed capillary lengths with respect to the pure thermal case are completely due to a higher temperature (i.e. R c (CM) = R c T=T (CM) = R c (CM) fcc = fcc ), Fig. 5.a shows the corresponding results for the solubilities c (CM). Since the simulation data are located far o the theoretical solubility curve [Eq. (3.4)] the assumption of Martin does not explain the observed decrease of the capillary length. Nevertheless it is interesting to determine an eective temperature on the basis of the solubility increase rather than the change in R c. Using the relation (e) fcc = ; ln(c (CM) =A fcc )=B fcc [see Eq. (3.4) and Table 3.6], which with respect to Fig. 5.a corresponds to shifting the observed solubilities on isoconcentration lines onto the solubility curve, Table 5.2 lists the relative temperature changes. For instance, the solubility increase in the case of the highest mixing eciency ( = 5 ;3 ;, = :5 a fcc ) corresponds to a pure thermal system, where the temperature is increased about a factor.5. Table 5.: Analysis of GTlike behavior of CM of a single NC shown in Fig. 5. (the uncertainty of the last given digit is indicated in parenthesis). For comparison, the respective results for the capillary length and the solubility in the pure thermal case ( = ) derived according to Eqs. (3.6) and (3.4) are added. ( ; ) 5 ;3 5 ;4 (a fcc ) R (CM) c (a fcc ) (4).86(3).32(2) 2.88(6) 2.32(3).58(5) c (CM) ( ;3 =a 3 fcc )..69().8() 3.79(2).8().28().47()
96 c (CM) (=a 3 fcc ) 86 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION a) b). E2 E3 E expf;6 fcc g GT (CM) fcc (CM) J ; NJ N = :5 ; = :5 ; A (a 2 fcc ) Figure 5.: In a) the solubilities (intersections in the limit R!, 'GT') are plotted versus the eective temperatures as determined by (CM) fcc = fcc R c (CM) =R c. In b) the dierence between the average number of broken bonds N J of NCs with or without CM is plotted versus the average surface area A =4R Assuming an unchanged temperature the solubility increase can also be interpreted in terms of an eectively reduced binding energy. In the absence of CM according to Eq. (3.4) on the average B fcc = 6 nearestneighbor bonds J have to be broken for an IA to go into solution. Under irradiation, this number is supposed to decrease, i.e. B fcc! B fcc ; B fcc, because due to the ballistic assistance less bonds have to be broken thermally. Writing the CMinduced solubility increase as c (CM) = c exp f;(b fcc ; B fcc ) fcc g = c exp fb fcc fcc g (5.3) Table 5.2 lists the corresponding values for B fcc. Besides assuming an articially increased temperature, in the equation for R c [Eq. (2.23)] the surface tension is the only other quantity changing in the presence of CM. Table 5.2: Analysis of CM of a single NC with respect to the eective temperature T (e) on the basis of the solubility increase, the corresponding number of ballistically broken bonds B fcc, and surface tension I. ( ; ) 5 ;3 5 ;4 (a fcc ) T (e) =T B fcc (CM) I (J=a 2 fcc ) 7.43() 8.2() 8.4() 8.53(2) 7.75() 7.87(2) 7.97(2)
97 5.3. ON THE INFLUENCE OF COLLISIONAL MIXING 87 Irradiated interfaces are in general rougher than nonirradiated ones. In the Ising model more broken bonds per unit area are observed, which increases the internal energy part I of the surface tension. The inuence of CM on I can be seen in Fig. 5.b. In this plot in comparison to the pure thermal case the excess number of dangling bonds of the cluster atoms is given as a function of the (assumed spherical 5 ) surface of the NC. In the chosen regime of CM the eective surface tensions (CM) I exhibit a linear dependence on the NC surface (the observed standard deviation is below.3% of the value (CM) I, whereas nonlinearities become only obvious for determining the dierence to the assumed linear surface dependence in the pure thermal case). Furthermore, for the range of the considered CM parameters, the leastsquare ts indicate a negative oset in the limit A!, which is a few times above the standard deviation. The meaning of this oset is not clear, but might be related to the size dependence of the surface tension for NCs consisting of O( ) atoms [92, 93]. The change in I (the observed values are listed in Table 5.2) is in line with the observed solubility increase. However, since the entropic part (CM) E of the surface tension has not been determined, the change of R c due to the modied surface tension (CM) is not clear. In this context it is interesting to note, that corresponding CM simulations of a at interface yield approximately the same eective solubilities as the asymptotic values in the limit R!of the GT relation (see Table 5.3). Fig. 5.2a shows a snapshot of the microstructure indicating the increased surface roughening. A measure of CM eects on the surface morphology is the mean interface width, which can be seen in Fig. 5.2b. The preliminary results of this simulation series seem to indicate a saturation of the surface width. Using a similar model, but restricting ballistic jumps to nearestneighbor exchanges, Bellon [94] has also reported a saturation of the interface width of () surfaces under irradiation. However, more simulations are needed to study the response of a at phase boundary on (isotropic) CM, e.g. the parameter regime of a transition of a at () surface to () facets, for which some evidence is present in the data. 5 The NC shape parameter [Eq. (3.8)] for the most intensive CMconditions is only approximately two percent higher than in the pure thermal case. Table 5.3: Steadystate solubilities in the case of CM of a at interface. ( ; ) 5 ;3 5 ;4 (a fcc ) c (CM) ( ;3 =a 3 fcc )..67().84() 3.75().8().29().49()
98 concentration (4=a 3 fcc ) 88 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION a) b) z (a fcc ) = = 5 = :5 2 4 Figure 5.2: Isotropic CM of a at phase boundary. In a) the microstructure exhibiting the induced surface roughening is shown in the case =5 ;3 ; and =:5 a fcc. In b) the eective interface prole is shown for the set of six CM parameters ( is given in units of ;3 ; ) corresponding to Table 5. and the pure thermal case (see Fig. 3.6). Discussion From the results presented above, it can be concluded, that the decrease of the capillary length with respect to the thermal value involves additional CMdependent factors. According to recent analytical work by Heinig [9] (whobyintegrating the isotropic, exponentially decaying, continuous displacement distribution over a spherical NC determined the prole of atoms mixed out, which enters then the radial diusion equation as a source term), the steadystate monomer concentration of spherical NCs subjected to irradiation is given by c (CM) (R) = c (CM) exp ) (R c (CM) R c (CM) = c +~q 2 (5.4) R (CM) c = ^R c c ; (5=4)~q 2 c +~q 2 : (5.5) Here the notation ~q = q=d has been used with the mixing amplitude q expressed in units of number of displaced atoms per nm 3 per second. The MC mixing intensity is related to q via the atomic density, i.e. N a = q. It should be noted, that q is the product of the ion current j times the number of displaced atoms per nm per incident ion, and is a function of the deposited nuclear energy per unit length. The analytical model predicts that the curvatureindependent solubility increase depends linearly on the product ~q 2. However, in the derivation of Eqs. (5.4) and (5.5)
99 (CM) =c c 5.3. ON THE INFLUENCE OF COLLISIONAL MIXING 89 a) 8 b) = =4 a fcc = 3=8 a fcc = =2 a fcc = 3=4 a fcc (CM) I =I x = =4 x = =3 x = =2 E3 2E3 2 (a 2 fcc =) 3E ( 2 ) x.2.25 Figure 5.3: In a) the observed solubilities c (CM) of the GTlike simulations are plotted versus the CM parameter 2. In b) the enhancement oftheinternal energy part I of the surface tension is plotted versus various roots of 2 [same symbols as in Fig. a)]. it has been assumed that every possible displacement of an IA out of a spherical NC is performed, which includes innitesimal small ballistic jumps. Due to the discrete character of the K3DLMC model, only a fraction of successful displacements contributes to the CMinduced modications [see Eq. (5.)]. According to this derivation, the eective capillary length R c (CM) is an explicit function of the CM parameters. However, while Eq. (5.5) gives an explanation for the observed reduced capillary lengths under irradiation, care has to be taken with respect to the intrinsic value of ^Rc. 6 The unperturbed pure thermal value R c is supposed to be a reasonable choice only in the limit ~q 2 c. For considerable CM levels the intrinsic capillary length has to be modied appropriately, i.e. ^Rc = R c (CM) =. Plotting the observed solubilities c (CM) versus 2 (see Fig. 5.3a) allows to check the simulation results with the curvatureindependent part of Eq. (5.4). For this purpose, in addition to the results of Table 5. further simulations have been performed for other values of the mixing intensity as well as for a fourth mixing length = :75 a fcc. A reasonable linear dependence is observed for each value of. Assuming the ansatz c (CM) = c + 2 = c + N a D 2 = c + ~q 2 (5.6) and using D = a 2 fcc = fcc ; [see Eq. (3.9)] and N a =4a ;3 fcc, the proportionality constants can be obtained (see Table 5.4). Here, however, a dependence not present in Eq. (5.4) is observed. This behavior is easily explained by taking into account the lattice character of the MC model. The smaller the ratio =a fcc the larger is the fraction of (i) displacements with r<r m, which do not contribute at all (see Fig. 5.9), and (ii) nearestneighbor 6 In Ref. [9] no prediction is given for the changes of the intrinsic capillary length ^R c due to CM.
100 9 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION Table 5.4: Dependence of the proportionality constant of Eq. (5.6) on the mixing length (the uncertainty of the last given digit is indicated in parenthesis). (a fcc ) (4).53(4).635(5).797(6) displacements of length r. Since only a fraction of nearestneighbor displacements corresponds to a detachment event (within the simulation ballistic jumps of surface atoms to an adatom position are the majority of these nearestneighbor displacements), the observed values of seem to be reasonable. Furthermore, a ballistic diusion coecient can be derived as D b = q2 c : (5.7) The last equation allows to express the observed solubility increase due to CM as the ratio of ballistic to thermal diusion coecients, i.e. c (CM) = c ( + D b =D). As can be seen by the leastsquare ts of Fig. 5.3b, the observed increase of the internal energy part of the surface tension (CM) = (CM) I + (CM) E is best described by (CM) I I =+ I ; 2 =3 : (5.8) In contrast to Fig. 5.3a, no dependence of the proportionality constant I is observed [an analysis with respect to individual mixing lengths yields values (in units of ( 2 ) ;=3 dropping the subscript I for convenience): :25 = :48, :375 = :54, :5 = :46, and :75 = :5, respectively]. For this empirically obtained relation between the increase of the internal energy part of the surface tension and the CM parameters, a derivation in the framework of (nonequilibrium) statistical mechanics remains to be given. The values of the capillary lengths plotted versus 2 can be seen in Fig. 5.4a. Here, for all four mixing lengths the mixing intensity has been increased until the regime of metastability (i.e. the CMinduced nucleation of new NCs see also Section 5.3.2) has been approximately reached. In the case of =:75 a fcc for high mixing intensities even a negative capillary length is observed. The change in the sign of R c with increasing mixing intensity can clearly be seen in Fig. 5.4b. A negative capillary length implies, that small NCs possess a lower steadystate equilibrium concentration than large ones. As a consequence, a new regime of NC evolution is expected, which will be discussed in Section Rewriting Eq. (5.5) the capillary length is given by R (CM) c = R c (CM) = ; (5=4)~q 2 =c +~q 2 =c : (5.9)
101 (CM) =c (CM) c 5.3. ON THE INFLUENCE OF COLLISIONAL MIXING 9 a) 4 b) (CM) c (afcc) R 3 2 = =4 a fcc = 3=8 a fcc = =2 a fcc = 3=4 a fcc = = :5 = = :25 = 2 = 3 E3 2E3 2 (a 2 fcc =) 3E =R (=a fcc ).4.5 Figure 5.4: In a) the tted capillary lengths are plotted versus 2. In b) the normalized GTlike c(r) relation for a single NC subjected to CM in the case of a mixing length = :75 a fcc (the values of are given in units of ;3 ; ) is displayed. The solid lines indicate the results of leastsquare ts. Combining Eqs. (5.4) and (5.5) and using a dimensionless CMinduced solubility u = c (CM) =c ; (which serves also as a measure of ballistic forcing) one obtains for the normalized eective capillary length R (CM) c R c = (CM) = ; c (CM) =c ; + c (CM) =c ; = (CM) = ; u +u = 5 4R c : (5.) The last equation expresses the CMdependence of the eective capillary length as a function of the solubility increase. Fig. 5.5a shows the CM behavior of R c (CM) =R c according to the analytical model [9], i.e. Eq. (5.) in the case (CM) = (see footnote 6). Plotting the simulated values of the eective capillary length versus the relative solubility increase (see Fig. 5.5b) it is observed, that within the K3DLMC model a higher ballistic forcing is needed to obtain the regime R c (CM) =R c < as predicted by the analytical model. This suggests, that in order to describe the simulation results in the framework of the analytical model [9], the ballistic forcing has to be scaled appropriately, i.e. u! u, with a free, dependent parameter. However, while the lattice character of the MC model gives a reasonable explanation for the proportionality constant between the predicted and simulated solubility increase [see Eq. (5.6)], the origins of the dierences with respect to the capillary length are presently not clear. It remains to describe the surface tension under CM completely, for which only the relative change of the internal energy part (see Fig. 5.3b) is known. Due to the lack of an appropriate nonequilibrium thermodynamic expression and inspired by Eq. (5.8), the relative change of the total surface tension under CM conditions is expanded in powers of
102 (CM) c =Rc R (CM) c =Rc R 92 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION a) b) = :25 a fcc = :375 a fcc = :5 a fcc = :75 a fcc = :25a fcc = :375a fcc = :5a fcc = :75a fcc c (CM) =c ; c (CM) =c ; Figure 5.5: In a) the theoretical dependence of R c (CM) =R c on the ballistic forcing u = c (CM) =c ; (as predicted in [9]) is plotted according to Eq. (5.) in the case (CM) =. In b) the simulation results for the eective capillary length are plotted as a function of the observed solubility increase. 6 7 u =3 (CM) =+ X n= n (u =3 ) n : (5.) Inserting the last expression into Eq. (5.), taking only the rst term of the expansion ( n2 =)into account, and performing the substitution u! u, one yields the following equation R (CM) = cr + ( u) =3 ; ( u) : (5.2) c +( u) Fitting the parameters and with respect to the simulation results (see Table 5.5) seems to give a reasonable description of the simulation data (see Fig. 5.6a). However, as the errors of the tted parameters are in the order of the values itself, this description is not satisfying. Table 5.5: Values for the surface tension parameter and the ballistic scaling parameter for ts of Eq. (5.2) with respect to the simulation data (see Fig. 5.6). (a fcc ) ;: :4 ;:68 :53 ;:36 :48 ;:43 :5 :88 :25 :23 :28 :85 :9 :84 :85
103 (CM) c =Rc R (CM) = 5.3. ON THE INFLUENCE OF COLLISIONAL MIXING 93 a) b) = :25a fcc = :375a fcc = :5a fcc = :75a fcc c (CM) =c ; = :25a fcc = :375a fcc = :5a fcc = :75a fcc c (CM) =c ; Figure 5.6: In a) the tted dependence of R c (CM) =R c [see Eq. (5.2)] is plotted versus the ballistic forcing u = c (CM) =c ;. In b) the corresponding tted surface tensions are shown. 6 7 The corresponding behavior of the normalized surface tensions is shown in Fig. 5.6b. According to this derivation a dependence not observed for (CM) I (see Fig. 5.3b) is obtained. The decrease of (CM) under mixing conditions implies, that the entropic part E decreases faster than the internal energy part I increases. Since in the limit u! no stable secondphase domains exist, which is equivalent to a vanishing surface tension [this corresponds to the pure thermal case in the regime T >T c see Eq. (3.7)], the tted behavior of (CM) =, although derived not quite convincingly, isphysically reasonable. In an ion beam mixing experiment one can easily control the magnitude of the ballistic forcing by varying the ion current and/or the implantation temperature, whereas the mixing length is given by the ionncsubstrate system. Therefore, in a series of simulations for a xed mixing length = :5 a fcc, the dependence of the solubility and the capillary length on the mixing intensity and the temperature (i.e. ) has been studied. Fig. 5.7 shows the results for the normalized capillary length as a function of 2. Obviously, for high temperatures ( / =T ) the capillary length remains positive until the regime of metastability is reached. Based on Eq. (5.5), Eq. (5.2) provides a reasonable qualitative description of the observed dependence of the eective capillary length on the CM parameters. Combining Eqs. (5.6) and (5.2) the condition R c (CM) =R c = is approximately given by (CM) = = (~q 2 =c ). Thus in the range =a fcc < the necessary ballistic forcing is roughly more than an order of magnitude larger than predicted by the analytical model. Knowing precisely (CM) (~q ) promises to provide a better correspondence between the predicted and simulated behavior of the eective capillary length and would allow to determine analytically the parameter window, for which R c (CM) < holds. While this has not been performed in this work, the general requirements are nevertheless clear. Basically, the ratio =R c denes the range of decrease of the eective capillary length. Therefore, a large mixing length (see Fig. 5.4) and/or a small intrinsic capillary length (see Fig. 5.7),
104 (CM) c =Rc R 94 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION fcc = :5 fcc = :75 fcc = 2: fcc = 2:25 fcc = 2: E3 2E3 2 (a 2 fcc =) Figure 5.7: Temperaturedependence of the simulation results of the normalized capillary length in the case =:5 a fcc. which according to Eq. (3.6) in this parameter range is roughly proportional to =T, support the decrease of R c (CM). In the above analysis it has been assumed, that the solubility enhancement (i) is completely due to ballistic eects and (ii) depends, accordingly, linearly on the product ~q 2 [9]. However, higher order powers of ~q 2 might become important for very large mixing intensities (in the above study has been varied for some orders of magnitude). It is also not clear, how the inevitably modied surface tension (not considered in [9]) inuences the observed solubility properties (for instance, thermally driven monomer detachment from an interface roughened by CM is facilitated with respect to a smooth one). Furthermore, it remains to be shown, how the lattice character of this CM model is compatible with the continuum description of displacements used in Ref. [9] Nucleation, growth, and Ostwald ripening in the presence of collisional mixing Eects during implantation As already pointed out in Section nucleation of precipitates during ion implantation can be described by appropriately modifying the rate equation (2.2) of cluster growth [64] and determining the modied kinetic coecients. As a consequence, a shift of the critical NC size is predicted, i.e. i? CM > i?. Therefore, the onset of nucleation is delayed roughly by a factor of the order of c (CM) =c as compared to the hypothetical case of impurity accumulation without ballistic side eects. After the end of the nucleation stage, also in the presence of CM all stable NCs are supposed to grow as essentially isolated precipitates as described in Section 2.4. During implantation a steadystate equilibrium should set in between monomer absorption and ballistically enhanced detachment like a thermal equilibrium establishes in the
105 5.3. ON THE INFLUENCE OF COLLISIONAL MIXING 95 absence of ballistic forcing. Thus, for constant conditions throughout the implantation, the concept of an eectively higher T imp may give a reasonable description of the NC evolution. Although it does not describe precisely the modications due to CM (see Section 5.3.), it might explain the similarities between experiment and results of K3DLMC simulations without including CM (see Section 5.). After a variation of implantation parameters the system transforms to a new steadystate. For instance, lowering the implantation temperature (or, equivalently, increasing the ion current) increases the value of the ballistic forcing u. Since now the monomer ux back to the NCs is reduced with respect to deposition of new impurities and CMinduced detachments, an overall increase of the monomer concentration is expected. As predicted by the pure thermal K3DLMC simulations a new nucleation stage may be initiated. Note however, that while stable NCs in the pure thermal case do not shrink in the case of a temperature decrease, in the case of CM the ratio of unchanged ballistic monomer detachment to reduced thermal condensation is supposed to support an overall NC shrinkage. This might explain, why no distinct bimodal size distribution has been observed in the Au implantation experiment described in Section 5.2. Eects during irradiation I. Inverse Ostwald ripening Irradiating a preexisting ensemble of NCs with a dierent kind of ions (e.g. with atoms building up the matrix) can cause a pronounced change of its steadystate properties. The resulting solubility increase towards a modied steadystate equilibrium [depending on the ballistic forcing from a few times c to some orders of magnitude (see Fig. 5.3a)] has to be fed by the NCs themselves. This causes initially a simultaneous size decrease of all irradiated NCs, where the smallest ones are expected to disintegrate, until modied coarsening sets in. From the behavior of a single NC in the presence of CM some conclusions can be drawn with respect to OR of an ensemble of NCs under irradiation. Assuming that NCs under irradiation remain spherical, for a xed and mixing intensities below the disintegration threshold (or, as will be shown below, the threshold for CMinduced nucleation of further NCs) u max, dierentphysical regimes should exist with respect to the minimum value R (CM) c min of the eective capillary length: R (CM) c min > : The capillary length remains positive for all mixing intensities below u max. Thus ordinary OR occurs, which proceeds, however, on a modied time scale (the CMinduced relative changes of the solubility and capillary length determine the modied velocity of OR see below). R (CM) c min =: For a specic mixing intensity u the capillary length vanishes. This implies that all stable NCs possess the same steadystate equilibrium concentration. Therefore, no OR occurs. R (CM) c min < : Within the parameter window u < u < u max, the eective capillary length becomes negative [9]. As a consequence, in this regime small NCs (in the range
106 96 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION 8 NIA therm al (:25 :2) (:75 :3) (:75 :25) 2 3 t ( 6 MCSs) 4 5 Figure 5.8: Analysis of the evolution of a model system of two diusionally interacting NCs with respect to the NC sizes (given as number of IAs N IA per NC). The corresponding mixing length (in [a fcc ]) and the mixing intensity (in [ ; ]) are indicated in parenthesis. of stable ones) have a lower steadystate equilibrium concentration than large ones. Such a dependence prevents coarsening and gives rise to a deltalike PRD, because the eective driving force and the resulting monomer ux reduce any size dispersion R i = jr i ; Rj [this becomes obvious by the substitution Rc!;R c in the single NC growth law Eq. (4.5)]. Therefore, in the following ballistically driven impurity redistribution towards equalsized NCs will be referred to as inverse OR. The above discussed modications of OR are demonstrated with respect to the evolution of two NCs diusionally interacting in a closed box (volume of simulation cell: a 3 fcc ) with periodic BCs.7 For four dierent conditions the detailed evolution of both NC sizes can be seen in Fig Taking the pure thermally driven OR as a reference (whose evolution can be seen in four snapshots in Figs. 5.9a { d), the range of modications due to CM can be seen. For mixing conditions favoring more the solubility increase than the decrease of the eective capillary length, accelerated OR is observed, i.e. the small NC dissolves within :2 6 MCSs (dasheddotted curve in Fig. 5.8). No OR occurs for CM parameters leading to avanishing capillary length (dashed curve in Fig. 5.8 despite the considerable uctuations of both NC sizes CM stabilizes this thermodynamically metastable system). Finally inverse OR occurs for negative R c (CM) (solid curve in Fig. 5.8). The growth of the small NC at the expense of the large one can be seen in Figs. 5.9e { h. It should be noted, that while in the pure thermal case both NCs maintain their quasiequilibrated octahedral form, here the faceting is smeared out due to CM. Although the surfaces are rough the NCs remain compact. Since the characteristic time constant of coarsening di is proportional to =(R c c ) [see Eq. (4.6)], the relative change of the velocity of coarsening can be obtained by inserting 7 This simple model system is certainly aected by selfinteractions. Nevertheless the governing physics should be clear.
107 5.3. ON THE INFLUENCE OF COLLISIONAL MIXING a) b) t e) c) t2 f) 97 d) t3 g) t4 h) Figure 5.9: Evolution of two NCs in a closed box with periodic BCs for fcc = :75. Starting with identical initial systems [R (t ) 4:5 afcc, R2 (t ) 7:5 afcc] in the top row ordinary, i.e. thermally driven, OR can be seen (no ballistic jumps), whereas in the bottom row for the CM parameters = :5 ; and = :75 afcc inverse OR is shown. Referring to Fig. 5.8 the snapshots have been recorded at t = 5, t2 = :6 6, t3 = 3:6 6, and t4 = 4:9 6 MCSs, respectively. the respective values under CM. Fig. 5.2 shows the modied time constants. Assuming a constant di usion coe cient (neglecting within this analysis a change in D due to the additional ballistic jumps per MCS as well as a concentration dependence, i.e. D 6= D(c)) an acceleration of ripening up to a factor of eight is predicted within the parameter regime of this study. It is interesting to note, that the largest acceleration of OR is obtained for the smallest mixing length. This can be understood in terms of the di erent mixing
108 (CM) di di= 98 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION c (CM) =c ; 6 7 Figure 5.2: Variation of the characteristic time constant for OR di parameters (for the data points of Figs. 5.3 and 5.4). for various CM dependences of the solubility and capillary length. The change in the coarsening velocity is given by (expressed in terms of the ballistic forcing u = c (CM) =c ; ) di (CM) di = R(CM) c c (CM) R c c = (CM) = ; u ( + u) (5.3) + u where Eq. (5.2) has been used. In addition to a negative eective capillary length, inverse OR is characterized by a negative time constant, the meaning of which is, however, presently not clear. Although NCs lose their faceted octahedral shape under CM, they essentially remain spherical. Within this CM model no evidence for a dynamical shape transition has been observed below the disintegration threshold. In this context it is interesting to note that applying his mixing model Bellon [94] has reported for a fcc NC a faceting transition from octahedral to cuboidal shape for a high ratio of ballistic to thermal nearestneighbor diusion steps. Eects during irradiation II. Collisional mixinginduced nucleation For a better understanding of the modications of the impuritysubstrate system due to ion irradiation the (c T ) phase diagram has to be determined. While some trivial limits are clear, e.g. the absence of CM or the limit u!, which corresponds to a completely random system free of thermal eects, the range of the metastable part of the phase diagram is presently not clear. In particular, a denition of the modied supersaturation (CM) has to be given. In this context it should be noted, that after the solubility increase c (CM) =c has exceeded a temperaturedependent threshold, nucleation of new NCs is observed. This can be seen in Fig. 5.2a, where for a model system analogous to Fig. 5.9 the evolution of the individual NCs is plotted. Whereas for the mixing intensity = :3 ; only
109 5.3. ON THE INFLUENCE OF COLLISIONAL MIXING 99 a) b) 4 3 = = :3 ; = :4 ; NIA t ( 6 MCSs) 2 4 Figure 5.2: Analogous to the model system of Fig. 5.9 [here: R (t ) 3:5 a fcc, R 2 (t ) 6: a fcc ] for the parameters fcc = 2:25 and = :5 a fcc the evolution of individual NCs is displayed in a) for various mixing intensities. The dashed lines indicate the pure thermal case. Inverse OR can be seen for = :3 ; and = :4 ;, where at t 5 6 MCSs an additional NC forms. In the case = :4 ; in b) a snapshot of the microstructure at t = :3 7 MCSs is shown indicating three essentially equalsized NCs. inverse OR 8 of the existing NCs is observed (at least during the nite simulation time), for a mixing intensity =:4 ; the system is clearly transformed to the metastable state, because an additional NC is formed at t 5 6 MCSs. For this system inverse OR is then observed among three NCs. Although Fig. 5.2b suggests at a rst glance, that the large NC has disintegrated, Fig. 5.2a rules out this possibility. The tendency for CMinduced nucleation can be understood as follows: From a thermodynamical point of view an increasing CM intensity drives the system to a higher energetic state, because more IAs are found as dissolved monomers [see Eq. (5.4)]. As already pointed out in Section 5.3., in the regime of a negative capillary length small NCs have a lower steadystate monomer concentration than large ones. This implies that the nucleation of new NCs is energetically favorable, if the eective solubility decrease due to the decreasing average precipitate size overcompensates the additional energy to be spent to create new phase boundaries. Thus it can be concluded, that beyond the limit of inverse OR at a constant NC density the higher the ballistic forcing u the more additional NCs will be nucleated. This, in turn, decreases the meanradius of the NC ensemble, because the precipitated amount of impurities will be equally shared among more clusters. 8 In the case of the parameters fcc = 2:25 and = :5 a fcc, the capillary length becomes negative slightly above =: ; (see Fig. 5.7).
110 CHAPTER 5. NANOCLUSTER EVOLUTION DURING ION IMPLANTATION General discussion One of the major approximations of this CM model is the neglect of matrix atoms mixed into the secondphase domains. This process is supposed to enhance the interface roughness, because it makes the phase boundary more diuse. While in the current model a vacancy is left after a ballistic jump of a bulk atom close to the interface into the matrix, the reverse process introduces matrix atoms into the NCs. This should promote the disintegration of small NCs, thus causing an additional shift in i? not observable in the current description. Thus the above model should give a reasonable description for NC/substrate systems, where (i) the solubility of matrix atoms in the NCs is high (no precipitation within the secondphase domains) and (ii) the diusion coecient of matrix atoms in the secondphase domains is high (they can quickly reach the phase boundary and rejoin the matrix). For a complete description of the NC evolution during implantation/irradiation also dwell time eects of the ion beam have to be considered. Since in CBII the substrate is scanned by the ion beam at a dened frequency, for a particular area periods of ion deposition accompanied with CM take place alternately with (in general larger) periods of basically thermally activated impurity redistribution. Dwell time eects have been rather extensively studied in the area of buried silicide layer formation using a FIB [95, 96], but are usually not even mentioned in IBS of NCs.
111 Chapter 6 Combination of K3DLMC and RDE simulation methods As already pointed out in Chapter 4, the RDE approach to OR needs as essential input the coordinates f~r i g and radii fr i g of NCs. Although some setting algorithms have been developed which try to cover some properties of real NC distributions (e.g. mean radius, volume fraction, density, size distributions, and spatial correlations) [72, 82], statistically generated input data are always to some extent articial. For innite homogeneous systems this is not much a problem, because all ensembles evolve towards an attractor state [62] regardless how unphysical the initial conditions were chosen. However, the main problem in simulations of OR of inhomogeneous (nite) systems remains the choice of the initial conditions. In nite systems small uctuations may have a strong eect on the (spatial) evolution [4], thus a reliable knowledge of the initial conditions is crucial for a RDE approach to OR. On the other hand, as shown in Chapter 5, the K3DLMC method covers the basic mechanisms of nucleation and growth of NCs. In principal, this atomic model allows to study consistently all basic processes of IBS of NCs including OR. However, due to the restricted power of current computer systems, it is in general not the method of choice for predictions of large scale and long time phenomena. Thus it is tempting to combine both simulation approaches via the transfer of data (f~r i g, fr i g) in order to study the evolution of NC ensembles from the very beginning of nucleation to the late stage of coarsening [84]. Before applying the combined simulation scheme to nite inhomogeneous systems, e.g. layers of NCs formed by IBS, rst the results of K3DLMC simulations of homogeneous coarsening have to be studied and discussed. 6. K3DLMC and RDE simulations of homogeneous OR Using the KIM (usually restricted to nearestneighbor interactions) MC studies in two (mostly on a square lattice) [97][2] and three (mostly on a sc lattice) [9][94] dimen
112 2 CHAPTER 6. COMBINATION OF K3DLMC AND RDE METHODS sions of the growth of minority phase domains in systems with conserved and nonconserved order parameter have been performed for many years (see, e.g. Gunton et al. [6] for a comprehensive review of the work up to 983). As a consequence of the scaling hypothesis [Eq. (2.42)] and the LSW theory (see Chapter 4) in the late stage of phase separation all physical quantities should depend only on a single length scale L, i.e. the average domain size or, equivalently, the average distance between domains (see e.g. the reviews of Furukawa [96] and Bray [97]). Usually, one assumes a power law for growth of the form L / t m (or, equivalently, k m / t ;m for the value of the wave number, which maximizes the structure function S( ~ k t) [Eq. (2.32)]), and tries to determine the coecient m. Additional to extensive MC studies of the properties of the structure function S( ~ k t), the evolution of NCs was also followed directly by an analysis of individual NCs and the mean cluster size. For instance, using a sc lattice gas model, Penrose et al. [] simulated cluster growth after a quench (T = :59 T c ) below the coexistence curve into the metastable region. For a system with c =:75 a ;3 sc they reported a linear dependence of the critical NC size i? on time for a run of 6 MCSs. Further MC studies in three dimensions with explicit analysis according to the droplet model have been performed, for instance, by Lebowitz et al. [94], Kalos et al. [98], and Penrose et al. [99], who concentrated on a detailed kinetic description of the phase transition. Surprisingly, since the middle eighties further work on domain coarsening in three dimensions using the KIM is very hard to nd [2]. 6.. K3DLMC simulations of homogeneous OR In order to analyze the properties of the K3DLMC model with respect to OR, in a series of simulations on a fcc lattice systems with volume fractions = : have been studied. For a system size of unit cells (using periodic BCs) the evolution of the IAs has been monitored over a period of 4 6 MCSs. Nucleation stage Quenching the statistically distributed IAs to ve nite temperatures well below T c (i.e. assuming c(t =)=4a ;3 fcc ), the initial dimensionless supersaturations =ln(c(t )=c ()) are listed in Table 6.. Combining Eqs. (2.) and (3.7) the energy barriers W min for homogeneous nucleation W min = fcc () 2 R (fcc) c a fcc fcc + fcc! 3 J fcc (6.) and the corresponding (continuous) critical NC sizes i? = 6 3 " fcc () R (fcc) c a fcc fcc + fcc!# 3 (6.2)
113 n (=a 3 fcc ) 6.. K3DLMC AND RDE SIMULATIONS OF HOMOGENEOUS OR 3 a) E3 b) 6 E4 E5 R (a fcc) t ( 6 MCS) t ( 6 MCS) 2 4 Figure 6.: Using doublelogarithmic scales the evolution of the density of NCs and of the mean radius are shown in a) and b), respectively. In the ln(n)ln(t) plot, from bottom to top the curves correspond to fcc = f:25 :5 :75 2: 2:25g, whereas the reversed order is valid in the ln( R)ln(t) plot. as given by classical nucleation theory are listed in Table 6. as well (note, however, the sensitivity of Eqs. (6.) and (6.2) with respect to the derived expression for the surface tension see Section 3.5.3). Due to the high supersaturation levels the critical NC sizes are extremely small (in the case fcc =2:25 even a dimer can be regarded as a critical nucleus). It is, however, questionable, if the capillarity approximation, and thus the classical nucleation theory, provides reliable results in a regime with no distinct surface and bulk energy states. Coarsening stage The further evolution of the NC density n(t) and the mean radius R(t) is shown in Fig. 6.. In these plots for each value of fcc the average of two independent runs has been Table 6.: Temperaturedependence of the initial supersaturation, the critical NC size i? [Eq. (6.2)] and the energy barrier W min for nucleation [Eq. (6.)] with respect to an initial monomer concentration c(t )=:4 a ;3 fcc. fcc i? W min =J fcc
114 ! 4 CHAPTER 6. COMBINATION OF K3DLMC AND RDE METHODS a) b).3.2 = :75 = 2: = 2:25 N=Ntot.2. K3DLMC LSW di LSW reac 2 t ( 6 MCS) Figure 6.2: In a) the evolution of the widths! of PRDs corresponding to the simulations for the three lowest temperatures of Fig. 6. are shown. As a reference the results of the both limiting LSW distributions (see Fig. 4.) are added. In b) the PRD of a single run for = 2 obtained after 2 6 MCSs is shown. used. Sizedependent eects should not have inuenced these simulations, since the largest diusional screening length of this series [as obtained by Eq. (3.8)] for fcc = :25 is D 42 a fcc. This value is considerably below the linear dimension of the simulation volume, thus selfinteraction eects are negligible. Care has to be taken in order to extract the growth behavior, since a t assuming R / t m is only justied for late times of phase separation. According to Eq. (4.6) this implies that the relation R(t) R must be valid. Due to the quench the initial system consisted entirely of monomers, thus for application of the LSW theory the mean radius has to be large with respect to R :39 a fcc. Assuming that this requirement isfullled (at least in the end of the simulations), leastsquare ts performed in the time interval 6 <t<4 6 MCSs yield growth exponents m( fcc =:25)=:9, m( fcc =:5) = :26, m( fcc =:75) = :23, m( fcc =2:)=:9, and m( fcc =2:25)=:7, respectively. These results would indicate a temperaturedependence of ripening (the data for fcc =:25 show avery bad statistics), which is not predicted in the LSW theory [Eq. (4.6)]. More insight into the dynamics of the K3DLMC method is gained by plotting the widths w [Eq. (4.3)] of the PRDs as can be seen in Fig. 6.2a. Fig. 6.2b shows the PRD for fcc = 2 obtained after 2 6 MCSs. While the size distribution is in reasonable accordance with the stationary form (LSW) of the PRD of diusion limited OR [Eq. (4.5)], it is on the average somewhat smaller (see also Fig. 4.) and seems to be more symmetric. Since the quasistationary form of the PRD is directly coupled to the growth law, the on the average smaller width! as compared to the result of the diusion controlled LSW regime is consistent with the observation m<=3. However, a more careful analysis reveals, that the simulated coarsening data can not be Using a 3 fcc =4V a.
115 6.. K3DLMC AND RDE SIMULATIONS OF HOMOGENEOUS OR 5.3 me = R (=afcc ).6 Figure 6.3: The eective domain growth exponent m e of the K3DLMC model is shown for the parameter fcc =:75 according to Eq. (6.3) with data points in the range t 5 5 MCSs. analyzed in the framework of the standard LSW theory, because Eq. (4.2) is based on the linearization of the GT equation (i.e. use of Eq. (4.) rather than Eq. (2.23) see also Fig. 4.3). This is, however, not justied for the rather small NCs of the current simulations, which becomes obvious by comparing the range of the mean NC radius R, as obtained by the simulations, to the corresponding capillary lengths. According to Eq. (3.6) the capillary length varies between R c ( fcc = :25) 2:42 a fcc and R c ( fcc = 2:25) 4:6 a fcc. Thus for the lowest temperature of the simulation series ( fcc =2:25), the mean domain size has only grown up to the order of the capillary length, whereas for the highest temperature ( fcc =:25) the ratio R c = R has become small at the end of the simulation a linearization of the GT relation would be justied in modeling this ensemble at later times. Since in all simulation of this series the LSW requirement R c = R is not satised, coarsening should be analyzed with respect to an eective growth exponent according to the growth law R(t) = A + Bt =3 [note the dierence to Eq. (4.6)!]. This approach has been motivated by domain growth studies in the twodimensional case [99, 2]. Without discussing the capillary length of the square lattice, these authors proposed an eective growth exponent m e = 3 ; C R(t) := dfln[ R(t)]g : (6.3) d[ln(t)] Thus an analysis of the growth behavior has been performed using an appropriate implementation of Eq. (6.3), i.e. m e (t f )=ln[ R(tf )= R(ti )]= ln(t f =t i ) with, e.g. t f =t i =2. 2 Fig. 6.3 shows the result of the analysis for fcc = :75 and the corresponding leastsquare t. Here, the eective growth exponent approaches the LSW prediction m = =3, but, as the 2 This (arbitrary) ratio should exclude uctuations, but guarantee 'local' time in this discrete implementation of the derivative of Eq.(6.3) [2].
116 6 CHAPTER 6. COMBINATION OF K3DLMC AND RDE METHODS a) 4 b) 4 R (a fcc) 3 2 = :25 = :5 = :75 = 2: = 2:25 R (a fcc) 3 2 = :25 = :5 = :75 = 2: = 2: MC MC Figure 6.4: In a) the results of Fig. 6.b are replotted by scaling according to Eq. (6.4). In b) the modied time constants MC =[R(i? ) 3 =V a ] MC have been used. large scatter of the data indicates, this particular results seems to depend on the range of included data (the considerable scatter in the data points for the other four simulation parameters gives partly even a negative m e ). Thus a good statistics is needed in order to obtain a smooth dependence of R on t (Amar et al. [2] used independent runs in their study of the twodimensional case). With more reliable data, the constant C in Eq. (6.3) can be determined, which should exhibit a temperature dependence proportional to the capillary length. Since all simulations of this series started from the same initial state (basically just dissolved monomers) followed coarsening of the nucleated NCs, it is interesting to check if a common scaling behavior can be extracted. Therefore, inspired by the LSW approach [Eq. (4.6)] a dimensionless MC time scale is introduced, MC = D sim c R c = l a 2 l A l expf;( l =2) l g(r (l) c + l a l l ) fcc 3expf6 fcc g (;:32 + 2:9 fcc ) (6.4) where Eqs. (3.), (3.4), and (3.6) have been combined (normalizing, as usually, a MCS). As Fig. 6.4a indicates, this approach does not scale the K3DLMC results, rather a systematic deviation is observed. This is, however, not a surprise, because according to the LSW theory scaling should only occur, if OR is governed by a stationary dynamics. This can not be expected here, since for all parameters R c = R is not given. Furthermore, the LSW approach assumes a ripening system, whereas in these simulations the nucleation stage is included. This suggests to derive a scaling constant MC =[R(i? ) 3 =V a ] MC, which is modied by the critical nucleation size. Using Eq. (6.2) in order to obtain i?, Fig. 6.4b shows the result of the modied scaling attempt. While there is an excellent agreement for :75 (the curves are hardly distinguishable) the other two cases deviate (with respect to Fig. 6.4a an overcompensation for high temperatures is observed). Having in mind the
117 6.. K3DLMC AND RDE SIMULATIONS OF HOMOGENEOUS OR 7 uncertainties related to Eq. (6.2) and that the LSW regime of coarsening could not be reached with the available computer capacities, a more detailed study of the K3DLMC scaling behavior remains to be done in future approaches Comparison of K3DLMC and RDE simulations of OR The RDE approach toorveries the LSW predictions provided that R c = R holds [4, 49], thus it is interesting to apply the RDE method to systems characterized by R c = R. The direct comparison to the K3DLMC method reveals, furthermore, the similarities and dierences of the atomic and thermodynamic descriptions of domain growth. Therefore, after a K3DLMC run for 4 5 MCSs of a system quenched to fcc =:75, the further evolution of the NC ensemble was followed also in parallel with the RDE description in the diusion controlled regime. Fig. 6.5 shows the corresponding results after 3:6 6 MCSs, where the RDE parameters have been chosen such astogive identical capillary lengths. At a rst glance both simulation results seem to be very similar, but a closer inspection reveals certain dierences of the microscopic evolution (positions and sizes of remaining NCs). In order to compare the dynamics of both simulation methods, Fig. 6.6 shows the evolution of the NC densities, which obey a quite similar behavior. The additional plot of n obtained by the RDE method using the linearized GT equation [LSW approximation, Eq. (4.)] exhibits the inuence of the choice of the driving force on the dynamics of OR. The dierences in the dynamics of both RDE simulations is also reected in the time scales of coarsening. For this particular comparison the durations of ripening [measured in units of di,eq.(4.6)] are related by t LSW 3t GT. In general, this time dierence is a function of the ratios R i =R c and R f =R c for the initial and nal mean radii and vanishes for R=Rc!. Since the K3DLMC method excellently reproduces the GT relation (see Fig. 3.8) it is obvious, that a parallel or subsequent RDE approach should use the same dynamical description. As already pointed out, a more detailed analysis reveals, that the sequence of dissolving NCs depends on the simulation approach. Fig. 6.7a shows the dierences of the evolution of the NC ensemble in the parallel treatments by directly comparing the sizes. These dierences with respect to the detailed evolution within each simulation method is not really surprising, because the RDE simulation is deterministic once the input data (f~r i g, fr i g) have been xed, while the K3DLMC simulation is stochastic in nature. A further analysis with respect to the movement of NCs inherently included in the K3DLMC method is shown in Fig. 6.7b. In this plot for each surviving NC of the MC simulation the nearest remaining NC in the RDE simulation is determined (note that the monopole approximation used in the RDE method does not allow for NC diusion they remain xed at their positions). While a majority of the NCs has moved at most r = j~r f ;~r i j4 a fcc, the few with no close remaining counterpart can easily be explained by the dierence in the sequence of NC dissolution of both descriptions. Although the dependence of the eective coarsening dynamics on the ratio R c = R seems to oer a reasonable explanation for the observed growth exponents, there might be ad
118 CHAPTER 6. COMBINATION OF K3DLMC AND RDE METHODS :6 6 MCSs 3:6 6 MCSs MCSs # (f~rig; frig) # tim e  Figure 6.5: Comparison of OR simulations with K3DLMC and RDE methods of a fcc system with volume fraction = : quenched to fcc = :75. Upper row: snapshots from the K3DLMC simulation; middle row: the corresponding spherical cluster representation. The RDE simulation starts with K3DLMC input data as recorded at t = 4 5 MCSs. Lower row: the ensemble is shown at equal NC densities, i.e. nrde = nmc.
119 RRDE (afcc) n (=a 3 fcc ) 6.. K3DLMC AND RDE SIMULATIONS OF HOMOGENEOUS OR 9.5E4 E4 K3DLMC RDE: GT RDE: LSW 5E5.5 time Figure 6.6: Comparison of the evolution of the density of NCs obtained by the K3DLMC and RDE methods in the normalized time interval between t =4 5 and t =3:6 6 MCSs (see Fig. 6.5). a) b) NNC R MC (a fcc ) 5 2 j~r f ; ~r i j min (a fcc ) 3 Figure 6.7: Comparison of the evolution of NCs obtained by the K3DLMC and RDE (with GT) methods. In a) the radii as obtained by both methods are directly compared. In b) for each remaining NC of the K3DLMC ensemble the distance to the nearest remaining NC of the RDE ensemble is determined. ditional factors inuencing the phase transformation. Since the K3DLMC method automatically includes the migration of NCs, it is tempting to analyze, if the NC dynamics can be brought into accordance with the BinderStauffer theory of cluster growth [22, 23, 78]. In their model the cluster evolution proceeds mainly via coagulation rather than monomer evaporation and condensation. Therefore, coarsening occurs via coalescence of diusing NCs and is thus determined by the eective diusion coecient D NC (i) ofncs. Depending on the detailed atomic mechanism, by which the center of mass of a NC moves (e.g. surface diusion, diusion of a vacancy within the NC or evaporation of a monomer
120 d (afcc) CHAPTER 6. COMBINATION OF K3DLMC AND RDE METHODS a) b) n ;=3 d min t ( 6 MCS) R (a fcc ) 5 6 Figure 6.8: In a) the evolution of the mean NC distance given by the inverse cubic root of the density is compared to the minimum NC distance in the ensemble. In b) the spectrum of the NC shape parameter during OR (4 5 <t<4 6 MCSs) as recorded every 2 5 MCSs is plotted. and recondensation at a dierent surface site) a growth law is derived, which in three dimensions varies between the regimes R / t =6, R / t =5, and R / t =4, respectively. For instance, Toral and Marro [24] interpreted the change of the evolution of the excess energy E=J / R ; from a =6 to a =3 growth regime with a change from the cluster coagulation to the OR coarsening mechanism. In order to proof, whether this cluster growth mode explains the observed time dependences, the K3DLMC results have tobechecked for the motion of NCs and for deviations from the quasiequilibrated shape of faceted octahedras due to coalescence events. This is done by measuring in intervals of t = 5 MCSs the minimum distance between any two precipitates dened as d min = j~r i ; ~r j j min ; R i ; R j. As the plateaulike behavior of d min in Fig. 6.8a indicates, no evidence for diusional encounters of NCs can be detected [the minimum observed distance of 5 a fcc is larger than the maximum analyzed diusion length r max 4 a fcc (see Fig. 6.7b) for the whole coarsening process]. The slight negative slope of the plateaus is not necessarily due to NC diusion also NC growth (see denition of d min ) can explain this observation. Consequently, in the recorded data of the NC shape parameter [Eq. (3.8)] no signicant deviations can be observed except for the smallest NCs shortly to their dissolution (see Fig. 6.8b). To summarize this subsection it should be noted, that both the atomic and mesoscopic simulation models result in the same cluster dynamics, provided the same driving forces are applied [use of the appropriate (i.e. exact or linearized) GT relation in the RDE approach]. This implies that the K3DLMC method would model the late stage of phase separation according to the LSW predictions if the computation power would allow for long lasting simulations (although here K3DLMC simulations of OR in three dimensions have been extended for two orders of magnitude in time (MCSs) compared to earlier studies, the LSW regime has not been reached for the chosen temperatures). With respect to
121 6.2. LATE STAGE EVOLUTION OF ASIMPLANTED SAMPLES the movement of NCs observed in the K3DLMC simulations it would be interesting to check the range of NCs diusion of corresponding RDE approaches extended to the dipole approximation (which take into account NC migration as well as shape deviation) [66]. 6.2 Late stage evolution of asimplanted samples Background Selforganization is a well known phenomenon occurring in nature on several time and length scales [54]. In the area of IBS of nanostructures the observation of layers of NCs aligned parallel to substrate interfaces, for instance in the SIMOX process [25][28], can be explained by selforganization. The underlying dynamics in such nite systems may be determined by OR [29], and spatial inhomogeneities (e.g. the presence of interfaces or concentration gradients) are believed to be the reason for the modulated arrangement of NCs. Computer simulations based on the RDE approach successfully described the occurrence of bands of NCs [4, 3] using a model, where an absorbing interface initiated the selforganization. Additionally the structure wavelength was determined as the characteristic interlayer distance, which is proportional to the diusional screening length D [] [see also Eq. (3.8)] (t) = D (t) = p 4n(t) R(t) 3: (6.5) The discussions of Refs. [4, 3] have assumed the rather articial initial condition of equalsized precipitates across the implantation prole. Though experimental evidence supports this assumption [2], simulations beyond this approximation are needed to clarify the physics of this process. Especially the competition between the coarsening of NCs, which is initially suppressed in the studies of Refs. [4, 3], and the selforganization of NC layers have to be considered in more detail. With the combination of both simulation tools, it is possible to consistently describe the evolution of IAs implanted into a substrate. In particular, the inuence of an absorbing interface on the impurity redistribution can be included from the very beginning, which allows to trace back the origins of the observed spatial patterns to the NC nucleation stage [84]. From such K3DLMC simulations one obtains consistent NC distributions as input data for the RDE modeling. Within the framework of OR it is then studied how BCs and internal ripening interfere during the evolution of these structures. K3DLMC simulations Here, the study is restricted to systems, where the physical conditions during implantation prevent a signicant redistribution of the deposited atoms before annealing. As an example, the evolution of an asimplanted Gaussianlike depth prole for a uence of F 3 a ;2 fcc IAs has been simulated in a volume of fcc unit cells for fcc =:75. The
122 c (=a 3 fcc) concentration (=a 3 fcc ) 2 CHAPTER 6. COMBINATION OF K3DLMC AND RDE METHODS a) t = t = 5 t = 4 b) 6E3 4E3 2E3 t = 3 t = 6 t = z (a fcc ) 2 25 Figure 6.9: In the top plot the evolution of the impurity prole during the K3DLMC simulation is shown. Times are given in units of 3 MCSs. In the bottom plot, the monomer concentration c averaged over the last 4 MCSs with respect to the indicated MC times can be seen. projected range of the peak concentration is R p = 28 a fcc (with R p =42a fcc ), and at a depth of L z = 256 a fcc an absorbing interface is set up. This corresponds to a symmetric implantation into a thin layer A on a substrate B, where either the impurities are volatile (diuse out through the surface) or B acts a sink for the IAs. The inuence of the absorbing BC is clearly seen in Fig. 6.9a, where MC simulation results of the evolution of the depth distribution of implanted IAs are plotted. The absorbing interface causes an asymmetry of the prole with a NC free region spreading out towards the center. Across the prole, some structuring occurs as indicated by the evolving peaks. 3 More insight in the mechanisms of impurity redistribution is gained by plotting the monomer concentration versus depth (see Fig. 6.9b). Whereas the reecting interface at z = is characterized by a vanishing concentration gradient at a nite value of c, the concentration gradient atz = L z is proportional the the monomer ow outofthesystem. The overall concentration decrease with time is due to the increase of the average radius 3 Note, that this local structuring is only visible due to the nite lateral dimension of the simulation volume.
123 6.2. LATE STAGE EVOLUTION OF ASIMPLANTED SAMPLES 3 (GT relation) during coarsening. Since the velocity of OR depends on the volume fraction of impurities (the higher the less is monomer diusion length between shrinking and growing NCs), the minimum of c around R p is in accordance with the observation, that the largest NCs can be found there (see also Fig. 6. below). It should be noted, that despite diusional screening eects the monomer concentration prole of Fig. 6.9b indicates a net ow of impurities from the tails of the prole towards the center. These concentration gradients give an explanation of experimentally observed accumulation of implanted impurities close to R p in terms of ordinary rather than "uphill" diusion. RDE simulations In order to discriminate between internal ripening eects and boundaryinduced structuring, two dierent sets of input parameters have been extracted from the K3DLMC method. In both cases, the positions of the NCs have been transferred. Then for one run of the RDE simulation the atomically derived radii have been used [case (i)], whereas in the other case (ii) the mean radius R has been assigned to each NC. The long time behavior of both systems can be seen in Fig. 6.. In both RDE simulations the absorbing interface was described by the BC 4 c(l z ) = c (as used in Ref. [4]). Obviously, for case (i), the BC has only a minor inuence on the impurity redistribution. Pronounced selforganization into layers of NCs is only observed using the rather articial condition R i (t RDE =)= R. Discussion Right from the beginning of thermally activated impurity diusion, nucleation of NCs starts beginning in the center of the prole, where the highest supersaturation is found. After the monomer concentration has dropped considerably, local OR is initiated by small size dierences. Since according to the GT equation the equilibrium monomer concentration decreases with increasing cluster size, precipitates slightly larger than the average become a more eective sink to diusing monomers. Thus small uctuations initiate a selfamplifying coarsening process over the whole implantation prole. Assuming an approximately constant mean NC radius across the prole (this should be a reasonable assumption for the early phase separation process), the diusive screening length D, and thus the structure wavelength [Eq. (6.5)], varies with depth and is smallest in the center of the prole, where the density of precipitates is highest. During annealing the diusive screening length evolves (in the case of diusion controlled coarsening) proportional to t =3 according to the time dependences of n(t) and R(t) [LSW theory, see Eqs. (4.6) and (4.7)]. This is the reason, why spatial structures, which are in phase with (i.e. selfamplifying) during a certain time, grow out of phase for later times and then start a competitive growth among each other. 4 Noting the value c( fcc =:75) = : ;3 a ;3 fcc, the choice c(l z) = used in the K3DLMC simulation (see Fig. 6.9) obviously has had a negligible inuence on the early stage of impurity redistribution.
124 4 CHAPTER 6. COMBINATION OF K3DLMC AND RDE METHODS (f~ri g; fri g) ;; (f~ri g; Ri = R )? Figure 6.: Combined K3DLMC and RDE simulations of the redistribution of IAs during annealing in the presence of an absorbing interface. In the top row, the microstructure of an asdeposited prole is shown after 4 5 MCSs for fcc = :75. For the left column the sets (f~rig; frig) are used as input for the RDE simulations. For the right column only the positions are transferred, whereas the mean radius R is assigned to each NC.
125 6.3. FOCUSED ION BEAM SYNTHESIS OF NC ARRAYS 5 It should be noted, that while the spatial inhomogeneity due to the (Gaussian) concentration prole inuences all NCs, the diusional interaction with the absorbing interface is screened by the precipitates located in the tail towards the interface. For the K3DLMC simulation the eective depth of this interaction range can be associated with the z coordinate breaking the symmetry of the monomer concentration eld (see Fig. 6.9b). Thus selfstructuring across the prole starts before diusional interaction between the interfaces and the main fraction of NCs sets in. However, as can be concluded from the RDE simulations of system (i), internal OR does not necessarily induce the formation of bands of NC. Yet the signature of this internal coarsening is pronounced enough to dominate over the disturbance present due to the absorbing BC. As can be seen in the right column of Fig. 6., only suppressing internal OR by assigning all NCs the same initial radius (i.e. all precipitates possess the same equilibrium concentration, thus no monomer concentration gradients are present) allows the formation of periodic layers induced by the absorbing interface. From the simulations presented above it can be concluded, that the observed tendency towards selforganization in systems modeled consistently beginning from the nucleation stage does not necessarily result in equalspaced layers of precipitates. Thus it is very likely, that in ionimplanted systems besides the driving force of phase separation further physical eects (e.g. inhomogeneities due to radiation damage) inuence the impurity evolution. 6.3 Focused ion beam synthesis of NC arrays In CBII the formation of NCs can be controlled to some extent with respect to ensemble properties like the average depth or the mean radius. Furthermore, a specic dispersion of the size distribution seems to be inevitable, whichisincontrast to the need of monodisperse sizes in certain applications. The use of a nely focused ion beam (FIB) [48] promises to open new methods of NC synthesis by a precise control of the lateral deposition pattern as well as of the implanted uence. Besides forming buried structures by "writing" the desired pattern with the FIB directly onto the substrate, an interesting application is the dened synthesis of a single nanocrystal atachosen position on the substrate. A straightforward extension would be the synthesis of a regular array of nanocrystals [2, 44], which would possess a monodisperse size distribution due to (ideally) identical implantation conditions at each spot. For appropriate NCsubstrate systems, the twodimensional periodic array can be regarded as a photonicbandgap material [22, 23] specically inuencing the properties of light transmission. While such structures have been designed with lattice spacings in the range of several m or larger, photonic bandgap materials in the range of visible light are dicult to synthesize. In this area, the formation of periodic arrays of NCs by FIB implantation might provide a promising alternative. It is, however, a priori not clear if the deposited uence per spot coalesces into a single NC, or if losses into the surrounding substrate dominate the evolution. Furthermore, in a periodic array of precipitates, there is necessarily diusional interaction among the spots. In this context it is interesting to explore, if the spots rst coalesce into single NCs and
126 6 CHAPTER 6. COMBINATION OF K3DLMC AND RDE METHODS a) b) c) Figure 6.: K3DLMC simulation of FIB implantation for a periodic array of implantation spots. Figs. a) and b) refer to stages during implantation, whereas Fig. c) shows the microstructure during annealing. then, on a quite dierent time scale, start to ripen, or if interspot ripening dominates over intraspot ripening right from the beginning of impurity redistribution. In a preliminary simulation series of idealized FIB synthesis of NCs, the evolution of a 4 4 array of implantation spots has been studied. Using system dimensions of fcc unit cells, per spot N spot = 5 IAs have been deposited according to a Gaussian depth distribution with R p =37a fcc and R p =8a fcc. Two lateral distributions have been considered, each dened by a radial Gaussian with R r = 8 a fcc and R r = 2 a fcc, respectively (recently Sakaguchi et al. [24] reported a beam size of 58 nm for a Ga metal ion source operating at an ion energy of some tens of kev 5 ). In what follows, these radial distributions are referred to as 'high' and 'low' focused implantations. Fig. 6. shows snapshots during and at the end of the simulation procedure of implantation in the case of the highfocused system at fcc = 3 using periodic BCs in lateral directions. The corresponding cluster distribution obtained after 8 5 MCSs for fcc =2canbe seen in Fig. 6.c. Once a characteristic NC distribution has been developed the computational eciency of the RDE approach with respect to OR can be used to model the further evolution of the samples. Figs. 6.2 and 6.3 show simulation results of the late stage evolution for the high and low focused systems, where in both cases material conservation was assumed. Although within one sample the implantation conditions were identical, the evolution for each spot seems to be governed by the statistical process of precipitation. While in some spots a large NC forms very early and thus mainly dominates intraspot OR, other spots are characterized by a few nearly equalsized NCs, which compete in coarsening. This can considerably slow down the intraspot redistribution and thus interspot OR becomes important. As can be clearly seen for the lowfocused sample (Fig. 6.3), the inuence of interspot coars 5 The eective radial impurity distribution within the substrate is given by the convolution of the beam prole and the radial straggling, which depends on the ion energy and the substrate composition.
127 6.3. FOCUSED ION BEAM SYNTHESIS OF NC ARRAYS 7 time  Figure 6.2: Evolution of the highfocused sample obtained by the RDE approach using K3DLMC input data. time  Figure 6.3: Evolution of the lowfocused sample obtained by the RDE approach using K3DLMC input data. ening can be so large, that spots disappear before the impurities within other spots have condensed to a single NC. A clear requirement for the formation of periodic arrays of dots is the absence of impurity losses, for instance evaporation through the surface or diusion into deeper parts of the substrate. For instance, in simulations assuming an absorbing interface at z = L z (not shown here), even in the highfocused sample NCs within certain spots completely dissolved before in other spots condensation into one single NC was achieved. The redistribution of IAs observed for annealing at low to moderate temperatures seems not to guarantee the condensation of the complete uence per spot into a single NC. Even in the highfocused example, where one NC per spot was temporarily obtained, there is a considerable dispersion in the size distribution due to diusional interaction between
128 8 CHAPTER 6. COMBINATION OF K3DLMC AND RDE METHODS a) b) c) Figure 6.4: K3DLMC simulation of rapid hightemperature annealing of a periodic array of implantation spots (the microstructure prior to annealing is similar to the one shown in Fig. 6.b). Here, N spot = 4 IAs per spot are initially annealed at fcc =. Increasing fcc every 5 4 MCSs about fcc =:25, Figs. a){c)show the evolution after 5 4 ( fcc = ), :5 5 ( fcc =:5), and 2:5 5 ( fcc = 2) MCSs, respectively. spots. The uncertainty in real experiments about the actually implanted uence per spot is supposed to increase this size dispersion even further. Although the spots are spaced regularly (an assumption, which can not expected to be met in experiments), the centers of mass of the remaining NCs do not coincide with the centers of the implantation spots. A more promising method seems to be rapid annealing to high temperatures followed by a controlled cooling as suggested by the simulation results of Fig Provided that material conservation holds within a thin lm of thickness s (e.g. ideally s 2R p ), the underlying idea is to tune the eective supersaturation in such a way, that only one large NC nucleates, onto which the impurities within the spot collapse. As a consequence of the high temperature needed for this method a considerable fraction (T ) of the N spot impurities will be found dissolved as monomers. Assuming a twodimensional spot density of n spot, the following equilibrium monomer concentration according to the GT relation [Eq. (2.23)] will be found ^c = N spot sn ; spot = c exp Rc R? R? = 3 4 ( ; )N spotv a =3 : (6.6) The NC size R? associated with ^c has to be larger than the critical size R? nuc(t ) for this temperature in order to prevent a complete dissolution. After the hightemperature anneal the subsequently applied cooling rate should be chosen such that secondary nucleation is hindered in the sample. This guarantees that essentially the whole fraction N spot of impurities diuses back to and condenses onto the central NC. According to Fig. 6.4 this methods supports the formation of a nearly monodisperse, highly periodic twodimensional array of precipitates.
129 Chapter 7 Application of the K3DLMC method to special topics in IBS Besides describing the evolution of a single implanted impurity species in a neutral matrix, the K3DLMC method can be applied to a variety of other systems. In this Chapter simulation results of the inuence of an oxidizing annealing atmosphere on the redistribution of impurities are shown [25]. Furthermore, the K3DLMC method is extended to include two types of interacting IAs in order to study various aspects of compound NC formation by IBS. 7. Inuence of the annealing atmosphere on the redistribution of impurities Nanocrystals of elemental semiconductors (Si, Ge, Sn) in SiO 2 are particularly interesting due to their electro and photoluminescence (see e.g. [22, 23, 26]) and their potential use for nonvolatile memory devices (see e.g. [27][29]). Besides various preparation methods based on thinlm deposition techniques (e.g. by chemical vapor deposition (CVD) [24] or by sputtering [22]), IBS of such NC/substrate systems is a promising option, because of its compatibility with standard microelectronics process technologies. The impurity redistribution and nanocrystal evolution can be strongly inuenced by the annealing ambient as has been reported for Ge implanted SiO 2 layers [22]. The origin of this behavior is indiusion of an oxidant from the annealing atmosphere, which changes substantially the Ge depth prole and NC distribution. In order to study systematically the inuence of the annealing ambient on the microstructure of Ge implanted SiO 2, samples have been annealed in N 2, Ar or dry O 2 atmospheres [25], which have dierent concentrations of chemical reactive components (H 2 O, O 2 ). 9
130 2 CHAPTER 7. APPLICATIONS OF THE K3DLMC METHOD IN IBS Ge concentration (at.%) asimplanted 4.5 a) T A = 95 C 4. b) T A = C Depth (nm) Ge concentration (at.%) asimplanted T A = 95 C T A = C Depth (nm) Figure 7.: Ge concentration proles obtained from RBS spectra (taken from Ref. [25]) of 5 nm thick SiO 2 layers on Si which were implanted with 35 kev Ge + and subsequently annealed in N 2 for one hour. (a) Fluence: :5 6 cm ;2,(b)Fluence: 5: 6 cm ; Experimental observations Experimental setup In a series of experiments aimed at studying the properties of ion beam synthesized semiconducting NCs in SiO 2, 35 kev Ge + ions have been implanted into 5 nm thick SiO 2 layers, which were thermally grown at Cbywet oxidation of [] oriented Si wafers. Implantations have been performed at "room temperature" (sample heating up to 9 C at current densities of 2 A/cm 2 ) in a uence range between 5 5 and 5 6 cm ;2, which results in peak concentrations of implanted Ge of.44 atomic percent. The annealing was performed at 95, and C in a standard furnace for 5 to 8 min using the "inert" gases of N 2, Ar or the "reactive" gas of dry O 2 (all of 5. purity). The Ge depth distribution in the SiO 2 layer after each annealing was measured by standard RBS (.7 MeV 4 He +, backscattering angle 7 ), while the precipitate structures were studied by XTEM. Annealing in "inert" gases N 2 or Ar In Fig. 7. RBS measurements of Ge depth distributions are shown. The asimplanted Ge proles are located inside the SiO 2 layer, i.e. the Ge concentrations at the surface and the SiO 2 /Si interface are below % of the peak concentration. For both uences the RBS analysis shows unusual changes in the Ge depth distributions after annealing at 95 Cin N 2. In general, three wellseparated peaks are found, whose separation from each other increases with increasing annealing temperature. The width and height of the central Ge peak decrease and the two satellite peaks grow. As it has been shown by STEMEDX analysis [7], the Ge at the SiO 2 /Si interface is located within a thin Si layer adjacent to the SiO 2 layer, where it forms a few monolayers of a SiGe alloy. In the asimplanted samples no Ge clusters could be detected by TEM as evidenced by Fig. 7.2a. However, after annealing (see Figs. 7.2bc), in the center of the SiO 2 layer Ge
131 7.. IMPURITY REDISTRIBUTION IN A REACTIVE AMBIENT 2 Figure 7.2: XTEM micrographs (taken from Ref. [25]) of 5 nm thick SiO 2 layers on Si implanted with Ge (uence 5: 6 cm ;2 at 35 kev) prior to annealing (a) as well as after annealing for one hour at 95 C (b) and C (c). NCs appear which are related to the central peak in the RBS spectrum (see Fig. 7.b). For the Ge NC distribution of Fig. 7.2c, a mean cluster size of 6 nm is observed, whichis in good agreement with the mean cluster size of 6:4 :7 nm measured by Xray diraction (XRD) [22]. Towards the SiO 2 surface, the Ge cluster band is terminated by avery narrow ( nm) edge region, which is in contrast to the smooth tail of NCs facing the Si substrate. Surprisingly no Ge clusters were found between the sharp edge of the cluster band and the SiO 2 surface, where a pronounced subsurface peak of Ge was observed by RBS (see Fig. 7.). Xray photoemission spectroscopy (XPS) measurements [25] reveal that Ge 2p 3=2 photoelectrons coming from the central, clusterrelated peak and from the interface peak can be attributed to a large extent to Ge{Ge and Ge{Si bonds respectively, whereas the energy of photoelectrons from the subsurface peak is shifted indicating Ge{O bonds. The Ge redistribution and NC evolution of identically implanted but Ar annealed SiO 2 layers are quite similar to the samples annealed in N 2. However, the Ge redistribution can be largely suppressed by the deposition of a 2 nm thick lm of Si 3 N 4 on top of the SiO 2 layer before implantation. Annealing in dry O 2 In order to study systematically the inuence of an reactive ambient, annealing of 5: 6 cm ;2 Ge implanted 5 nm thick SiO 2 layers has been also carried out in dry oxygen at 95
132 22 CHAPTER 7. APPLICATIONS OF THE K3DLMC METHOD IN IBS C. After annealing for 5 min the general features of the NC depth and size distribution appear to be similar to samples annealed in N 2 or in Ar. In particular, elemental Ge nanocrystals form in the center of the prole and the RBS spectrum shows a subsurface peak of Ge in a region where no nanocrystals can be seen by XTEM. At longer annealing times (3 and 45 min) the sharp edge of the cluster band of elemental Ge shifts progressively into the depth of the layer. In contrast to annealing in N 2 or Ar, on the rearside of the moving sharp edge of the Ge NC band a layer of diuse precipitates is observed. Since (i) in TEM micrographs these NCs exhibit a weaker Zcontrast than elemental Ge nanocrystals and (ii) under highresolution conditions no lattice planes could be found, they are assumed to be oxidized (disordered or glassy) Ge clusters. After annealing for 9 min the elemental Ge clusters disappeared completely, and a region of GeO 2 precipitates remains. Discussion The following model for the Ge redistribution and NC evolution is proposed: The Ge + ion implantation forms a highly supersaturated solid solution of Ge in SiO 2. At the initial stage of annealing most of the Ge nucleates to tiny Ge NCs, whereas a small fraction of Ge remains dissolved in SiO 2 (inserting the mean radius R into the GT relation [Eq. (2.23)] yields a good measure of the average supersaturation, provided that the materials parameters entering the capillary length are known). During annealing an oxidant (e.g. moisture being present with an extremely low concentration in the annealing atmosphere) can diuse into SiO 2, where it oxidizes dissolved Ge. Assuming for both species comparable monomer uxes (i.e. D ox c ox D Ge c Ge ), the zone of GeO 2 formation should lie between the surface and the cluster band. This explains immediately two features of the experiments. (i) As the oxidant reacts with Ge dissolved in SiO 2, the resulting GeO 2 does not form clusters, rather it is transformed to become part of the glassy SiO 2 matrix. Thus, the Ge accumulated there as GeO 2 can be seen as a peak in the RBS spectra, however not as clusters in XTEM images. (ii) The small distance between the sink (the zone of GeO 2 formation) and the source (the layer of Ge clusters) of Ge monomers leads to a steep gradient of dissolved Ge. Therefore, an eective dissolution of clusters occurs only within a narrow layer of the cluster band whose width is in the order of the diusional screening length D [see Eq. (3.8)]. Estimating the mean cluster radius R from Fig. 7.2 and calculating the corresponding cluster density n according to the implanted uence, the diusional screening length can be calculated to be D nm. This value is in excellent agreement with the width of the edge of the NC band (see Fig. 7.2). The disappearance of the drastic Ge redistribution during annealing in samples protected by a diusion barrier (Si 3 N 4 capping layer) underlines the strong inuence of tiny oxidant concentrations in the annealing ambient. An interaction of N 2 of the annealing ambient with the Ge implanted into the SiO 2 layer can be ruled out as annealing in an inert Ar atmosphere results in a similar Ge redistribution. Thus, it can be concluded that the few ppm of oxidizing impurities in the highpurity annealing gases N 2 and Ar cause the strong impact on the Ge prole in SiO 2. The main impurity in these gases is moisture
133 7.. IMPURITY REDISTRIBUTION IN A REACTIVE AMBIENT 23 a) b) Figure 7.3: Using a twodimensional scheme in a) the impurity() and oxidant() diusion on both fcc sublattices are shown. An oxidation event can be seen in b), which occurs upon a nearestneighbor encounter (r = j~r IA ; ~r ox j = a fcc =2) of IA and oxidant. (H 2 O), which dissolves and diuses readily in SiO 2 [22]. In comparison to annealing in N 2 or Ar, annealing in dry O 2 increases the surface concentration of the oxidant by orders of magnitudes which overcompensates the smaller diusivity ofo 2 compared to H 2 O[22]. Thus, the zone of GeO 2 formation shifts towards the edge of the NC band. Finally, the arriving oxidant cannot be consumed completely by dissolving Ge which results in direct oxidation of Ge nanocrystals. At the SiO 2 /Si interface the concentration c of Ge dissolved in SiO 2 is lower than c because the Ge{Si bond strength is more than % larger than the Ge{Ge bond strength [222]. In the NC region c is higher than c due to the convex interface curvature. The resulting concentration gradient leads to a diusion ux and to an accumulation of Ge at the interface. There, Ge can either grow epitaxially on top of the Si substrate, or, for suciently high annealing temperatures, it can diuse into the Si substrate Modeling of redistribution of implanted Ge in the presence of an oxidizing atmosphere Modications of the K3DLMC method Modeling the evolution of implanted impurities in a reactive ambient requires the introduction of a second atomic species into the K3DLMC program. Dening the IAs on a fcc lattice, the second fcc lattice [shifted by (=2 )a fcc ] of the bitarray not used so far is taken to accommodate the oxidant (see Fig. 7.3a) without the need to change the ecient bit encoding procedures. For this application, the evolution of the IAs (here Ge in the following referred to as species X) is determined by their solubility [established by the bond strength J XX see Eq. (3.4)) and diusion coecient (the activation energy EA X ). For simplicity, the oxidant (species Y ) is not allowed to cluster, i.e. J YY =. In this model, an oxidation event occurs upon a nearestneighbor encounter of both impurity species (see Fig. 7.3b), which is a simple estimate of the capture radius entering the recombination term of a corresponding rateequation description. By assuming an innite bond strength between IA and oxidant (J XY!) the reverse reaction (reduction of an
134 24 CHAPTER 7. APPLICATIONS OF THE K3DLMC METHOD IN IBS oxidized impurity) is suppressed. The oxidation site is recorded, and the reaction partners removed from the list of active atoms. Therefore, the oxidized impurities are not allowed to perform further diusion or reactions. For the simulations to be presented below it is assumed, that the use of an absorbing BC at z = z SiO2 /Si opposite to the surface describes the physics at the SiO 2 /Si interface. This approach lowers the impurity concentration (c = rather than c = ~c due to the evolving SiGe alloy) at the interface, but is not supposed to distort the impurity evolution considerably. Thus in the course of the simulation the evolving decoration of the SiO 2 /Si interface with Ge is approximated by counting the number of IAs diusing across the interface (and recording the site of the crossing). The frequency of diusional jumps of IAs (Ge) and the oxidant is according to their (assumed) diusion coecients D Ge and D ox. In each single diusion step for an IA (an oxidant), the sc neighborhood of the nal site is checked for the presence of an oxidant (an IA). K3DLMC simulations In order to obtain a qualitative understanding of the observed impurity redistribution, the evolution of an asimplanted prole was studied. Having in mind that Ge nanocrystals have diamond structure, the length scale a fcc is gauged according to the Ge density ( Ge =5:32 g/cm 3 ) a fcc =:45 nm). Rather than seeking on the atomic scale an exact geometrical matching of the simulation box with the experiment (for this problem a computationally favored simulation volume of fcc unit cells does not pose any signicantproblem on computer memory but requires a very powerful CPU in order to achieve diusional transport) a model system of dimension fcc unit cells was studied. Using a uence of F 5 a ;2 fcc the initial sample was characterized by a Gaussian distribution with R p =27a fcc and R p =4a fcc, and its evolution was followed at fcc =:8 for 6 MCSs. (In order to match the annealing at, say, C, this would correspond to an activation energy for solution of E S :8 ev (see Section 3.5.3). However, since no reliable data of solubility properties of Ge in SiO 2 have been available, the simulation has to remain qualitative innature.) A snapshot of the corresponding microstructure obtained after 6 MCSs can be seen in Fig. 7.4a. For this simulation the oxidizing species were continuously deposited by keeping their concentration xed in the surface layer (c ox j z= = :4 a ;3 fcc ) and assuming a ratio of the diusion coecients D ox =D Ge = :5. While close to the surface the oxidized Ge accumulates, in the center of the deposited prole NCs have been formed. The interface decoration at z = z SiO2 /Si marks the impurityow out of the system, whichapproximately corresponds to the evolving SiGe alloy. The driving forces of the impurity redistribution can be seen in Fig. 7.4b, which shows the respective monomer concentration proles after : 5 MCSs. Since both the In a more advanced treatment one would set up a thin bulk layer of a third atom type Z (Si) at z = z SiO2 /Si additionally to the implanted impurities of type X (Ge) and use appropriate bond strengths fj XX J XZ J ZZ g in order to describe the SiGe alloy.
135 7.. IMPURITY REDISTRIBUTION IN A REACTIVE AMBIENT 25 a) b) c) 3E4 (a ;3 fcc ) concentration 2E4 E4 c Ge c ox =2 / c ox c Ge (a ;3 fcc ) concentration asimplanted GeO Ge 5 5 z (a fcc ) z (a fcc ) 2 25 Figure 7.4: In a) the microstructure decomposed into oxidized Ge, Ge NCs and the interface decoration is displayed after a simulation period of : 5 MCSs. In b) the corresponding impurity monomer concentration c Ge (averaged over the last 4 MCSs) and the prole of the indiusing oxidant are plotted indicating the reaction zone. In c) the (smoothed) impurity prole as obtained after 6 MCSs is shown (the interface decoration has been articially broadened). SiO 2 /Si interface and the subsurface oxidizing region are sinks for dissolved Ge atoms, steep concentration gradients at both tails of the NC region reect the resulting impurity ow. However, due to diusional screening only the NCs in the very tails of the prole are subjected to the driving forces, whereas around R p undisturbed coarsening is observed (see also Fig. 6.9). The total Ge prole of the K3DLMC simulation (see Fig. 7.4c) is in excellent qualitative agreement with the RBS spectrum (see Fig. 7.). In particular, the concomitant formation of a subsurface peak of oxidized Ge, coarsening of NCs, and the evolving interface decoration have been observed. Furthermore, the steepening of the Ge prole towards the oxidizing zone is reproduced. However, also certain dierences to the experiment should be mentioned. For instance, both tails of the simulated NC region appear to be similar, i.e. the K3DLMC simulation of Fig. 7.4 does not show a sharp edge of the cluster band towards the surface. Additional to these simulations featuring the qualitative understanding of the observed Ge redistribution, more quantitative simulations are needed to understand the inuence of
136 26 CHAPTER 7. APPLICATIONS OF THE K3DLMC METHOD IN IBS the level of oxidant concentration at the surface (related to the partial pressure of oxidant in the atmosphere) and to estimate the ratio of impurity and oxidant diusion coecients. Also the role of hydrogen supposed to be set free upon Ge oxidation (i.e. H x O + Ge GeO+H x ) and its further inuence on the system remains to be explored (upon otherwise identical conditions a Si 3 N 4 capping layer not only suppresses the formation of a subsurface region of GeO 2, but also, surprisingly, modies the amount of Ge transferred to the SiO 2 /Si interface [25]). As a summary it is found that in Ge implanted SiO 2 layers the kinetics of Ge redistribution and NC evolution depends strongly on the annealing ambient. Atmospheres having oxidant (moisture) concentrations as low as a few ppm can cause a sequence of complex processes of diusion and chemical reactions. Due to the low concentration of the moisture, the oxidant reacts with dissolved Ge monomers only (not with Ge clusters) in a zone between the surface and the cluster band and forms GeO 2 which is built homogeneously into the glassy SiO 2 network. Annealing in dry O 2 increases the surface concentration of the oxidant by orders of magnitudes which shifts the reaction zone into the band of Ge NCs, i.e. noncrystalline GeO 2 clusters are formed. The accumulation of Ge at the SiO 2 /Si interface is due to the lower solubility at a at interface and the relatively strong Ge{Si bonds. 7.2 Ion beam synthesis of compound nanoclusters As already mentioned in the introduction, a large class of compound NCs has been synthesized in various substrate types by co and sequential implantation of two or more species of IAs. In order to apply the K3DLMC method for multicomponent systems, it has to be modied appropriately. Rather than applying the qstate Potts model [52] with spin variables q in order to have the necessary degrees of freedom to dene the occupation state of a lattice site, 2 two spatially identical llattices are used, which aremutually occupied by either X or Y species. While the ecient bit encoding of the singlecomponent lattice gas can still be used, the computational eort for each jump attempt now more than doubles, because the nearestneighbor sites of the jump conguration have to be checked in both the X and Y lattices. Whereas a restriction to the fcc and bcc lattices would have allowed to dene the second species on a free sublattice, the above choice was motivated by the wish to have a common implementation for all three lattice types K3DLMC model for two types of interacting IAs The decomposition of supersaturated multicomponent solid solutions can be described in terms of classical nucleation theory [223][225]. Restricting the current study to two types X, Y of IAs and assuming like in Section that NC growth and shrinkage proceeds by 2 In a q =Potts model the occupation states C i = ;, C i =, and C i = can be used to represent a X particle, a vacancy, or a Y particle, respectively.
137 7.2. ION BEAM SYNTHESIS OF COMPOUND NANOCLUSTERS 27 bimolecular steps only, the suitable extension of Eq. (2.) X i Y = 2X j= The rate factors are now given by [I(i j ) ; I(i j + )] j 2fX Y g: (7.) I(i j )=k + (i j ; i l )U(i j ; i l t) ; k ; (i j i l )U(i j i l t) j l 2fX Y g: (7.2) The attachment and detachment coecients k (i X i Y ) are in general complicated functions of the local impurity concentrations as well as of NC composition. Like in Chapter 3 a modeling approach is sought within the eective particle picture rather than via the determination of the coecients k (i j i l ). Assuming that the substrate is chemically inert with respect to both types of IAs, the complex interactions between an IA and the atoms of the host matrix as well as with other IAs of the same and/or of dierent kind are expressed in a set of eective nearestneighbor bond strengths fj XX l J XY l J YY l g. For instance, the energetics of an IA of type X is given by the sum nj XX l + mj XY l over all nearestneighbor interactions, where n and m are the corresponding numbers of alike or dierent bonds. The diusion of monomers of types X or Y is determined by their individual activation energies EA X and EA Y, respectively, for a single diusional jump. Using the Metropolis algorithm [8] for the jump kinetics, the transition probability Wif X for atoms of type X to jump from the initial site i to the nal site f is W X if =( X ) ; exp ; ; " X + E X A " X =(n i ; n f )J XX l +(m i ; m f )J XY l : (7.3) The jump probability reduces to Wif X =( X ) ; exp ;EA X in all cases for which "X. For simplicity, the (constant) rates of jump attempts f( X ) ; ( Y ) ; g are assumed not to depend on the particular chemical neighborhood. The corresponding singlecomponent impuritysubstrate systems can be used to determine the activation energies E A and the bond strength J l via proper adjustments to measured diusion coecients and solubilities. The mixed bond strength Jl XY can then be derived from tabulated values of chemical bond strengths (see e.g. [222]). The ratio of the numbers of MCSs of both subsystems is proportional to the ratio of the diusion coecients. Since in this K3DLMC model both impurity types are dened on the same lattice, eects of a possible lattice mismatch between the pure X and Y phases can not be taken into account. The length scale of the twocomponent K3DLMC model is dened by the lattice constant a l of the bulk phase of the compound system. Three major regimes of NC systems can be dened if the nearestneighbor bond strengths obey specic relations: for Jl XY Jl XX Jl YY there is essentially no interaction between the two kinds of IAs. In this case, two virtually independent subsystems of NCs will evolve for Jl XY Jl XX Jl YY the formation of an ordered compound phase is highly favored. Hence, fairly stoichiometric NCs are expected to evolve in cases of equal uences and sucient overlap of both implantation proles
138 28 CHAPTER 7. APPLICATIONS OF THE K3DLMC METHOD IN IBS for J XY l J XX l J YY l mainly kinetic reasons and the local concentration of both impurity components determine the cluster (alloy) formation and composition On core/shell NC formation by sequential ion implantation Background Core/shell NCs [a NC of composition A (the core) is coated by a few nanometer thick lm of composition B (the shell)] 3 represent aninteresting nanocrystalline state of matter. For instance, if both materials (A and B) are semiconductors and the shell has a slightly larger energy band gap than the core, then a very interesting behavior with respect to excitons is observed. In this case, the hole is conned to the core, whereas the electron is delocalized throughout the entire structure [33]. This property considerably reduces nonradiative transitions and thus very high luminescence eciencies have been measured [226]. These unique luminescence properties have made them very interesting in detecting and analyzing biological processes [227, 228]. Avariety of IIIV semiconducting core/shell nanocrystals has been synthesized by means of colloidal chemistry, e.g. CdSe/CdS [33] or CdSe/ZnS [228]. So far there have been no direct attempts to synthesize core/shell nanocrystals in an inert matrix by IBS via the scheme of coating the previously formed NCs by subsequently implanted impurities. However, Hosono [229] has found Cu NCs coated by a CuO layer embedded in SiO 2 for an implantation sequence of Cu + followed by F + ions, but not vice versa. In this case ballistic and chemical eects are used to explain the core/shell formation. Very recently, Cattaruzza et al. [23] reported Ag/Ag 2 S core/shell NCs in silica for sequential implantation of rst Ag + and then S + ions. Additionally, Meldrum et al. [23] found evidence for voids within CdS precipitates in silica formed by IBS, which represent a special core/shell structure. It is worth noting that in most publications about co or sequential implantation aimed at the formation of compound NCs, the compound phase is detected by Xray diraction measurements. However, this type of analysis provides averaged information for a large ensemble of NCs with possibly diering nanocomposition but is not suited to detect core/shell NCs. Neglecting lattice distortions at the core/shell interface, these nanostructures would be analyzed as two elemental phases. Only analyzing methods sensitive to single NCs like highresolution TEM, electron energy loss spectroscopy (EELS) or EDX can reveal information of their spatial structure and composition. K3DLMC simulations In the case of a sequential implantation of two ion species, some light should be shed on how nucleation, CM and coarsening aects core/shell NC formation. In a series of preliminary simulations the evolution of a Xtype NC is studied in presence of a source of Y monomers. 3 Both A and B can be mono or multicomponent materials.
139 7.2. ION BEAM SYNTHESIS OF COMPOUND NANOCLUSTERS 29 a) b) c) d) b ) c ) d ) Figure 7.5: Sequence of snapshots from K3DLMC simulations of core/shell NC formation. Fig. a) shows the Xtype "core" NC. The microstructure of the compound NC after the deposition of N Y = 2N X impurities is shown in the cases of b) no mixing, c) low intensity and d) high intensity of mixing. In b ){d ) corresponding cuts through the NCs (perpendicular to the plane of view) are shown. For this purpose the initial setup is a quasiequilibrated NC consisting of atoms of type X in a simulation box with periodic BCs (see Fig. 7.5a). However, ion implantation of Y atoms causes CM (see Section 5.3), which can hinder pure core/shell formation. For this study the following (arbitrarily chosen) ratios of bond
140 3 CHAPTER 7. APPLICATIONS OF THE K3DLMC METHOD IN IBS.8 no CM low CM high CM NC F Y =F Y Figure 7.6: Evolution of the mean square radial X and Y distributions during the deposition of the Y component plotted versus the fraction of the implanted total Y uence. In each of the three cases the upper curve shows the evolution of Y, whereas the lower one shows X. For comparison, in the case of no CM NC represents the homogeneous (X = Y ) NC. strength have been used: J XX l J XY l J YY l =Jl XY = 9=8 and Jl YY =Jl XY = 7=8 (the relation Jl XX > energetically stabilizes NCs having a Xtype core covered by a Y type shell against an internal, thermodynamically driven mixing). The Y deposition rate was kept low enough to prevent satellite nucleation in the case of no mixing. In order to allow for a reasonable coating of the preexisting core N Y = 2N X was chosen. The evolution of this model system has been studied in the case of no CM during deposition of the Y component and for two dierent intensities of CM corresponding to :9 displacements per atom (dpa) of X impurities and 2 dpa, respectively, recorded during the period of deposition of Y atoms. Results and Discussion The spatial inhomogeneity of the X and Y components within a core/shell NC can be analyzed with respect to the radial concentration proles. For this purpose, in an extension of Eq. (3.8), the normalized mean square distance of an impurity component from the center of mass of the NC can be used Z i = M i R 2 r 2 dm i i 2fX Y g: (7.4) The evolution of X and Y during "implantation" of species Y without and with CM can be seen in Fig Figs. 7.5b { 7.5d show the resulting microstructure of the compound NC if CM is neglected (b) and if two dierent degrees of CM are included (c,d). The corresponding cuts through the NC (Figs. 7.5b { 7.5d ) reveal more clearly the composition. Whereas in case (b) the chosen energetics and kinetics leads to a pure core/shell formation, the X and
141 7.2. ION BEAM SYNTHESIS OF COMPOUND NANOCLUSTERS 3 Figure 7.7: Largescale simulation of the evolution of a sequentially implanted two component system in the presence of CM. The snapshot shows the microstructure right at the end of the second implantation. Y replacements caused by CM lead to a random distribution of both components within the NC. As can be seen in Fig. 7.6 the more eective the mixing the more homogeneous is the resulting radial distribution of both components. Additionally, depending on the level of CM, the pronounced faceting (octahedrallike shape) of the NC tends to be smeared out. CM enhances also the impurity monomer concentration in the vicinity of a NC. These monomers can diuse back to the NC and reattach, but if this enhanced supersaturation exceeds a critical value, small satellite NCs may form, as is indicated in Fig. 7.5d. For high ion uxes j Y even the complete dissolution of preexisting NCs can be achieved. After the Y implantation a compound NC is characterized by a random XY composition due to the collisional displacements and the random attachment ofx or Y monomers. An isolated NC would then evolve to an energetically more favorable state by local XY rearrangements mediated most eectively by vacancy as well as by X or Y interstitial diusion within the NC or by direct XY site changes. Depending on the XY energetics an isolated NC would then tend either to an ordered or segregated composition, which in the latter case could be a core/shell structure. Obviously, CM competes with the coating of a X NC with Y impurities, which makes core/shell NCs unlikely to be found in asimplanted samples. Fig. 7.7 shows the typical microstructure after the implantation of the second component (F Y = 2F X ) into a substrate having a preimplanted ensemble of X"core" NCs for a reasonable overlap of the implantation proles (Rp X = 2 a fcc, Rp X = 32 a fcc, Rp Y = 35 a fcc, Rp Y = 4 a fcc ). Obviously, noreasonably coated Xtype NCs are observed. NCs formed by IBS interact with each other due to their size and space distribution (OR). Due to their metastability (GT relation) small NCs are continuously dissolving and there is always a certain degree of supersaturation of monomers, which mediate the diusional transport from the small to the large NCs. Generally the dynamics is governed by the diusion and solubility properties as well as the phase diagrams and the local concentration of both components. The evolution of the compound NCs, e.g. in a subsequent annealing step, depends then on the ratio of the time scales of ensemblelike (coarsening) and NClike (local ordering mechanisms) processes.
142 32 CHAPTER 7. APPLICATIONS OF THE K3DLMC METHOD IN IBS Since ion implantation is inevitably accompanied by a specic level of CM, for sequential implantation of twoiontypes there is a competition between a coating of the preimplanted NCs and a random arrangement of X and Y impurities. As a rule of thumb core/shell formation is favored if (i) the solubility ofy exceeds the solubility ofx in the matrix, i.e. Jl XX > Jl YY for reasonable Jl XY, if (ii) the atomic mass of Y is small, i.e. low CM, and (iii) for rather low ion ux j Y and/or high second implantation temperature, which favors a compensation of displacements by thermodynamically driven atomic movements Shiftedprole compound NC synthesis Compound NC formation by co and/or sequential implantation of two or more ion species is a highly complex process much less understood than the governing physics in the singlecomponent case. Restricting this study two types of impurities in a neutral matrix the evolution is governed by two diusion coecients and three solubilities (besides the compound phase also the singlecomponent phases have to be considered), not to mention the modications arising due to nontrivial interactions with point defects or other damage structures caused by the implantations. Essentially all experimental studies on IBS of compound NCs in chemically neutral substrates reported so far have been based on achieving a rather good overlap of both implantation proles. The spirit of these experiments was to demonstrate, that compound NCs can be synthesized by ion implantation [4, 5, 232, 233]. However, rather than presenting simulation results of the standard approach to compound NC formation, in this Section some preliminary predictions are given for implanted systems with only partly overlapping impurity proles. With the help of K3DLMC results of a few exemplifying model systems, the physics of impurity redistribution and compound NC formation in a homogeneous environment is qualitatively discussed. Figure 7.8: Compound NC of bcc structure consisting of roughly 4 IAs. Without referring to a specic materials system, simulations have been performed for two interacting types of IAs on a bcc lattice. Fig. 7.8 shows the typical microstructure of such a compound NC. In a series of simulations the evolution of an asimplanted sample corresponding to two shifted impurity proles (simulation volume bcc unit cells, absorbing interface at z = L z, uences of F X = F Y 2:4a ;2 bcc, Gaussian proles characterized by RX p = 75 a bcc, Rp X = 7:5 a bcc, Rp Y = 55 a bcc, Rp Y = 25 a bcc ) is studied. Within the K3DLMC model, the evolution depends on ve parameters, namely the two diusion coecients D X and D Y and the three bond strengths J XX l, J XY l, and J YY l. Table 7. lists the parameter relations for three model systems, which in the following serve to discuss the physics of compound NC formation in this approach. Fig. 7.9a shows the asimplanted initial sample, which in implantation experiments may be qualitatively achieved be suitably tuning the ion energies. In the left column of Fig.
143 7.2. ION BEAM SYNTHESIS OF COMPOUND NANOCLUSTERS a) DX = DY ; cxy cx; cy d) DX = DY ; 33 cxy cx; cy t b) e) t c) f) t3 Figure 7.9: For model system A compound NC synthesis is shown in the case of double (X; Y ) or triple (X; Y; X ) implantations with shifted proles. The further evolution of the initial states is shown at times t = 5 4 MCSs and t3 = :9 6 MCSs, respectively. 7.9 the evolution of model system A (equal di usion coe cients and an energetics strongly favoring compound NC formation) can be seen. Obviously, in this highly symmetric case, a band of NCs starts to form at the region of the overlap of the implantation proles. Assuming a physical system can be found (two species X and Y with approximately equal di usion coe cients, for which in an inert substrate the compound phase XY is favored due to the driving chemical forces), which tends to form a NC band in the overlapping region, a straightforward extension would be a triple implantation. Figs. 7.9df show such a model simulation, where the initial distributions are described by RpX = 5 abcc, RpX = 2:5 abcc, RpY = abcc, RpY = 2 abcc, RpX2 = 75 abcc, RpX2 = 3 abcc. The Table 7.: Parameter relations for three exemplifying model systems of compound NC formation. XY YY Y X system XX bcc bcc bcc D =D A 3 B C
144 34 CHAPTER 7. APPLICATIONS OF THE K3DLMC METHOD IN IBS a) b) system B DX = DY ; cxy < cy < cx ; ; t e) R DX = DY ; system C cxy < cy < cx t c) f) t2 d) g) t3 Figure 7.: In the top row, the initial sample can be seen (asimplanted state). The further evolution for the model systems B and C is shown at times (given for the X component) t = 5 4 MCSs, t2 = 2:5 5 MCSs, and t3 = :9 6 MCSs, respectively. deposited uences F X :3 a;bcc2, F X2 :6 a;bcc2, and F Y 2:4 a;bcc2 have been chosen such as to have an excess amount of X impurities on order to compensate for the absorbing interface at z = Lz. Here, two planar NC layers should evolve, whose distance is given as a function of the respective implantation energies, and can thus be changed by a proper choice of implantation parameters. In the case of model system B the in uence of the solubilities can be seen in Fig. 7.. Here, additional to the compound NC formation, due to the nite solubilities cx and cy singlecomponent NCs of both species start to form. In the course of the simulation, the NCs with the highest solubilities (i.e. the lowest bond strength J ) start to dissolve, since concentration gradients to spatial regions with lower solubility will build up. The impurity redistribution can be monitored with the help of the monomer concentration proles. Fig. 7.a shows the corresponding depthdependence of cx and cy. Clearly, the region of compound NC formation acts as sink for both types of impurities. Furthermore, the di erence in the singlecomponent solubilities is re ected in the respective monomer concentration levels.
145 c (=a 3 bcc ) c (=a 3 bcc ) 7.2. ION BEAM SYNTHESIS OF COMPOUND NANOCLUSTERS 35 a) 2E4 b) 2E4 8E4 4E4 c X c Y 8E4 4E4 c X c Y 5 5 z (a bcc ) z (a bcc ) 2 25 Figure 7.: Monomer concentrations averaged over the last 4 MCSs as recorded at times (from top to bottom) t, t 2, and t 3 of Fig. 7. (on this scale c Y essentially vanishes for late times). Figs. a) and b) correspond to systems B and C, respectively. The evolution of both singlecomponent NC subsystems can be understood with the help of the time scale of OR di, which is proportional to =(DR c c ) [Eq. (4.6)]. Assuming, that as in the case of the fcc lattice the capillary length is given by R c = R (bcc) c + bcc a bcc bcc bcc a bcc bcc (see Section omitting the term R (bcc) c should be a reasonable approximation in the current parameter range), the following relation can be derived X di Y di DY J YY Y D X expf;4(y J XX bcc ; XX bcc )g: (7.5) Besides characterizing OR, di furthermore gives a measure of the time a system of NC needs to interact with an external disturbance, for instance a nearby region with a different solubility. Accordingly, a small value of di (i.e. a large product Dc ) implies an ecient impurity redistribution by diusional mass transport. For system B (equal diusion coecients, but considerable solubility dierence), the evolving asymmetry of the NC distribution with respect to the overlapping region is thus simply a consequence of the relation di X :7 di Y. A more general situation is represented by model system C, whose evolution can be seen in the left column of Fig. 7.. Here, in addition to diering solubilities, the diusion coecients dier by one order of magnitude. The time constants are, however, similar, i.e. di X :7 di Y. Thus both singlecomponent subsystems show similar response to the eective sink created by the small region of compound NC formation. This explains, why the formation of a pronounced NC band in the overlapping region is very similar to model system A (see Fig. 7.9), for which di X = di Y trivially holds. Furthermore, it is instructive to analyze the NC evolution on the basis of the numbers and compositions of the nearestneighbor bonds [see Eq. (7.3)]. As can be seen in Fig. 7.2 the fraction of compound bulk IAs (n + m = 8)increases for both impurity components,
146 N Y =N Y tot N Y =N Y tot N Y =N Y tot N X =N X tot N X =N X tot N X =N X tot 36 CHAPTER 7. APPLICATIONS OF THE K3DLMC METHOD IN IBS a) b) c) t = :2 t = t = :2 t = t = :2 t = n + m n m d).6 e).6 f) t = :2 t = t = :2 t = t = :2 t = n + m n m Figure 7.2: Analysis of number and type of nearestneighbor bonds during the evolution of system B (times are given in units of 6 MCSs, see Fig. 7.). For the Xtype IAs the normalized histograms in the top row show the complete neighborhood (n + m), and the distributions of X{X (n) and X{Y (m) bonds, respectively. The corresponding analysis for the Y type IAs is shown in the bottom row. whereas the fraction of singlecomponent bulk atoms (n = 8) decreases. The formation of the energetically favored compound phase is also reected in the increasing number of atoms having m = 8nearestneighbor bonds to the other impurity component. It is interesting to note, that in model system B a large fraction of Y atoms is in a bulk state (n + m = 8), whereas a signicant fraction of X atoms can be found to be part of the surface of the compound NCs (see peak at n + m = 4 in Fig. 7.2a). The eect of the ow of Xtype atoms into the region of the Y prole can be interpreted as a tendency of core/shell NC formation. This can be understood as follows: The evolving predominantly Y type NCs within the Y prole close to the overlapping region represent a diusion barrier for Xtype monomers (the mean undisturbed penetration depth can be estimated with the help of the diusional screening length). Thus the rst arriving Xtype monomers will be able to form energetically most favored X{Y bonds by condensing on these predominantly Y type NCs. Later on, subsequently arriving monomers nd essentially Xtype coated NCs. Although these NCs still act as monomer traps, the detachment rate is accordingly higher (note, that these lately arriving monomers have basically formed only X{X bonds), and hence they may readily diuse further into the Y region. The above introduced method of shiftedprole compound NC synthesis should in prin
147 7.2. ION BEAM SYNTHESIS OF COMPOUND NANOCLUSTERS 37 ciple work also for an interchange in the ion types (i.e. X $ Y ). While it is clear, that due to the massdependent straggling the proles can not simply be reversed, at least qualitatively the same impurity redistributions should occur after achieving a mirror image with respect to the overlapping region of the asimplanted proles. Obviously, the presented results rely on homogeneous conditions throughout the simulation volume. However, radiation damage can signicantly alter the redistribution e.g. by inhomogeneous nucleation. Therefore, it would be very interesting to conduct corresponding shiftedprole implantation experiments in order to explore the predictability of the K3DLMC results.
148 38 CHAPTER 7. APPLICATIONS OF THE K3DLMC METHOD IN IBS
149 Chapter 8 Summary and outlook In this work various aspects of the ion beam synthesis of nanostructures, in particular nanoclusters, have been studied by atomic and mesoscopic computer simulation methods. Nucleation of precipitates out of (in general depthdependent) supersaturated solid solutions, their subsequent growth and the early stages of coarsening phenomena have been studied using a kinetic threedimensional lattice MonteCarlo method based on the nearestneighbor Ising model (also known as lattice gas model). For all simulations the impurity atoms have been regarded as eective particles dened in an inert and homogeneous matrix (i.e. no depthdependent inhomogeneities due to irradiation damage have been considered). The late stage of phase separation of isolated secondphase domains, i.e. Ostwald ripening, is modeled by a mesoscopic approach. This has been done by the stepwise numerical integration of the reactiondiusion equations of coarsening nanoclusters formulated in the framework of a local meaneld theory. The rst purpose was to give a solid foundation of the intrinsic properties of the K3DLMC model with respect to the governing physics of nanocluster evolution. For the three major lattices implemented (fcc, bcc, and sc lattices, respectively), Arrheniuslike laws for the solubility have been derived, which allows a coupling to thermodynamic data. Furthermore, the GibbsThomson relation, which by establishing the curvaturedependence of the equilibrium monomer concentration denes the dynamical properties of coarsening systems, has been proven to be valid down to nanocluster sizes of a few tens of atoms, i.e. on a nanometer scale. Based on the GibbsThomson relation an explicit expression for the surface tension has been derived in the temperature range well below the roughening transition. An existing computer model for diusion limited Ostwald ripening has been extended to be applicable for an arbitrary degree of diusion and reaction control. Based on the approximation of a radiusindependent interface reaction rate, it has been shown that the mesoscopic method successfully reproduces the basic results of the LSW theory in the two limiting cases. For the intermediate parameter regime, the simulation results of Ostwald ripening have been compared to an alternative description and the observed dierences have been discussed. In the case of nanocluster formation during implantation (typical for highdose metal 39
150 4 CHAPTER 8. SUMMARY AND OUTLOOK implantations into insulators) the basic dependence of the size distribution on substrate temperature and ion current has been studied. A comparison of K3DLMC simulation results with experiments (MeV Au + implantation into SiO 2 for varying temperatures) has been presented. A good qualitative correspondence has been observed even though ballistic eects have not been taken into account in this particular study. Additional MonteCarlo simulations predict that a controlled variation of the implantation conditions (decreasing the implantation temperature or increasing the ion current) can initiate a second nucleation regime, thus leading to a bimodal size distribution. Corresponding Au + implantations into SiO 2 are discussed with respect to these predictions. On the basis of an isotropic collisional mixing model, temperatureindependent ballistic jumps of impurity atoms have been added to the K3DLMC method, which aretypical for irradiation eects. In particular, the modications of the GibbsThomson relation in the presence of collisional mixing have been studied. The simulation results indicate, that irradiationinduced modications of nanocluster properties cannot merely be explained by the concept of an eectively higher temperature. As predicted recently it has been shown, that collisional mixing (i) increases the solubility and (ii) causes a decrease of the eective capillary length, which can even result in negative values for specic parameter regimes. Based on these observations, K3DLMC simulations show the predicted modications of Ostwald ripening under irradiation, especially inverse coarsening (i.e. the growth of small nanoclusters on the expense of large one). It is demonstrated, that inverse Ostwald ripening leads to a deltalike size distribution. Furthermore, for very high mixing intensities or low diusivities, the nucleation of additional precipitates is predicted, which in combination with inverse Ostwald ripening causes a decrease of the mean nanocluster size. The atomic and mesoscopic computer simulation methods have been combined to perform a multiprocess and multiscale modeling of the evolution of nanoclusters. It has been found, that the ratio of the mean nanocluster radius to the capillary length determines the dynamics of phase separation. For equivalent dynamical descriptions the dierences in the evolution of an nanocluster ensemble have been shown to be due to the stochastic and deterministic characters of the atomic and mesoscopic methods, respectively. As an application the competition of internal Ostwald ripening and boundaryinduced selforganization has been investigated with respect to the evolution of asimplanted samples. Furthermore, simulation results regarding the synthesis of periodic twodimensional arrays of nanoclusters by focused ion implantation are presented, where the competition between intraspot and interspot Ostwald ripening has been discussed. It is predicted that for the formation of nanocluster arrays hightemperature rapid thermal annealing followed by awellcontrolled coolingdown stage is superior to conventional annealing techniques. Extending the K3DLMC method to two types of interacting species, various specic phenomena encountered in ion beam synthesis have been modeled. For instance, the redistribution of implanted impurities has been studied taking into account the inuence of a reactive annealing atmosphere. A comparison to experimental results of annealing of a Geimplanted SiO 2 layer in various ambients (N 2, Ar, or O 2 ) has been given. In the area of compound nanocluster synthesis by means of ion implantation, some aspects of perspectives
151 4 b) a) Figure 8.: K3DLMC modeling of ultralow energy Si implantation into a thin gate oxide on () silicon (the silicon structure is approximated by the fcc lattice). The simulated redistribution of implanted Si + (partly nucleating into nanoclusters and partly condensing onto the at Si layer) can be seen in Fig. a) as a crosssection view and in Fig. b) as a plane view (omitting here the Si substrate for clarity). on core/shell nanocluster formation by sequential ion implantation have been discussed. It has been shown that collisional mixing seems to be a major obstacle concerning ion beam synthesis of core/shell nanoclusters. Furthermore, predictions have been made concerning the formation of a narrow layer of compound nanoclusters by shiftedprole implantation of two ion species. As an atomic model describing eciently the evolution of impurities within a chemically neutral matrix, the K3DLMC method has the potential to enlarge our understanding of basic physical processes on length scales up to mesoscopic dimensions. Noting potential applications of this modeling approach also outside implantationspecic phenomena, two more interesting areas related to the ion beam synthesis of nanostructures should be briey mentioned. From the technological point of view a very promising option is ultralow energy implantation into thin gateoxides (thickness nm) in order to position nanoclusters within the tunneling length in the gate oxide of a transistor. From the modeling point of view, the implantation of Si + into a thin SiO 2 layer on Si [42] can be described consistently by considering only a single atom type (see Fig. 8.). In this process the formed nanoclusters are in a highly metastable state due to the close at Si interface. Thus an essentially twodimensional layer of Si nanoclusters will evolve, whose stability is expected to be very sensitive to the applied heat budget. Furthermore, aspects of buried layer formation can be addressed (see Fig. 8.2). While these simulation results are obtained starting with a (from the modeling point of view) simple initial conguration, the observed microstructures are very similar to experimental
Twodimensional turbulence: a physicist approach
Physics Reports 362 (2002) 1 62 Twodimensional turbulence: a physicist approach PatrickTabeling Laboratoire de Physique Statistique, Ecole Normale Superieure, 24 rue Lhomond, 75231 Paris, France Received
More informationSYNTHESIS AND PROPERTIES OF NEW SEMICONDUCTOR ALLOYS FOR LONG WAVELENGTH COHERENT EMITTERS ON GALLIUM ARSENIDE
UNIVERSITÀ DEGLI STUDI DI TRIESTE XVI CICLO DEL DOTTORATO DI RICERCA IN FISICA SYNTHESIS AND PROPERTIES OF NEW SEMICONDUCTOR ALLOYS FOR LONG WAVELENGTH COHERENT EMITTERS ON GALLIUM ARSENIDE DOTTORANDO
More informationNuclear Magnetic Resonance as a Tool for OnLine Catalytic Reaction Monitoring
Nuclear Magnetic Resonance as a Tool for OnLine Catalytic Reaction Monitoring Von der Fakultät für Mathematik, Informatik und Naturwissenschaften der RheinischWestfälischen Technischen Hochschule Aachen
More informationSpectroscopy of Discrete Breathers
Institut für Theoretische Physik Fakultät Mathematik und Naturwissenschaften Technische Universität Dresden Spectroscopy of Discrete Breathers Dissertation zur Erlangung des Doktorgrades der Naturwissenschaften
More informationAlN Thin Film Electroacoustic Devices
Comprehensive Summaries of Uppsala Dissertations from the Faculty of Science and Technology 817 AlN Thin Film Electroacoustic Devices BY GONZALO FUENTES IRIARTE ACTA UNIVERSITATIS UPSALIENSIS UPPSALA 2003
More informationProperties of Electrons, their Interactions with Matter and Applications in Electron Microscopy
Properties of Electrons, their Interactions with Matter and Applications in Electron Microscopy By Frank Krumeich Laboratory of Inorganic Chemistry, ETH Zurich, VladimirPrelogWeg 1, 8093 Zurich, Switzerland
More informationSingleElectron Devices and Their Applications
SingleElectron Devices and Their Applications KONSTANTIN K. LIKHAREV, MEMBER, IEEE Invited Paper The goal of this paper is to review in brief the basic physics of singleelectron devices, as well as their
More informationUNIVERSITA' DEGLI STUDI DI PADOVA
UNIVERSITA' DEGLI STUDI DI PADOVA Sede Amministrativa: Università degli Studi di Padova Dipartimento di Scienze MM.FF.NN. SCUOLA DI DOTTORATO DI RICERCA IN SCIENZA ED INGEGNERIA DEI MATERIALI XX CICLO
More informationColloidal Suspensions in Temperature Gradients with Mesoscopic Simulations
Colloidal Suspensions in Temperature Gradients with Mesoscopic Simulations I n a u g u r a l  D i s s e r t a t i o n zur Erlangung des Doktorgrades der MathematischNaturwissenschaftlichen Fakultät der
More informationRealistic Cellular Automaton Model for Synchronized TwoLane Traffic
Realistic Cellular Automaton Model for Synchronized TwoLane Traffic Simulation, Validation, and Applications Vom Fachbereich Physik der Universität DuisburgEssen zur Erlangung des akademischen Grades
More informationGeopolymer technology: the current state of the art
J Mater Sci (2007) 42:2917 2933 DOI 10.1007/s108530060637z ADVANCES IN GEOPOLYMER SCIENCE & TECHNOLOGY Geopolymer technology: the current state of the art P. Duxson Æ A. FernándezJiménez Æ J. L. Provis
More informationOnedimensional wave turbulence
Physics Reports 398 (4) 65 www.elsevier.com/locate/physrep Onedimensional wave turbulence Vladimir Zakharov a;b,frederic Dias c;, Andrei Pushkarev d a Landau Institute for Theoretical Physics, Moscow,
More informationTheir Scales with a ScaleSpace Primal Sketch: A Method for FocusofAttention. Tony Lindeberg
Detecting Salient BlobLike Image Structures and Their Scales with a ScaleSpace Primal Sketch: A Method for FocusofAttention Tony Lindeberg Computational Vision and Active Perception Laboratory (CVAP)
More informationQuantum Point Contacts
SEMICONDUCTORS AND SEMIMETALS VOL 35 CHAPTER 2 Quantum Point Contacts H. van Hauten and C. W. J. Beenakker PHILIPS RESEARCH LABORATORIES EINDHOVEN THE NETHERL \NDS B J. van Wees DEPARTMENT OE APPLIED PHYSICS
More informationReview of the Present Status of Rotor Aerodynamics
WIND ENERGY Wind Energ., 1, 46±69 (1998) Review Article Review of the Present Status of Rotor Aerodynamics H. Snel,* Netherlands Energy Research Foundation, Petten, The Netherlands Key words: aerodynamics;
More informationSimulation of Medical Irradiation and XRay Detector Signals
Simulation of Medical Irradiation and XRay Detector Signals Der Naturwissenschaftlichen Fakultät der FriedrichAlexanderUniversität ErlangenNürnberg zur Erlangung des Doktorgrades Dr. rer. nat. vorgelegt
More informationThe critical current of superconductors: an historical review
LOW TEMPERATURE PHYSICS VOLUME 27, NUMBER 9 10 SEPTEMBER OCTOBER 2001 The critical current of superconductors: an historical review D. DewHughes* Oxford University, Department of Engineering Science,
More informationWhy a Simple Herding Model May Generate the Stylized Facts of Daily Returns: Explanation and Estimation
Why a Simple Herding Model May Generate the Stylized Facts of Daily Returns: Explanation and Estimation Reiner Franke and Frank Westerhoff Working Paper No. 83 December 2011 0 b k* B A M B AMBERG E CONOMIC
More informationSimulation of Spin Models on Nvidia Graphics Cards using CUDA
Simulation of Spin Models on Nvidia Graphics Cards using CUDA D I P L O M A R B E I T zur Erlangung des akademischen Grades DiplomPhysiker (Dipl.Phys.) im Fach Physik eingereicht an der MathematischNaturwissenschaftlichen
More informationBreakdown of Local Thermodynamic Equilibrium...
II Stellar Atmospheres Copyright (2003) George W. Collins, II 15 Breakdown of Local Thermodynamic Equilibrium... Thus far we have made considerable use of the concepts of equilibrium. In the stellar interior,
More informationSelfAssembly of Block Copolymers in External Fields
SelfAssembly of Block Copolymers in External Fields DISSERTATION zur Erlangung des akademischen Grades eines Doktors der Naturwissenschaften (Dr. rer. nat.) im Fach Chemie der Fakultät für Biologie, Chemie
More informationElectrowetting: from basics to applications
INSTITUTE OF PHYSICSPUBLISHING J.Phys.: Condens. Matter 17 (2005) R705 R774 JOURNAL OFPHYSICS: CONDENSED MATTER doi:10.1088/09538984/17/28/r01 TOPICAL REVIEW Electrowetting: from basics to applications
More informationNonlinear physics (solitons, chaos, discrete breathers)
Nonlinear physics (solitons, chaos, discrete breathers) N. Theodorakopoulos Konstanz, June 2006 Contents Foreword vi 1 Background: Hamiltonian mechanics 1 1.1 Lagrangian formulation of dynamics.......................
More informationSupporting RealTime Applications in an Integrated Services Packet Network: Architecture and Mechanism
Supporting RealTime Applications in an Integrated Services Packet Network: Architecture and Mechanism David D. Clark 1 Laboratory for Computer Science Massachusetts Institute of Technology ddc@lcs.mit.edu
More informationMatter Waves. In the previous chapter we discussed some important discoveries and theoretical. Chapter Outline
5 Matter Waves Chapter Outline 5.1 The Pilot Waves of de Broglie De Broglie s Explanation of Quantization in the Bohr Model 5.2 The Davisson Germer Experiment The Electron Microscope 5.3 Wave Groups and
More informationThe Hamiltonian Mean Field Model: From Dynamics to Statistical Mechanics and Back
The Hamiltonian Mean Field Model: From Dynamics to Statistical Mechanics and Back Thierry Dauxois 1, Vito Latora 2, Andrea Rapisarda 2, Stefano Ruffo 1,3, and Alessandro Torcini 3,4 1 Laboratoire de Physique,
More informationCurrent Status of TransitionState Theory
J. Phys. Chem. 1996, 100, 1277112800 12771 Current Status of TransitionState Theory Donald G. Truhlar* Department of Chemistry and Supercomputer Institute, UniVersity of Minnesota, Minneapolis, Minnesota
More informationPatterning: Principles and Some New Developments**
Patterning: Principles and Some New Developments** By Matthias Geissler and Younan Xia* This article provides an overview of various patterning methodologies, and it is organized into three major sections:
More informationApplication of CFD in Membrane Technique
Application of CFD in Membrane Technique Der Fakultät für Ingenieurwissenschaften, Abteilung Maschinenbau der Universität DuisburgEssen zur Erlangung des akademischen Grades DOKTORINGENIEUR genehmigte
More informationCombustion control and sensors: a review
PERGAMON Progress in Energy and Combustion Science 28 (2002) 107±150 www.elsevier.com/locate/pecs Combustion control and sensors: a review Nicolas Docquier 1,SeÂbastien Candel* Laboratoire EM2C, Ecole
More information